1 UNIVERSIDAD DE CANTABRIA ESCUELA TÉCNICA SUPERIOR DE INGENIEROS INDUSTRIALES Y DE TELECOMUNICACIÓN DEPARTAMENTO DE INGENIERÍA QUÍMICA Y QUÍMICA INORGÁNICA Membrane technologies for hydrogen and carbon monoxide recovery from residual gas streams (Tecnologías de membranas para la recuperación de hidrógeno y monóxido de carbono de gases residuales) Memoria de Tesis Doctoral presentada para optar al título de Doctora por la Universidad de Cantabria. Programa de Doctorado en Ingeniería Química y de Procesos Directores de Tesis: Dra. Ane Miren Urtiaga Mendia Dr. Eugenio Daniel Gorri Cirella Oana Cristina David Santander, Mayo 2012
3 Agradecimientos Me gustaría expresar mi gratitud a mis directores de tesis, la Dra. Ane Miren Urtiaga y el Dr. Daniel Gorri, por la confianza el esfuerzo y tiempo dedicados para que este trabajo saliera adelante. Gracias por haberme dado la oportunidad de trabajar en el fascinante mundo de la investigación. También me gustaría agradecer a la responsable del grupo de investigación Procesos avanzados de separación, dentro de cual este trabajo ha sido llevado a cabo, a la Dra. Inmaculada Ortiz por su exigencia y profesionalidad que determinó la calidad de este trabajo. Gracias a la Dra. Kitty Nijmeijer por la oportunidad de trabajar en el grupo de investigación Membrane Science and Technology Group, University of Twente y a todo el personal de dicho departamento por la calurosa acogida y por dedicarme una buena parte de su tiempo en transferir sus conocimientos y experiencia en el campo de las membranas. I want to express my acknowledgments to Prof. Dr. Kitty Nijmeijer for giving me the opportunity to work in Membrane Science and Technology Group, University of Twente. I am also grateful to the people from this group for dedicating important part of their time in sharing their knowledge and experience in the membrane field Gracias a la Dra. Nazely Diban por animarme en los momentos difíciles y por ser un ejemplo a seguir de dedicación y trabajo. Gracias a Dra. Clara Casado por ayudarme en los primeros pasos en el campo de las membranas y de las instalaciones de gases. También quiero agradecer a todos los compañeros de trabajo, entre ellos a Alfredo, Marcos, Gabriel, Mariana, Marisol, Sonia, Hala, Vanesa, Elia, Karima, Bea, Esther, Antía el que hayan compartido estos años conmigo y haber recibido su atención. También quiero agradecer al personal de mantenimiento, Felix, Elena y Rafa y al personal administrativo, Inmaculada y Pilar. Quiero expresar mis agradecimientos a mis padres, mi hermana y mis abuelas por apoyarme incondicionalmente en todas las decisiones tomadas durante mi vida y por soportar estar tan lejos de mí. Vreau să mulţumesc părinţilor, surorii şi bunicilor pentru sprijinul necondiţionat ce mi l-au acordat în toate deciziile luate pe parcursul vieţii şi pentru faptul că au suportat sa fie atât de departe de mine Por último agradezco al Ministerio de Educación Cultura y Deporte la concesión de la beca FPU que ha permitido la elaboración de este trabajo de Tesis Doctoral.
4 Reconocimiento Nuestro agradecimiento a Huntsman Corporation por la autorización para la reproducción del documento Matrimid 5218/ Matrimid 9725
5 SUMMARY (RESUMEN)
7 SUMMARY This PhD thesis work is aimed to the separation and recovery of valuable gases, hydrogen and carbon monoxide, from industrial residual gas streams by means of membrane technology. The work has been developed within the Research Group Advanced Separation Processes of the Department of Chemical Engineering of the University of Cantabria (Spain) under the frame of the projects: ENE , CTQ /PPQ and CTM supported by the Ministry of Science and Innovation of Spain. Also, the PhD candidate has been granted with a FPU postgraduate research fellowship with the reference AP from the Ministry of Education, Culture and Sport (Spain). The training period has been completed by a short stage period in the Membrane Science & Technology Group, University of Twente, The Netherlands under, the supervision of Dr. Kitty Nijmeijer. Sustainable industrial growth is based on the development of new industrial processes able to solve global important problems like greenhouse gas emissions, energy efficiency and toxic waste. Many academic and industrial efforts are being made in order to reach the zero discharge goal. The separation and valorization of industrial flue gases with complex composition allows approaching sustainability by means of different routes. The production of streams concentrated in valuable components can include (i) a reuse in the same industrial process to increase the energy efficiency of the overall process or (ii) the further use as reactants in the synthesis of various chemicals. In this thesis, a case of study is defined as the tail gas generated in the manufacturing of carbon black, a commodity whose global production reaches 80 million tons, in medium - high sized installations. The tail gas is formed, in a dry basis, by the following gas mixture, in vol %: 60.5% N2, 17.9 % CO, 16.4 % H2 and 5.3 % CO2. Hydrogen and carbon monoxide are identified as major valuable components. It is envisaged that membrane technology will allow to obtain H2 enriched permeate stream when polymeric membranes are used and CO can be obtained as permeate gas stream when facilitated transport - supported liquid membranes are used. Chapter I of this thesis gives a brief introduction over different gas separation methods and shows the industrial sources and importance of H2 and CO. The first part of chapter I focuses on more detailed aspects of polymeric membrane-based H2 separation, including the transport mechanism, the selection of the polymeric material for the manufacturing of membranes, and the mixed gas permeation through polymeric membranes. Also, a description of the production process of carbon black is included. In the second part the CO separation by means of π - complexation is exposed showing the particular aspects involved when facilitated transport - supported liquid membranes are used. Also, an overlook on room temperature ionic
8 liquids is given with the principal focus on their potential use as liquid phase in facilitated transport - supported ionic liquid membranes. Chapter II and III of this thesis deal with the study of polymeric membrane based separation of hydrogen from mixed gas streams composed of H2, CO, N2 and CO2 at different operation conditions, using membranes prepared with a commercial glassy polymer, Matrimid. The methodologies used to prepare both planar and asymmetric hollow fiber membranes are described in detail. In chapter II the use of a planar Matrimid membrane allowed to describe H2 and CO2 permeation behavior of pure, binary, ternary and quaternary mixtures using the dual-mode sorption, partial immobilization model. Non-ideal effects, such as competitive sorption between permeants, have been characterized, providing the mass transfer parameters for the systems. These results provide useful knowledge related to the intrinsic material properties. In chapter III the use of a asymmetric hollow fiber membrane made of the same polymeric material allowed to determine the major differences between the gas permeation (pure and mixed) through an dense isotropic structure (planar membrane) and an asymmetric structure (hollow fiber). Also, a comparative permeation performance with another asymmetric hollow fiber made from a much more permeable glassy polymer, polyphenylene oxide, was made. Chapter IV is focused on the design of a liquid phase system to be used in facilitated transport-supported ionic liquid membranes for the recovery of carbon monoxide. A comprehensive look at the reaction mechanism and the equilibrium parameters obtained from the experimental characterization of the physical and chemical solubility of carbon monoxide in pure ionic liquid 1-Hexyl-3- methylimidazolium chloride ([hmim][cl]) and 1-Hexyl-3-methylimidazolium chlorocuprate obtained by mixing copper chloride with [hmim][cl] is presented. The latter one presented excellent solubility selectivity properties for the separation of the mixture CO/N2. Finally, in Chapter V overall conclusions of the entire work are made. Also prospects for further research are included.
9 RESUMEN Esta tesis doctoral está enfocada hacia la separación y recuperación de hidrogeno y monóxido de carbono de efluentes gaseosos residuales procedentes de procesos industriales de combustión mediante la tecnología de membranas. El presente trabajo ha sido llevado a cabo en el grupo de investigación Procesos Avanzados de Separación del Departamento de Ingeniería Química y Química Inorgánica de la Universidad de Cantabria (España), en el marco de los proyectos ENE , CTQ /PPQ y CTM financiados por el Ministerio de Ciencia e Innovación de España. Asimismo, la candidata a doctora Oana C. David disfruto de una Beca del Programa de Formación de Profesorado Universitario (FPU) con la referencia AP , financiada por el Ministerio de Educación, Cultura y Deporte de España. La formación ha sido completada mediante una estancia de 4 meses en el grupo de investigación Membrane Science & Technology de la University of Twente (Países Bajos) bajo la supervisión de la Dra. Kitty Nijmeijer. El crecimiento industrial sostenible está basado en el desarrollo de nuevos procesos industriales capaces de resolver problemas globales como la emisión de gases residuales, la eficiencia energética y la generación de residuos tóxicos. En la actualidad, se realizan muchos esfuerzos académicos e industriales para conseguir el objetivo de vertido cero. La separación y valorización de gases residuales de la industria con composición compleja permite acercarse al objetivo de sostenibilidad mediante varias aproximaciones. Las corrientes gaseosas concentradas en componentes con valor añadido se pueden reusar mediante combustión en el mismo proceso industrial para aumentar la eficiencia energética global, o bien posteriormente como reactivos en la síntesis de compuestos químicos múltiples. En el presente trabajo se ha definido como caso de estudio la corriente de gases generada en la fabricación de negro de carbono, un commodity cuya producción mundial alcanza los 80 millones de toneladas anuales, en plantas de tamaño medio - grande. Esta corriente residual está formada por la siguiente mezcla gaseosa, cuya composición en porcentajes de volumen es: 60.5 % N2, 17.9 % CO, 16.4 % H2 and 5.3 % CO2, de la cual el hidrógeno y el monóxido de carbono son los más valiosos. Se espera que el uso de tecnologías de separación con membranas permita obtener en el lado del permeado de la membrana una corriente enriquecida en hidrógeno al emplear una membrana polimérica y una corriente enriquecida en monóxido de carbono mediante el transporte facilitado a través de una membrana líquida soportada. El Capítulo I de la tesis contiene una introducción sobre los distintos métodos de separación de gases y presenta las fuentes e importancia industrial de H2 y CO. La primera parte del capítulo I enfoca aspectos detallados relacionados con la
10 separación de H2 basada en la tecnología de membranas, así como el mecanismo de transporte, la selección del material polimérico empleado en la fabricación de las membranas y la permeación de mezclas gaseosas a través de membranas poliméricas. Además, se incluye una descripción del proceso productivo del negro de carbono. En la segunda parte del capítulo I se expone la separación del CO mediante la complejación - π indicando los aspectos particulares que aparecen en procesos de transporte facilitado a través de membranas líquidas soportadas. Los capítulos II y III de la tesis abarcan el estudio de la separación selectiva de hidrógeno a partir de corrientes gaseosas compuestas por mezclas de H2, CO, N2 y CO2 utilizando membranas preparadas a partir de un polímero comercial de tipo vítreo, denominado Matrimid. Se describen en detalle las distintas metodologías empleadas en la elaboración de membranas con morfología bien de película plana densa o bien en configuración de fibra hueca. En el capítulo II el uso de una membrana plana de Matrimid permitió la descripción de las propiedades de permeación del H2 y CO2 puros y en mezclas binarias, ternarias y cuaternarias mediante el uso del modelo matemático modo dual de adsorción, inmovilización parcial ( dual-mode sorption, partial immobilization ). Se caracterizaron efectos no-ideales como son la adsorción competitiva, que permitieron determinar los parámetros de transferencia de materia implicados en los sistemas bajo estudio. En el capítulo III el uso de una membrana con una morfología de fibra hueca asimétrica preparada del mismo material polimérico permitió establecer las principales diferencias en la permeación de gases puros o mezclas de gases que aparecen al utilizar una estructura asimétrica (fibra hueca) frente al caso de aplicar una estructura isotrópica densa (membrana plana). Además, se realizó un estudio comparativo entre las propiedades de permeación de gases de la fibra hueca de Matrimid con los de otra fibra hueca asimétrica basada en un polímero mucho más permeable (PPO). El capítulo IV está enfocado al diseño de un sistema líquido para ser usado en el transporte facilitado a través de membranas líquidas soportadas para la recuperación del CO. Se realizó un análisis exhaustivo sobre el mecanismo de reacción y los parámetros de equilibrio obtenidos mediante la caracterización experimental de la solubilidad física y química del monóxido de carbono en el líquido iónico puro 1- Hexil-3-metilimidazolio cloruro ([hmim][cl]) y en 1-Hexil-3-metilimidazolio clorocuprato obtenido mediante la mezcla de cloruro de cobre (I) con [hmim][cl]. Esta última mezcla presenta unas propiedades de selectividad de la solubilidad excelentes para la separación CO/N2. Finalmente, el capítulo V presenta las conclusiones globales del trabajo de tesis doctoral. Además, se incluyen perspectivas para la investigación futura.
11 Table of contents
13 Summary (Resumen) V Chapter I INTRODUCTION Gas separation Carbon Black manufacture Hydrogen Hydrogen separation by polymeric membranes Polymer selection Mixed gas permeation in polymeric membranes Carbon monoxide Carbon monoxide separation Facilitated transport supported liquid membranes Ionic liquids Thesis scope and outline 31 References 32 Chapter II MIXED GAS SEPARATION STUDY FOR THE HYDROGEN RECOVERY FROM H2/CO/N2/CO2 POST COMBUSTION MIXTURES USING A MATRIMID MEMBRANE 41 Abstract The dual-mode sorption, partial immobilization theory The non equilibrium lattice fluid model NELF model Experimental methodology Materials Preparation of dense planar Matrimid polymeric membranes Membrane characterization Mixed gas separation set up 54
14 Experimental procedure and operation conditions Results and discussion H2, N2, CO2 and CO pure gas permeation experiments H2/N2/CO2/CO binary, ternary and quaternary mixed gas permeation experiments Mixed gas selectivity Mathematical modeling Conclusions 73 References 74 Chapter III HYDROGEN MIXED GAS SEPARATION STUDY USING ASYMETRIC HOLLOW FIBER MEMBRANES 77 Abstract Preparation of asymmetric hollow fiber membranes background Experimental methodology Materials Fabrication of asymmetric hollow fiber membranes by the dry/wet spinning process Permeation set-up Experimental procedure and operation conditions Results and discussion Morphological and structural characterization Gas permeation through asymmetric Matrimid hollow fibers Gas permeation through asymmetric PPO hollow fibers Conclusions 115 References 116
15 Chapter IV ON THE IMPROVED ABSORPTION OF CARBON MONOXIDE IN THE IONIC LIQUID 1-HEXYL-3-METHYLIMIDAZOLIUM CHLOROCUPRATE 121 Abstract The selection of carrier/solvent system Equilibrium modeling Experimental methodology Preparation of the copper (I) based ionic liquid Absorption set-up and measuring procedure Experimental procedure and operation conditions Results and discussion The physical solubility of CO and N2 in pure [hmim][cl] and in the reactive CuCl/[hmim][Cl] medium The total solubility of CO in the reactive CuCl/[hmim][Cl] medium Desorption study Conclusions 149 References 150 Chapter V OVERALL CONCLUSIONS AND PROSPECTS FOR THE FUTURE 155 Appendices 165 Publications in relation with this PhD thesis 183
17 Chapter I INTRODUCTION
18 2 Chapter I
19 Introduction GAS SEPARATION The major, industrially applied gas separation technologies like pressure swing adsorption (PSA), temperature swing adsorption (TSA), liquid absorption and stripping, cryogenic distillation and membrane separation play today a critical role in a number of large chemical processes as summarized in Table I - 1. Table I - 1. Gas separation technologies and their applications Technology Separation Process Ref PSA and TSA Cryogenic distillation Absorption and stripping Membrane separation O2/N2 CO, CO2, CH4, N2/H2 H2O/EtOH, air CO2/C2H4, CH4 O2/N2 olefin/paraffin SO3 CO2/H2S NH3 CO2 olefin/paraffin O2/N2 CO2, H2S, H2O/CH4 CO, CO2, CH4, N2/H2 Ethylene, propylene/n2 H2O/Air, H2O/CH4 Air separation Hydrogen purification Ethanol and air drying Enrichment of natural gas Air separation Ethylene plant Concentration of sulfuric acid CO2 Recovery from flue gases Phosam process The production of sodium carbonate Ethylene plant N2 or O2 enrichment of air Enrichment of natural gas Hydrogen purification Polyolefin plant resin degassing Air drying, natural gas drying     As listed in Table I - 1 gas separation technologies are in most cases competing for the same application. For high product purity requirements, a combination of technologies is preferred. For example, in the production of high purity N2, O2 and Ar from air, a PSA unit is used to remove CO2 and H2O prior to the cryogenic distillation in order to avoid the deposition of frozen CO2 and H2O within the process equipment . The selection of a separation process must take into account first the recovery and purity specifications of the product, then the difference between the properties of the components to be separated and finally the scale of operation [3, 5, 6]. The specific advantages and disadvantages of each technology are reported in Table I - 2.
20 4 Chapter I Table I - 2. Pros and cons of existing gas separation technologies Technology and property differences PSA and TSA Surface sorption Cryogenic distillation - Gas boiling temperatures Absorption and stripping Physical or/and chemical absorption Membrane separation Diffusivity and solubility Supported liquid membranes Diffusivity and reaction equilibrium Advantages High purity product Suitable at small-scale for air separation The most economic for large scale separation of air Excellent for acid gas (H2S, COS) removal before PSA Low power usage and costs, Simplicity in operation , Compactness and portability Small scale separations Scalability to small sizes High gas selectivity and permeability values The possibility to use expensive carriers (low quantity used) Disadvantages High power usage and costs Slow heating and cooling steps for TSA Low adsorbate concentrations in the feed (less than 3 wt. %) It is not practical for high purity High energy requirements Difficulty in separating gases of similar volatility  Limited loadings High energy requirements. Solvent corrosion and degradation. Modest operating temperature Limited gas purity Structural damage with plasticizing gases Productivity/selectivity trade off Low pressure product (H2) Carrier chemical degradation Loss of solvent (volatilization) Membrane instability It is not yet industrialized  Table I - 2 stresses the economics and operational advantages that membrane technology presents over the other gas separation alternatives, making it the preferred technology for modest product purity requirements and for small scale separation. In recent years much progress has been made in the field of gas separation by supported liquid membrane technology, but the implantation of this technology at industrial scale is expected to be on the midterm since developments are still needed . Since 1980 when the first large industrial application of membrane technology was launched by Permea, membrane based operations, substituting or integrated with the traditional ones, have experienced a rapid growth,
21 Introduction 5 with many companies, such as Cynara Natco, Separex UOP, GMS, Generon, Praxair, AirProducts, UBE. A list of the main industrial applications of membrane technology in gas separation along with the membrane materials used and the status of the membrane technology is given in Table I -3. Also, a comparison of membrane with other gas separation technologies is made in references [10, 11]. Table I 3. Main applications of membrane technology for gas separation . Separation Process H2/N2 H2/CO H2/ hydrocarbons H2/light hydrocarbons O2/N2 N2/CH4 Ammonia purge gas Adjustment of H2/CO ratio in syngas plant H2 recovery in refineries Ethylene cracker Air separation Nitrogen removal Traditional technology PSA PSA PSA Cryogenic distillation Cryogenic distillation Cryogenic distillation Membrane material Pd-based Polysulfone Pd-based Silicon rubber Polyimide Pd-based Silicon rubber Polyimide Status of membrane technology application Lab scale Plant installed (Prism by Permea) Lab scale Lab scale Plant installed (Separex) Lab scale Plant installed (Sinopec Zhenhai, China); Prism by Permea (Du Pont) Cellulose acetate Separex UOP (Petronor, Spain) Pd-based PTMS, PMP Lab scale Pilot plant Silicon rubber Plant installed: (Cynara; Separex; GMS; Air Products) Polysulfone Polyimide Plant installed (Permea) Plant installed (Medal; Dow-Generan; UBE) Polyphenylene Plant installed (Aquilo) Ethyl Cellulose Plant installed (Air Liquide) Ion transport Lab scale Silicon rubber PMP Parel PEBAX Pilot plant Lab scale
22 6 Chapter I Table I 3. (continued) Separation Process H2O/CH4 CO2/CH4 CO2/ Hydrocarbons CO2/N2 VOCs/gas Traditional technology Dehydration Glycol absorption Sweetening of natural gas Natural gas liquid removal CO2 capture from flue gases streams Polyolefin plant resin degassing; Ethylene recovery Amine absorption Glycol absorption and cooling in a propane refrigeration plant (-20 o C) Amine absorption Adsorption, Refrigeration and turbo expander plants Membrane material Cellulose acetate Polyimide Polyaramide Cellulose acetate Status of membrane technology application Plant installed Offshore platforms in Thailand gulf (Cynara NATCO; Grace Separex) Polyaramide Plant installed (Medal) Polyimide Perfluoro - polymers Cellulose acetate Polyaramide Polyimide Polyimide FSC, PEEKWC, Zeolite, silica based carbon. Silicone rubber, PTMS Plant installed (Medal) Plant installed (MTR) Early commercial stage. A demonstration system installed Pilot plant Lab scale Plant installed (MTR; OPW Vaporsaver ) 1.2. CARBON BLACK MANUFACTURE Carbon black is a generic term for an important family of products used widely to modify the mechanical, electrical, and other physical properties of the medium in which it is dispersed. It is the most widely used nano - material, with particle dimensions ranging from tens of nanometers to a few hundred nanometers. It plays a major role in elastomers, plastics, paints and inks as a reinforcing agent, a black pigment, and an electrically conductive material .
23 Introduction 7 There are two main types of carbon black: rubber grade, and special grade. The rubber grades are primarily used as a reinforcing agent in tyres and other rubber products to improve their mechanical properties. Most of the special grades are manufactured to meet product specifications for imparting certain properties required by the end - use products, such as dispersion, pigmentation, and electrical conductivity. There are several alternatives for the manufacture of carbon black, including oil-furnace black process, thermal black process, acetylene black process, lampblack process, and impingement black process. The oil-furnace black process is predominant. In this process carbon black is produced by injecting a hydrocarbon raw material into a flow of reducing hot gas wherein the feedstock is pyrolyzed and converted into a smoke before being quenched by a water spray. The carbon black formation can be described in terms of nucleation, growth and structure development and occurs by condensation and dehydrogenation reaction as described by Equation I 1. . 1 (I - 1) The carbon black production process scheme using an axial flow reactor developed by Columbian Black Company  is shown in Figure I 1. Figure I 1. Carbon black manufacturing process scheme
24 8 Chapter I The hot gas is produced by burning fuel into a combustion chamber. The hot gas flows from the combustion chamber into a reaction chamber which is in open communication with the combustion chamber. The hydrocarbon raw material is introduced into the hot gas as the hot gas flows through the reaction chamber, thereby forming a reaction mixture comprising particles of forming carbon black. The reaction mixture flows from the reaction chamber into an exit chamber which is in open communication with reaction chamber. At some location in the exit chamber a quench spray is introduced into the flowing reaction mixture, thereby lowering the temperature of the reaction mixture below the temperature necessary for carbon black production and halting the carbon black formation reaction. The carbon black particles are then separated from the flow of gas. The carbon black formation occurs in the temperature range of 1250 to 1650 o C. After collecting carbon black in bag filters a tail gas stream is generated that can contain as much as 40 to 55 mol% of water vapor due to the process water used to control the reaction effluent. Even diluted with water the tail gas stream possesses sufficient heating value in order to be used as flue gas under dryers, boilers, and in incinerators. On dry basis the heating value of the tail gas is of 1011 kcal/m 3 (STP) . This combustion step to recover heat has the added benefit of cleaning up the effluent gas from carbon black particulate. It ultimately contains gaseous components in an oxidized state: CO2, SO2, NOx with small amount of CO and it is discharged to the atmosphere or given further treatment (stack gas scrubbing). Typical hydrocarbon feedstock for the oil-furnace process include: cat cracker decant oil, ethylene plant residuum from naphtha cracking, ethylene plant residuum from gas oil cracking, extract from solvent refining of cat cracker cyclic oils and coal tar distillate. A comprehensive review of the technical and commercial aspects of carbon black usage along with the history of carbon black, its microstructure, chemical composition, morphology, surface activity, and characterization are discussed in reference  HYDROGEN Hydrogen (H2) in the lithosphere is, with few exceptions, bound to other elements (e.g., as in water) and must be separated by using other sources of energy to produce molecular hydrogen. Properly considered, hydrogen fuel is not a primary energy source in the context of a hydrogen economy . The increased awareness of the finite nature of our fossil fuel sources and their uneven distribution favor today a transition to a new energy system based on hydrogen, a clean energy vector.
25 Introduction 9 Hydrogen can be produced by various means: steam reforming, partial oxidation, autothermal reforming, combined two step reforming of light hydrocarbons (mainly methane), gasification of coal, petroleum, petcoke, biomass, petroleum refining, from coke oven gas, supercritical water gasification (dissolution of organic compounds and lignocellulosic materials as solid biomass in supercritical water at elevated temperature) electrolysis of water by wind, solar or grid energy, thermal splitting of water by nuclear energy. Today, the most widely used method (80 %) for H2 production is the steam reforming of light hydrocarbons [18, 19]. The production of H2 from the gasification of coal is expected to present a significant increase in the future due to the great research effort dedicated to the technological improvement to make the process economic. The gasifier feed stocks (coal, biomass and petroleum coke) are all significantly lower cost than oil or natural gas, but gasification and downstream processing of syngas to make electricity are expensive . In the low oxygen environment of the gasifier secondary compounds like hydrogen sulfide (H2S), carbonil sulfide (COS), ammonia (NH3), hydrogen cyanide (HCN), hydrogen chloride (HCl) together with trace elements like mercury, arsenic and other heavy metals are formed and must be removed. Technologies such as the co-production of H2 and power from the coal generated syngas in an Integrated Gasification Combined Cycle (IGCC) are contemplated . Both methods generate in the first stage syngas that is followed by the high or low temperature, water-gas shift (WGS) reaction for further hydrogen conversion: (I - 2) The separation of CO2 from shifted syngas is done currently by amine absorption, but may also be done by the absorption of CO2 in chilled methanol or ethylene glycol (the Rectisol or Selexol process, respectively) or by means of membrane technology. Membrane-based technology approaches may reduce the cost of amine based process estimated in $40-100/ton CO2 . Other sources of hydrogen include the tail gas stream from petroleum refining, ammonia purge gas, coke oven gas and the flue gases from carbon black manufacturing. The typical composition of these major sources of H2 is listed in Table I - 4.
26 10 Chapter I Table I 4. Typical compositions found in common hydrogen sources. Hydrogen source Composition (mol %) Syngas from autothermal reforming of natural gas H N2 0.2 CO2 2.9 CO 29 Syngas from gasification of coal with oxygen and steam Dry shifted syngas Hot shifted syngas Petroleum refining Naptha hydrotreater Light naptha isomerization Mild hydrocracking Ammonia purge gas Dry coke oven gas Carbon black manufacturing tail gases CH H2S Other 10.1 H2O 2-30 H2O - 10 H2O 4.8 C C C2+ 2 NH3, 4.5 Ar - - T ( o C) P (bar) Ref       
27 Introduction Hydrogen separation by polymeric membranes Today, membrane technology is successfully applied at industrial level for hydrogen recovery from ammonia purge streams, syngas ratio adjustment and hydrogen recovery in refineries. These three applications involve easy task separations since the extraordinary small molecular size of H2 makes it extremely permeable and easily collected as permeant compared to the other slower permeating components: N2, CO and CH4. Surprisingly, it is difficult to separate H2 from CO2 . Broadly, hydrogen selective membranes (based on the materials used) can be categorized into two types: organic (polymer) and inorganic (metallic, carbon, and ceramic). High-purity hydrogen (up to 99.99%) could be available through dense metallic membranes and especially through Pd and its alloys, but the commercial application of metallic membranes faces today important limitations due to drawbacks like: (i) poisoning effect that hydrogen sulfide (H2S) and other feedstocks have on the hydrogen transport mechanism, (ii) high cost for the preparation of Pd membranes and (iii) mechanical stability . The key advantages of polymer membranes are the ability to cope with high pressure drops and low cost. Therefore, the separation of H2 by polymeric membranes has become an attractive existing technology. Generally, gas transport in non-porous (dense) membranes occurs via the solution-diffusion mechanism, comprised of three main steps: 1. Sorption of the gaseous penetrants at the upstream side of the membrane, 2. Diffusion of the penetrants across the membrane, 3. Desorption of the penetrants at the downstream side of the membrane . The solution diffusion mechanism is driven by a difference in the thermodynamic activities existing at the upstream and downstream faces of the membrane as well as the interacting force working between the molecules that constitute the membrane material and the permeate molecules. The activity difference causes a concentration difference that leads to diffusion in the direction of decreasing activity. Fick s law is the simplest description of gas diffusion through a nonporous structure , i.e. I 3 where Ji is the permeation flux through the membrane of a component i, Di is the diffusion coefficient and the driving force dci/dx is the concentration gradient across
28 12 Chapter I the membrane. Under steady-state conditions this equation can be integrated to give:,, I 4 where C2,i and C1,i are the concentration at the upstream and downstream side of the membrane, respectively and δ is the thickness of the membrane. In ideal systems, the concentrations are related to the partial pressures by Henry s law which states that a linear relationship exists between the concentration inside the membrane (Ci) and the (partial) pressure of gas outside the membrane (pi), i-e. I 5 where Si (cm 3 (STP) cm -3 bar -1 ) is the solubility coefficient of component i in the membrane. Henry s law is mainly applicable to amorphous elastomeric polymers because solubility behavior is often more complex below the glass transition temperature, as described in chapter II by the dual sorption partial immobilization model. Combining Equation I - 4 with Equation I - 5 gives:,, I 6 an equation which is generally used for the description of gas permeation through membranes. The product of the diffusion coefficient and solubility coefficient is called the permeability coefficient Pi, i.e. I 7 The diffusion coefficient is a kinetic parameter that measures the mobility of the penetrant molecules in the membrane and is mainly dependent by the gas kinetic diameter. The kinetic diameter of a gas is defined as the intermolecular distance of closest approach for two molecules colliding with zero initial kinetic
29 Introduction 13 energy . This is dependent on the molecular size, shape, as well as dipole-dipole interactions. In polymer materials, diffusion coefficients decrease as the molecular size increases, because large molecules interact with more segments of the polymer chain than small molecules do. The solubility coefficient is a thermodynamic parameter expressed by the ratio of the dissolved penetrant concentration in the polymer to the pressure of the continuous gas phase and it is a measure of the energy required by the gas to be sorbed by the polymer . The value of the solubility coefficient increases with increasing gas condensability. A measure of the gas condensability is given by the gas critical temperature . In general, gases with large diffusivity values present low solubility values and the opposite. Table I - 5 lists the values of the kinetic diameter and the critical temperature of a range of species found in H2 recovery. Table I 5. Kinetic diameter  and critical temperature  of various molecules found in H2 recovery. Gas Kinetic diameter (Å) H2O H CO O H2S N CO CH C3H Critical temperature (K) Below the glass-transition temperature, the polymer chains are essentially fixed; the polymer is a rigid, tough, glassy material and the effect of differences in size of the permeating gases on their relative mobility is large. If the polymer is above its glass transition temperature, motion of the polymer chains is possible. The polymer is then rubbery and elastic and the effect of molecular size of the permeating gases on relative mobility is reduced. Therefore, glassy polymers discriminate gas species transport according to gas diffusivity and elastic polymer according to gas solubility. Consequently, the order of gas permeability in glassy
30 14 Chapter I polymers is therefore determined by the gas kinetic diameter, whereas in rubbery polymers the order is determined by gas condensability . In Figure I 2 the values of the kinetic diameter and gas critical temperature are listed in an increasing order to show the difference in the order of gas permeability for glassy and for rubbery polymeric membranes. Figure I - 2. Depiction showing the relative size (kinetic diameter) and condensability (boiling point) of various gases. Glassy membranes generally separate using differences in size; rubbery membranes separate using differences in condensability. The separation factor (ideal selectivity) characterizes membranes in terms of separation and is defined, in the case of negligible downstream pressure, as the ratio of permeabilities / I 8 In the case of gas mixture the gas selectivity is calculated according to equation I 9:
31 Introduction 15 / I 9 where C is the gas concentration (vol %) and P refers to the permeate and F to the feed side of the membrane Membranes based on rubbery polymers minimize size selectivity and maximize sorption selectivity, and, therefore are used for the separation of highly condensable gases like propane and other hydrocarbons from methane. Membranes based on glassy polymers are best used for the separation of highly mobile gases like hydrogen, i.e. H2/CO and H2/N2 separations. Although H2 has a high diffusivity, because of its low condensability, it has a very low solubility in membranes. A more soluble, lower diffusivity gas such as CO2 may have a steady state permeability comparable to that of H2 . Therefore, for H2/CO2 separation both glassy and rubbery polymers can be used with H2 or CO2 respectively as the permeating specie, but the application of polymeric membranes for separation H2 and CO2 is restrained. Gas separation membranes need to be highly permeable to one of the mixture components while significantly rejecting the other components. The vast amounts of polymers that have been investigated, however, show the general trend that highly permeable polymers possess low selectivities. This effect is referred as the permeability/ selectivity trade off relationship and Robeson  has suggested that possesses an upper limit which needs to be exceeded in order to obtain progress in the application of polymeric membranes for gas separation. This upper limit, also referred to as upper bound, was determined by plotting the ideal separation factor versus permeability values of multiple gas pairs of interest. This limit is given by the latest gas separation data available in the literature and belongs to high performance polymers unavailable at commercial scale. The last available upper bound correlations were reported in 2008 and are shown in Figure I - 3 for H2/N2 and H2/CO2 gas pairs of interest in this work. Figure I 3 also includes the prior upper bound reported in 1991 . In the case of H2/N2 correlation, although a large amount of data has been generated since 1991, a very minor shift in the upper bound relationship is noted. In the case of H2/CO2 a limited shift in the upper bound relationship is noted, primarily a slight slope change resulting from a number of data points at the higher permeability end of the relationship. The limited number of data points at the lower permeability area of the dataset may have skewed the slope versus the original correlation.
32 16 Chapter I Figure I 3. The upper bound correlations for H2/N2 and H2/CO2 separation . A further limitation for H2 recovery is given by streams like the shifted syngas and refinery purges that contain components that strongly affect the membrane performance and durability (CO2 and light hydrocarbons) . Different ways to overcome this problems include today the development of new membrane materials like polymers with high inner porosity [37-40], hiperbranched polyimides [41, 42], perfluorinated copolymers [43, 44] or the incorporation of inorganic nano particles of high porosity and permeability into the polymer matrix (Mixed Matrix Membranes - MMMs) [45-47] Polymer selection In order to choose the best performance material for H2 recovery from the carbon black manufacturing tail gas stream first of all it must be determined if a glassy or rubbery polymer will be used. As explained in section the separation of H2 from N2 is best done by membranes based on glassy polymers meanwhile for H2/CO2 separation both glassy and rubbery polymers can be used. Therefore, considering the high concentration of N2 in the carbon black manufacturing tail gas (see Table I 4) it was determined that a H2 permeable polymer (a glassy polymer) must be used. Also, due to the low concentration of H2 in the gas mixture of case studied in this work, a polymer with high selectivity towards H2 and reasonable permeability is needed. At this point, an analysis of gas permeation properties of various commercial polymers was made (data listed in Table I 6) by plotting H2/N2 and H2/CO2 selectivity values versus H2 permeability in Robeson-type plots (see Figure I - 4)
33 Introduction 17 where the Robesson upper - bound limit was included. Little or no available data was found for CO, but it is known that CO transport behavior is similar to that of N2 and therefore it can be assumed that an optimum polymer choice for H2/N2 will also apply for H2/CO separation. Table I - 6. Glass transition temperature (Tg), density and permeation properties of commercial available polymers used in membrane based gas separation Commercial Polymers Tg (K) Density (g/cm 3 ) P H2 (Barrer) Ideal selectivity H 2/N 2 H 2/CO 2 Exp. Cond. Poly (vinylidene floride), PVDF 238 a 1.75 a 2.4 b 3.42 b 2 b 30 o C, 1.4 bar Poly (methyl methacrilate), PMMA 379 a 1.17 a 2.4 b 2 b 4 b 30 o C, 1.4 bar Cellulose acetate, CA a 2.63 c c 0.4 c 30 o C 473 a Polyetersulfone, PES 498 a 1.37 a 8.96 d 69.5 d 2.7 d 35 o C, 3.5 bar Polyetherimide, Ultem 209 e 1.27 e 11 f 50 f 5.9 c 30 o C Bisphenol-A polycarbonate 423 a 1.2 e 11.5 g 42.6 g 2.1 g 25 o C, 3.7bar Bisphenol A Polysulfone 459 a 1.24 e 14 c 56 c 2.5 c 30 o C Poly (ethylene) low density, LDPE 148 a 0.92 a 17.3 b 4.1 b 1 b 30 o C, 1.4 bar Polystyrene, PS Polyimide, Matrimid 373 a 1.04 a 23.8 b 28.8 b 2.3 b 30 o C, 1.4 bar 502 d 1.24 e h 97 h 3.9 h 35 o C, 3.5 bar Polyimide, PBI 691 i i 0.6 i 125 i 3.75 i 35 o C, 20 bar Ethyl cellulose, 316 a 1.14 a 87 c 27.2 c 3.3 c 30 o C Polyphenyleneoxide, PPO 483 a 1.06 e 113 c 29.7 c 1.5 c 30 o C Poly (4-methyl pentene-1) 323 a a 125 c 18.7 c 1.5 c 30 o C Poly (dimethylsiloxane), PDMS 150 a 0.97 a 550 c 2.2 c 0.2 c 30 o C a :, b :, c :, d :, e :, f :, g :, h :. i :
34 18 Chapter I Figure I 5. The chemical structure of (a) Matrimid 5218 and (b) PPO monomer unit It was decided that the commercial Matrimid 5218, an aromatic polyimide of 3,3,4,4 -benzophenone tetracarboxylic dianhydride and diaminophenylidane, presents a good tradeoff between H2 permeability and both H2/N2 and H2/CO2 selectivities and it was considered to be the optimum polymer for H2 recovery. Also, it was decided to study a more permeable material. PPO, poly(2,6- dimethyl-1,4-phenyelene oxide), is a polymer that, because it posses high fractional free volume, it exhibits unexpectedly high values of gas permeabilities for a glassy polymer. The gas selectivity of this material is relatively low but still higher when compared with rubbery polymers. This opposite gas performance properties are reflected in Figure I 4 and the chemical structure of these polymers is shown in Figure I - 5. Aromatic polyimides are one of the most important classes of high performance polymers. They are highly thermally stable, have high glass transition temperatures and relatively low dielectric constants. The various polyimides have become important in many applications, such as semiconductor devices, high temperature adhesives, and high performance composite materials . Matrimid attracted a lot of attention for gas separation membranes due to the combination of
35 Introduction 19 relatively high gas permeability coefficients and separation factors coupled with excellent mechanical properties solubility in non-hazard organic solvents and commercial availability . It has a high glass transition temperature (see Table I 6). Detailed polymer data are found in the Polymer Data Sheet provided by the manufacturer (see Appendix I). As means of improving membrane performance towards the permeation of gas mixtures of H2 that contain CO2 and suppress CO2 induced plasticization, polymer blending method has been recently approached [58, 59]. New asymmetric hollow fiber membranes were fabricated from polymer blends of Matrimid and another polyimide, poly(2,2 -(1,3- phenylene)-5,5 -bibenzimidazole), (PBI) . PBI is a high performance polymer with a relatively high glass transition temperature ( 418 C), outstanding thermal and chemical stabilities , high H2/N2 and H2/CO2 gas selectivity but extremely low gas permeability due to a high packing density of the polymer matrix (see Table I 6). Severe brittleness of PBI material has been a major limitation for its applications in membrane processes and in literature a blend of Matrimid with PBI was already employed to synergize the advantages of each material to create a superior membrane for pervaporation and gas separation [60-62]. The nature of miscibility of Matrimid/PBI in all polymer compositions is believed to be the intense hydrogen bonding between N-H group of PBI and C=O group of Matrimid which provides a specific interaction for intermolecular compatibility  as expressed in Figure I - 6. Figure I 6. Chemical structures of PBI and Matrimid. The dotted line between the polymers represent hydrogen bonding interaction between functional groups of polymers.
36 20 Chapter I A literature survey shows that a blend of 50 wt % of each polymer was revealed to be the best for H2 separation with a value of H2 permeability of 13 Barrer and H2/CO2 and H2/N2 selectivity of 6.05 and respectively . Therefore, asymmetric hollow fiber membranes based 50 wt % of each polymer where fabricated in this work Mixed gas permeation in polymeric membranes Generally, the permeation behavior of a pure gas through a membrane depends mainly on the properties of the gas and membrane as well as the operation conditions. As for gas mixtures the transport behavior of one component through the membrane is affected by the presence of other penetrants so that it deviates from that of the pure gas. Therefore, using the permeation data of pure gases to estimate the separation properties of gas mixtures may lead to wrong results [64, 65]. The deviations are in general attributed to different factors, from which the solubility coupling by competitive sorption effects, membrane plasticization and the concentration polarization phenomena are more prevalent. The solubility coupling occurs between the penetrants and the polymer matrix, and in the case of glassy polymers is a negative effect which means that induces a decrease in the gas permeability. In the polymer matrix a fixed amount of sorption sites are present, which get saturated at a certain pressure, thereby leading to a decrease in solubility coefficient at higher penetrant pressures . This may be explained in terms of the simple dual-mode sorption, partial immobilization model: penetrants compete for sorption sites which are associated with the nonequilibrium free volume in glassy polymers . On the other hand, some penetrants sorb into polymers to such a degree that they plasticize the polymer. Plasticization effectively increases the chain spacing in the polymer and increases the chain mobility so that the diffusion and permeation coefficients increase with increasing penetrant pressure. Finally, the concentration polarization phenomenon is a consequence of the depletion of fast permeating molecules at the membrane surface due to the accumulation of slow permeating molecules in the gas phase adjacent to the membrane.
37 Introduction CARBON MONOXIDE Carbon monoxide is a key raw material in the synthetic routes for a variety of major chemical products including methanol, formaldehyde, acetic acid, isocyanates, aldehydes, formic acid, pesticides, and herbicides. It has an increased importance as raw material for liquid hydrocarbon fuels in the Fischer-Tropsch process where CO molecules are coupled to C-C bond formation . All sources of carbon monoxide are essentially gas mixtures, most common being the synthesis gas and coke-oven gas  with typical composition listed in Table I - 4. Today, chemicals and liquid transportation fuels obtained from synthesis gas represent the leading products with 45% and 38%, respectively, of the world gasification capacity for operating plants identified in the 2010 database compiled by the U.S. Department of Energy - National Energy Technology Laboratory . The other products are electric power and gaseous fuels (40-60 vol % H2 purity requirement). The recovery of CO from synthesis gas and coke oven gas would represent an abundant and relatively inexpensive source of CO that would greatly enhance further growth of CO as a raw material for the chemical industry. Such growth could result in the CO-based chemical industries approaching the same level of importance as the ethylene-based chemical industries . The recovery of CO from the flue gases would also contribute to the reduction in the process emissions approaching the zero discharge goal Carbon monoxide separation Pure carbon monoxide is obtained either by reversible complexation or cryogenic separation, using technologies like CO absorption in ammoniacal cuprous chloride, aromatic CuAlCl4 solution (COSORB), cryogenic fractionation and pressure swing adsorption (PSA) [72-74]. Chemical complexation The separation of CO by reversible complexation is based on its ability along with that of olefins, aromatic and thiophenic compounds to form a π complexation bound with d- block transition metals and their ions . As shown in Figure I 7 the bound is constituted of two contributions: the usual σ bound formed by the
38 22 Chapter I overlapping of the bounding π electrons of the gas to the unoccupied outermost s orbital of the metal and the additional back-donation from the metal d orbital to the empty antibonding π orbital of the gas [76-79]. Also a possible redistribution between d orbitals is shown. Figure I 7. Scheme of the CO-Cu interactions by π-complexation, showing (a) donation of π-electrons of carbon monoxide to the 4s orbital of Cu, (b) backdonation of electrons from the 3dyz orbitals of Cu to the antibonding π orbitals of carbon monoxide, and (c) electron redistribution. (c) depicts the possible electron redistribution from the 3dz 2 orbitals to the 3dyz orbitals Calculations based on the molecular orbital theory estimate that the bounding strength follows the order : Cu + > Ag + and CO > C2H4 The π-complexation bonds are stronger than those formed by van der Waals interactions, but they are also weak enough to be broken by traditional engineering means such as increasing temperature and/or decreasing pressure . Therefore the chemical complexation reaction is reversible and thus industrially applicable. In addition, like all chemical reactions, the complexation reactions are highly selective. In order for the reaction to be reversible in an economically attractive process it must have appropriate bond energy. Figure I 8 shows the typical bond energy involved in some chemical reactions. Complexation reactions with bond energies
39 Introduction 23 less than 10 kj mol -1 are similar to ordinary associations by van der Waals forces in the condensed state, and reactions with bound energies above 50 kj mol -1 tend to be difficult to reverse without undue expense. Figure I 8. Bound energy most suited for reversible chemical complexation separation processes . Copper (I) salt solutions are able to absorb carbon monoxide to form carbonyl complexes. This property is used in two industrial processes to selectively separate carbon monoxide from a mixture of gases . The copper ammonium salt wash developed by BASF uses aqueous ammonia solutions of copper carbonate, formate, acetate, lactate, or a mixture thereof. The absorption desorption reaction is thought to be an equilibrium between free and coordinated carbon monoxide that is highly dependent on the temperature, pressure, and acidity of the medium (see Equation I 10) (I - 10)
40 24 Chapter I The regeneration of CO is done by heating the rich solution to 350 K, usually at atmospheric pressure. The vapor pressure of ammonia at this temperature is significant and a scrubber can be used to wash the off-gas. The Cosorb process, developed in the early 1970s by Tenneco Chemicals, is based on a similar principle. It uses a copper (I) organometallic complexes in organic solvents (preferably CuAlCl4 in toluene). First a complex is formed with one molecule of CuAlCl4 and one or two molecules of toluene. The chemical complexation between CO and this complex was proposed to follow the reaction described by Equation I 11. (I - 11) This process provides several advantages such as lower corrosion, higher complex stability, and higher purity of the gas produced. Nevertheless, several impurities such as water or sulfur compounds (SO2, H2S, COS, etc.) destroy the copper complex. A very careful purification of the feed gas is therefore required. Also, the availability of Cu + is lowered due to the mixture of CuCl with AlCl3 Generally, conventional absorption processes present the drawback of high energy consumption and operating cost and in particular for CO the main problem is the low solubility in liquid media and the instability of Cu + ion which in a disproportionation reaction gives Cu 0 and Cu 2+. Cryogenic separation and PSA Processes for the cryogenic separation of pure carbon monoxide from a mixture of gases have been developed by, among others, Air Liquide and Linde. The CO/H2 separation is made by a low-temperature partial-condensation process where the mixture of gases is cooled to a temperature of approximately 70 K. The CO/N2 separation is difficult owing to the similar boiling point. Cryogenic distillation is also an energy intensive and expensive separation method. Two commercial PSA plants have been in operation in Japan since 1989 for the recovery of CO from converter gases of steel plants. Depending on the use of the syngas the desired composition ranges from 100% hydrogen (for the production of hydrogen or ammonia) to 100% CO for carbon monoxide or acetic acid production.
41 Introduction Facilitated transport supported liquid membranes The principle of the transport of CO through facilitated transport supported liquid membrane is described in Figure I 9. Figure I 9. The principle of the transport of CO through facilitated transport supported liquid membrane In an SLM system an organic solvent is immobilized into the pores of a porous polymer or inorganic support material by capillary forces . Solution diffusion is the typical solute transport mechanism in a dense, non porous polymer or liquid phase . Facilitated transport membranes operate based on solute partitioning (solubility) and diffusion but also include a reversible complexation as a component of the membranes separation. The complexation reaction in the membrane creates an additional transport that is synergetic with the solution diffusion mechanism. Facilitated transport is analogous to a chemical absorption process on the feed (high partial pressure) side and a stripping process on the permeate side of the membrane (low partial pressure side) .
42 26 Chapter I At the feed side of the membrane CO first dissolves in the membrane, and then it can diffuse or react with the complexing agent. CO diffusion across the facilitated transport membrane can take place by two mechanisms: (a) diffusion of the uncomplexed species or (b) diffusion of the carrier solute complex. The selectivity and reversibility is critical for the separation performance of facilitated transport membranes. Therefore, the key issue in developing a separation process based on reversible complexation is the ability of a carrier to bind selectively to the permeant with appropriate bond energy equilibrium and rate constants (Keq). For a system to be efficient enough recommended values of the equilibrium parameters by Noble et al  are between 2 x 10 2 M -1 and 2 x 10 4 M -1 for facilitated transport of gases in liquid membranes at solubilities around 5 x 10-3 M and partial pressures from 1.01 x 10 4 Pa to 1.01 x 10 5 Pa. Table I - 7 shows the values of the equilibrium constants (Keq) reported in the literature for CO complexation with transition metals and their ions. The literature data listed in Table I 7 are in general previous to 1995; little research effort is dedicated at the present to the facilitated transport of CO through supported liquid membranes. Facilitated transport membranes have several general characteristics: 1. They can be highly selective, especially at low driving forces where other separation methods are not. 2. Very high permeability compared to conventional membranes can be obtained for the solute of interest at very low concentration driving forces. 3. A minimum permeability is reached at high concentration driving forces due to saturation of the reactive transport pathway. 4. The amount of solvent used is very small in comparison with conventional solvent extraction separation approaches for liquid membranes. 5. The quantity of complexing agent used is also very small. 6. Membrane technology allows for continuous separation. 7. Membrane technology is easily scaled for various applications. 8. The use of chemical reaction provides enhanced solute flux as well as selectivity. 9. They are often unstable in the immobilized liquid membrane configuration due to evaporation and/or solvent displacement. Three methods to address the stability problems with facilitated transport membranes are the use of fixed site carrier membranes, hollow-fiber-contained liquid membranes and the use of molten salts with negligible vapor pressure as solvents [83, 84]. Ionic liquids can also be excellent solvents for the carrier agent.
43 Introduction 27 Table I 7 Equilibrium constants (Keq) for CO complexation with transition metal derivatives using facilitated transport liquid membrane systems Element Coordination complex Cu Experimental conditions Keq (kg mol -1 ) Ref CuCl 0.2 M CuCl, 1.0 M KCl, [69, M HCl in water 0.1 M CuCl, 1.0 M KCl, 0.2 M HCl in water CuAlCl4tol2 pco max = 1 bar, CuI/NMIm a M in toluene 2 x10-5 M in Dimethyl CuSCN/NMIm sulfoxide ]  447 e  1700  L b CuB(C6F5)4 Tetrahydrofuran solvent  2+ Fe Fe( TIM )( C 6 H 5CN ) 2 Cl 2 c M in Benzonitrile 420 e  Fe ( Me Cl M in Benzonitrile 180 e 4 TIM )( C 6 H 5CN ) 2 2 Ph2TIM )( C6H 5CN ) 2 2 Fe ( Me Cl M in Benzonitrile 130 e 4 TIM)( C6H5CN) Fe ( Ph Cl M/Nitrobenzene e  Pd 0 d Pd 2 ( dpm ) 2 NCO Dimethylacetamide  2 Pd ( dpm Cl ) 2 2 ) 2 2 Pd ( dpm Br ) Pd ( dpm I 1300 a N-methylimidazole ligand, b Ligand-Cu(I) complexes based on pyridylalkylamine compounds, c Tetraimine macrocyclic ligand (2,3,9,10- tetrametbyl-l,3,8,11-tetraazacyclotetradeca-1,3,8,10 tetraene), d Ph2PCH2PPh2 ligand, e the presented values belong to the reduced equilibrium constant (M -1 ) defined as the ratio between the equilibrium constant (-) and the constant concentration (M) of touene, benzonitrile and nitrobenzene respectively.
44 28 Chapter I Ionic liquids The common definition of ionic liquids (ILs) is that they are liquids that are composed entirely of ions and are fluid below 100 o C . Often, this melting point is even lower than room temperature; therefore ionic liquids are free flowing at room temperature, hence the generic term, room temperature ionic liquids (RTILs). The term ionic liquid covers inorganic as well as organic molten salts. However, the recent literature deals with RTILs made of a bulky nitrogen or phosphorouscontaining dissymmetrical and diffusely charged organic cation and a variety of organic or inorganic anions , leading to a disturbed molecular packaging with high cohesive energy density given by Coulombic interactions between the constituents [94, 95]. Figure I 10 shows the chemical structure of typical anions and cations of commonly found in ionic liquids. Cations: Anions: [CH3COO] - 1-Alkyl-3-methylimidazolium N-Alkylpyridinium R1,2,3,4 = CH3(CH2)n, n = (0, 1, 3, 5, 7, 9); aryl, etc. [CF3COO] -, [NO3] - Br -, Cl -, I - [Al2Cl7] -, [AlCl4] - Water miscible [BF4] - a [OTf] - [N(CN)2] - N, N-Dialkilpyrrolidinium [PF6] - b [NTf2] - [BR1R2R3R4] - Water - inmiscible Figure I 10. Some commonly used ionic liquids . a trifluoromethanesulfanate: [CF3SO3] -, b bis(trifluoromethylsulfonyl)imide: [(CF3SO2)2N] There are a large number of organic cations and anions that can be combined to form different ionic liquids. Overall, the number of possible ionic liquids is estimated around 10 18, whereas the number of traditional solvents widely used in industry accounts for a few hundred .
45 Introduction 29 In addition, their miscibility with water or organic solvents can be tuned through side chain lengths on the cation and choice of the anion. Furthermore, they can be functionalized to act as acids, bases or ligands . Therefore, the possibility arises to optimize the ionic liquid for a specific application by stepwise tuning the relevant solvent properties. For this reason ionic liquids have been referred to as designer solvents . The main advantage of ionic liquids is that they are a new class of solvents by their non-molecular nature. The ionic liquid environment is very different of that of all molecular polar or non-polar organic solvents giving them the following main physical properties: non-measurable vapor pressure which makes them very easy to contain, manipulate, transfer, and allows their use under high vacuum or heating conditions; thus they are considered environment friendly alternatives to VOCs, intrinsic conductivity (Coulombic fluids) and wide electrochemical stability window non-flammability associated with the low vapor pressure, thermal stability (some of them can be heated up to 400 C without degradation which is much greater than most classical organic solvents), wide liquid range (ranging from 75 to 300 o C, which allows a better kinetic control on reactions ), solvating properties for a wide range of organic, inorganic, and organometallic compounds . high heat capacity Based on their unique properties ionic liquids have been extensively studied over the last 10 years and more than publications contain the phrase ionic liquid(s) in the title. There have been many reviews on ionic liquids focused on particular applications, e.g., analysis [ ], synthesis and (bio)catalysis [95, 106], electrochemical devices [107, 108], engineering fluids [ ], separation and purification technology [ ]. The first international congress dedicated to the use of ionic liquids in separation and purification technology (ILSEPT) took place last year (2011) in Sitgets, Spain. A brief overview on the applications of ionic liquids is given in Table I 8.
46 30 Chapter I Table I - 8. Current status of ionic liquids applications at R&D, pilot and commercial level. Functional fluids Synthesis and Catalysis Analytics Electrochemical applications Thermodynamic applications Enzymatic reaction Electrophoresis Solvents for GC head-space Fuel cells and batteries Metal deposition and Metal finishing, Thermal fluids (storage and transfer) Phase changing materials Hydraulic oils, storage media for gases, lubricants, surfactants Immobilization of catalysis matrix-materials for MALDI-TOF-MS Dye sensitized solar cells Sorption cooling media Entrainer in extractive distillation (Basil process BASF ) Application Status R&D Pilot Commercialized Separation and Deep desulfuration Liquid-liquidextraction purification Gas separation technology Nano-particulesynthesis Solvents for organic reactions Solvents for Karl- Fischer titration Solvents for protein crystallization Materials for GC columns Sensors Supercapacitors The use of ionic liquids also has some disadvantages: the physical properties are not always known, their viscosity is usually higher than that of common solvents. Also, the green credentials of ionic liquids are being increasingly questioned due to the growing evidence of their toxicity to aquatic ecosystems, although the mechanisms of toxicity are unknown [ ]. Ionic liquids have found much interest in gas separation by supported liquid membranes (SILMs) as efficient means to suppress the drawbacks associated to this technology (see Table I - 2). The use of these new solvents as a liquid membrane phase results in the stabilization of the SLMs due to their negligible vapor pressure, and their high viscosity (up to 500 cp) which could slow down the displacement of the liquids from the micropores under pressure .
47 Introduction THESIS SCOPE AND OUTLINE The separation and valorization of industrial flue gases with complex composition such as the tail gas generated in the manufacturing of carbon black needs a complex approach. First, membrane technology was selected as the best technology because presents over the other gas separation alternatives economics and operational advantages. Then, the low concentration in valuable components, i. e. H2 and CO, with N2 as the major impurity and the permeation order through membranes (H CO N determines the need for a dual approach: (I) the separation and recovery of H2 using H2 permeable polymers and (II) the separation and recovery of CO by means of chemical complexation using facilitated transport membranes. Therefore the present thesis has the following objectives: 1. The study of polymeric based membrane permeation for pure gases, binary, ternary and quaternary mixtures of H2, CO, N2 and CO2 at different operation conditions using dense polymeric films. 2. The description of H2 and CO2 permeation behavior of pure, binary, ternary and quaternary mixtures using an appropriate mathematical model. 3. The study of permeation behavior of pure gases, binary, ternary and quaternary mixtures of H2, CO, N2 and CO2 through hollow fiber membranes in order to determine the major differences between the gas permeation through a dense isotropic structure (dense-thick film) and an asymmetric structure (hollow fiber, dense thin film supported on a porous sublayer). 4. The design and experimental characterization of a liquid phase system to be used in facilitated transport-supported ionic liquid membranes (SILMs) for the recovery of carbon monoxide. 5. General prospects for further research and industrial implementation.
48 32 Chapter I References 1. S. Sircar, Basic research needs for design of adsorptive gas separation processes, Ind. Eng. Chem. Res. 45 (2006) R.W. Rousseau, Handbook of Separation Process Technology, John Wiley & Sons, New York, P. Bernardo, E. Drioli, G. Golemme, Membrane gas separation: A review/state of the art, Ind. Eng. Chem. Res. 48 (2009) Universal Industrial Gases Inc., Overview of cryogenic air separation and liquefier systems, (2011). 5. H.R. Null, Selection of Separation Process, in: R.W. Rousseau (Ed.), Handbook of Separation Process Technology, John Wiley & Sons, New York, 1987, pp E. Drioli, A.I. Stankiewicz, F. Macedonio, Membrane engineering in process intensification-an overview, J. Membr. Sci. 380 (2011) S. Adhikari, S. Fernando, Hydrogen membrane separation techniques, Ind. Eng. Chem. Res. 45 (2006) L. Shao, B.T. Low, T.-S. Chung, A.R. Greenberg, Polymeric membranes for the hydrogen economy: Contemporary approaches and prospects for the future, J. Membr. Sci. 327 (2009) V.S. Kislik, Liquid membranes: principles and applications in chemical separations and wastewater treatment, Elsevier, Amsterdam, R. Prasad, R.L. Shaner, K.J. Doshi, Comparision of membranes and other gas separation technologies, in: D.R. Paul, P.Y. Yampolskii (Eds.), Polymeric Gas Separation Membranes, CRC Press, Boca Raton, 1994, pp W.J. Koros, G.K. Fleming, Membrane-based gas separation, J. Membr. Sci. 83 (1993) A. Brunetti, P. Bernardo, E. Drioli, G. Barbieri, Membrane Engineering: Progress and Potentialities in Gas Separation, in: Y. Yampolskii, B. Freeman (Eds.), Membrane Gas Separation, John Wiley and Sons Ltd, Chichester, 2010, pp M. -J. Wang, C.A. Gray, S.R. Reznek, K. Mahmud, Y. Kutsovsky, Carbon Black, in: J. Kroschwitz (Ed.), Encyclopedia of Polymer Science and Technology, John Wiley & Sons, Inc., New York, 2002.
49 Introduction G. Kuhner, M. Voll, Manufacture of carbon black, in: D. Jean-Baptiste, R.C. Bansal, M.-J. Wang (Eds.), Carbon black: science and technology, CRC Press, Boca Raton, W.R. Jones, Reactor and method for production of carbon black with broad particle size distrtibution EP A2 (1989). 16. Columbian Carbon (Spain) personal communication. 17. Committee on Alternatives and Strategies for Future Hydrogen Production and Use, National Research Council, The Hydrogen Economy: Opportunities, Costs, Barriers, and R&D Needs, National Academies Press, N.W. Ockwig, T.M. Nenoff, Membranes for hydrogen separation, Chem. Rev. 107 (2007) W.J. Koros, D.G. Woods, Elevated temperature application of polymer hollowfiber membranes, J. Membr. Sci. 181 (2001) T.C. Merkel, M. Zhou, R.W. Baker, Carbon dioxide capture with membranes at an IGCC power plant, J. Membr. Sci. 389 (2012) The National Energy Technology Laboratory, U.S. Department of Energy, Hydrogen from Coal Program Central Production RD&D, (2012). 22. M. Ramezan, T.J. Skone, N. Nsakala, G.N. Liljedahl, Carbon Dioxide Capture from Existing Coal-Fired Power Plants DOE/NETL-401/ (2007). 23. J.R. Rostrup-Nielsen, Syngas in perspective, Catal. Today 71 (2002) National Energy Technology Laboratory, U.S. Department of Energy, Gasification encyclopedia, gasifiers/index.html (2012). 25. S.P. Kaldis, G.C. Kapantaidakis, G.P. Sakellaropoulos, Simulation of multicomponent gas separation in a hollow fiber membrane by orthogonal collocation - Hydrogen recovery from refinery gases, J. Membr. Sci. 173 (2000) D.L. Maclean, R. Krishnamurthy, S.L. Lerner, Argon recovery from hydrogen depleted ammonia plant purge gas utilizing a combination of cryogenic and noncryogenic separation means Patent US (1987). 27. J. Yang, C.-H. Lee, Adsorption dynamics of a layered bed PSA for H2 recovery from coke oven gas, AIChE J. 44 (1998)
50 34 Chapter I 28. W.J. Koros, R.T. Chern, Separation of Gaseous Mixtures Using polymer Membranes, in: R.W. Rousseau (Ed.), Handbook of Separation Process Technology, John Wiley & Sons, New York, 1987, pp P. Pandey, R.S. Chauhan, Membranes for gas separation, Progr. Polym. Sci. 26 (2001) M. Mulder, Basic Principles of Membrane Technology, Kluwer Academic Publishers, Dordrecht, D.W. Breck, Zeolite Molecular Sieves: Structure, Chemistry, and Use, John Wiley & Sons, New York, R.W. Baker, K. Lokhandwala, Natural gas processing with membranes: An overview, Ind. Eng. Chem. Res. 47 (2008) C.A. Scholes, S.E. Kentish, G.W. Stevens, Effects of minor components in carbon dioxide capture using polymeric gas separation membranes, Sep. Purif. Rev. 38 (2009) J.A. Dean, Lange's Handbook of Chemistry, 15th ed., McGraw-Hill, New York, L.M. Robeson, The upper bound revisited, J. Membr. Sci. 320 (2008) L.M. Robeson, Correlation of separation factor versus permeability for polymeric membranes, J. Membr. Sci. 62 (1991) N. Du, G.P. Robertson, J. Song, I. Pinnau, M.D. Guiver, High-performance carboxylated polymers of intrinsic microporosity (PIMs) with tunable gas transport properties, Macromolecules 42 (2009) W. Fang, L. Zhang, J. Jiang, Gas permeation and separation in functionalized polymers of intrinsic microporosity: A combination of molecular simulations and ab initio calculations, J. Phys. Chem. C 115 (2011) B.S. Ghanem, N.B. McKeown, P.M. Budd, N.M. Al-Harbi, D. Fritsch, K. Heinrich, L. Starannikova, A. Tokarev, Y. Yampolskii, Synthesis, characterization, and gas permeation properties of a novel group of polymers with intrinsic microporosity: PIM-polyimides, Macromolecules 42 (2009) I. Pinnau, S. Thomas, M.D. Guiver, N. Du, J. Song, Gas transport properties of intrinsically microporous polymers, ACS National Meeting Book of Abstracts (2009). 41. J. Peter, A. Khalyavina, J. Kříž, M. Bleha, Synthesis and gas transport properties of ODPA-TAP-ODA hyperbranched polyimides with various comonomer ratios, Eur. Polym. J. 45 (2009)
51 Introduction D.M. Sterescu, D.F. Stamatialis, M. Wessling, Boltorn-modified polyimide gas separation membranes, J. Membr. Sci. 310 (2008) V. Arcella, A. Ghielmi, G. Tommasi, High performance perfluoropolymer films and membranes, Ann. N. Y. Acad. Sci. 984 (2003) N.A. Belov, A.A. Zharov, A.V. Shashkin, M.Q. Shaikh, K. Raetzke, Y. Yampolskii, Gas transport and free volume in hexafluoropropylene polymers, J. Membr. Sci. 383 (2011) P. Gorgojo, S. Uriel, C. Téllez, J. Coronas, Development of mixed matrix membranes based on zeolite Nu-6(2) for gas separation, Micropor. Mesopor. Mat. 115 (2008) M. Askari, Y. Xiao, P. Li, T.-. Chung, Natural gas purification and olefin/paraffin separation using cross-linkable 6FDA-Durene/DABA co-polyimides grafted with α, β, and γ-cyclodextrin, J. Membr. Sci (2012) M.G. García, J. Marchese, N.A. Ochoa, High activated carbon loading mixed matrix membranes for gas separations, J. Mater. Sci. (2011) J.E. Mark, Polymer Data Handbook, 2nd ed., Oxford University Press, Oxford, C.J. Orme, M.L. Stone, M.T. Benson, E.S. Peterson, Testing of polymer membranes for the selective permeability of hydrogen, Sep. Sci. Technol. 38 (2003) V. Abetz, T. Brinkmann, M. Dijkstra, K. Ebert, D. Fritsch, K. Ohlrogge, D. Paul, K.-. Peinemann, S.P. Nunes, N. Scharnagl, M. Schossig, Developments in membrane research: From material via process design to industrial application, Adv. Eng. Mater. 8 (2006) Y. Li, T.-S. Chung, Highly selective sulfonated polyethersulfone (SPES)-based membranes with transition metal counterions for hydrogen recovery and natural gas separation, J. Membr. Sci. 308 (2008) D. Wang, W.K. Teo, K. Li, Permeation of H2, N2, CH4, C2H6, and C3H8 through asymmetric polyetherimide hollow-fiber membranes, J. Appl. Polym. Sci. 86 (2002) P. Hacarlioglu, L. Toppare, L. Yilmaz, Polycarbonate-polypyrrole mixed matrix gas separation membranes, J. Membr. Sci. 225 (2003) S.S. Hosseini, M.M. Teoh, T.-S. Chung, Hydrogen separation and purification in membranes of miscible polymer blends with interpenetration networks, Polymer 49 (2008)
52 36 Chapter I 55. S.C. Kumbharkar, P.B. Karadkar, U.K. Kharul, Enhancement of gas permeation properties of polybenzimidazoles by systematic structure architecture, J. Membr. Sci. 286 (2006) H. Kawakami, M. Mikawa, S. Nagaoka, Gas permeability and selectivity through asymmetric polyimide membranes, J. Appl. Polym. Sci. 62 (1996) S. Shishatskiy, C. Nistor, M. Popa, S.P. Nunes, K.V. Peinemann, Polyimide asymmetric membranes for hydrogen separation: Influence of formation conditions on gas transport properties, Adv. Eng. Mater. 8 (2006) B.T. Low, T.-S. Chung, H. Chen, Y.-. Jean, K.P. Pramoda, Tuning the free volume cavities of polyimide membranes via the construction of pseudo-interpenetrating networks for enhanced gas separation performance, Macromolecules 42 (2009) B.T. Low, Y. Xiao, T.-S. Chung, Amplifying the molecular sieving capability of polyimide membranes via coupling of diamine networking and molecular architecture, Polymer 50 (2009) S.S. Hosseini, N. Peng, T.-S. Chung, Gas separation membranes developed through integration of polymer blending and dual-layer hollow fiber spinning process for hydrogen and natural gas enrichments, J. Membr. Sci. 349 (2010) G. Kung, L.Y. Jiang, Y. Wang, T.-S. Chung, Asymmetric hollow fibers by polyimide and polybenzimidazole blends for toluene/iso-octane separation, J. Membr. Sci. 360 (2010) S.S. Hosseini, T.-S. Chung, Carbon membranes from blends of PBI and polyimides for N2/CH4 and CO2/CH4 separation and hydrogen purification, J. Membr. Sci. 328 (2009) E. Földes, E. Fekete, F.E. Karasz, B. Pukánszky, Interaction, miscibility and phase inversion in PBI/PI blends, Polymer 41 (2000) F. Wu, L. Li, Z. Xu, S. Tan, Z. Zhang, Transport study of pure and mixed gases through PDMS membrane, Chem. Eng. J. 117 (2006) T.-S. Chung, L. Shao, P.S. Tin, Surface modification of polyimide membranes by diamines for H2 and CO2 separation, Macromol. Rapid Comm. 27 (2006) S.S. Dhingra, E. Marand, Mixed gas transport study through polymeric membranes, J. Membr. Sci. 141 (1998) W.J. Koros, R.T. Chern, V. Stannett, H.B. Hopfenberg, Model for permeation of mixed gases and vapors in glassy polymers., J. Polym. Sci., Part A-2: Polym. Phys. 19 (1981)
53 Introduction C.A. Koval, R.D. Noble, J.D. Way, B. Louie, Z.E. Reyes, B.R. Bateman, G.M. Horn, D.L. Reed, Selective transport of gaseous CO through liquid membranes using an iron(ii) macrocyclic complex, Inorg. Chem. 24 (1985) G.S. Patil, S. Baruah, N.N. Dutta, Facilitated transport of carbon monoxide: A review, Gas Sep. Purif. 5 (1991) National Energy Technology Laboratory (NETL), U.S. Department of Energy, 2010 Worldwide gasification database, ex.html. (2012) 71. J.L. Anthony, J.L. Anderson, E.J. Maginn, J.F. Brennecke, Anion effects on gas solubility in ionic liquids, J. Phys. Chem. B 109 (2005) J. Kumełan, A.P.S. Kamps, D. Tuma, G. Maurer, Solubility of CO in the ionic liquid [bmim][pf6], Fluid Phase Equilib (2005) C.A. Ohlin, P.J. Dyson, G. Laurenczy, Carbon monoxide solubility in ionic liquids: Determination, prediction and relevance to hydroformylation, Chem. Comun. 10 (2004) J. Bierhals, Carbon Monoxide, in: Ullmann's Encyclopedia of Industrial Chemistry, Wiley-VCH, Weinheim, A.J. Hernández-Maldonado, R.T. Yang, Desulfurization of transportation fuels by adsorption, Catal. Rev. Sci. Eng. 46 (2004) R.T. Yang, π-complexation sorbents and applications, in: Adsorbents: Fundamentals and Applications, John Wiley & Sons, Inc., Hoboken, New Jersey, 2003, pp D.J. Safarik, R.B. Eldridge, Olefin/paraffin separations by reactive absorption: a review, Ind. Eng. Chem. Res. 37 (1998) T.A. Reine, Olefin/paraffin separation by reactive absorption, PhD dissertation, University of Texas at Austin (2004). 79. A. Ortiz, L.M. Galán, D. Gorri, A.B. De Haan, I. Ortiz, Kinetics of reactive absorption of propylene in RTIL-Ag+ media, Sep. Purif. Technol. 73 (2010) C.J. King, Separation processes based on reversible chemical complexation, in: R.W. Rousseau (Ed.), Handbook of Separation Process Technology, Wiley - Interscience, New York, 1987, pp R.D. Noble, C.A. Koval, Review of facilitated transport membranes, in: Y. Yampolskii, I. Pinnau, B.D. Freeman (Eds.), Materials Science of Membranes, Wiley, West Sussex, 2006, pp. 411.
54 38 Chapter I 82. R.D. Noble, C.A. Koval, J.J. Pellegrino, Facilitated transport membrane systems, Chem. Eng. Prog. 85 (1989) M.F. San Román, E. Bringas, R. Ibañez, I. Ortiz, Liquid membrane technology: Fundamentals and review of its applications, J. Chem. Technol. Biotechnol. 85 (2010) P. Luis, L.A. Neves, C.A.M. Afonso, I.M. Coelhoso, J.G. Crespo, A. Garea, A. Irabien, Facilitated transport of CO2 and SO2 through Supported Ionic Liquid Membranes (SILMs), Desalination 245 (2009) D.R. Smith, J.A. Quinn, Facilitated transport of carbon monoxide through cupprous chloride solutions., AIChE J. 26 (1980) A. Dindi, R.D. Noble, J. Yu, C.A. Koval, Experimental and modeling studies of a parasitic binding mechanism in facilitated membrane transport, J. Membr. Sci. 66 (1992) J.A. Hogendoorn, W.P.M. van Swaaij, G.F. Versteeg, The absorption of carbon monoxide in COSORB solutions: absorption rate and capacity, Chem. Eng. J. Biochem. Eng. J. 59 (1995) M. Junidi, O. Munchise, K. Osama, New carrier systems for separation of carbon monoxide, Mitsubishi Kasei R&D Review 6, (1) (1992) H.C. Fry, H.R. Lucas, A.A.N. Sarjeant, K.D. Karlin, G.J. Meyer, Carbon monoxide coordination and reversible photodissociation in copper(i) pyridylalkylamine compounds, Inorg. Chem. 47 (2008) C.S. Sharma, P.K. Goswami, N.N. Dutta, Studies on facilitated transport of carbon monoxide using a novel iron(ii) complex, Sep. Sci. Technol. 28 (1993) S.E. Lyke, M.A. Lliga, R.M. Ozanich, D.A. Nelson, B.R. James, C.-. Lee, Separation of syngas components using a dissolved palladium complex, Ind. Eng. Chem. Prod. Res. Dev. 25 (1986) G.W. Meindersma, M. Maase, A.B. De Haan, Ionic Liquids, in: Ullmann's Encyclopedia of Industrial Chemistry, Wiley-VCH Verlag GmbH & Co. KGaA, P. Wasserscheid, T. Welton, Ionic Liquids in Synthesis, 2nd ed., Wiley, New York, T. Welton, Room-Temperature Ionic Liquids. Solvents for Synthesis and Catalysis, Chem. Rev. 99 (1999) J.P. Hallett, T. Welton, Room-temperature ionic liquids: Solvents for synthesis and catalysis. 2, Chem. Rev. 111 (2011)
55 Introduction A. Stark, K.R. Seddon, Ionic Liquids, in: Kirk-Othmer Encyclopedia of Chemical Technology, John Wiley & Sons, Inc., L.C. Branco, G.V.S.M. Carrera, J. Aires-de-Sousa, I. Lopez Martin, R. Frade, C.A.M. Afonso, Physico-Chemical Properties of Task-Specific Ionic Liquids, in: A. Kokorin (Ed.), Ionic Liquids: Theory, Properties, New Approaches, InTech, 2011, pp G. Laus, G. Bentivoglio, H. Schottenberger, V. Kahlenberg, H. Kopacka, T. Röder, S. Sixta, Ionic Liquids: Current developments, potential and drawbacks for industrial applications, Lenzinger Berichte 84 (2005) M. Freemantle, Designer solvents, Chem. Eng. News 76 (1998) R.D. Rogers, K.R. Seddon, Ionic Liquids - Solvents of the Future?, Science 302 (2003) S.A. Shamsi, N.D. Danielson, Utility of ionic liquids in analytical separations, J. Sep. Sci. 30 (2007) D. Bankmann, R. Giernoth, Magnetic resonance spectroscopy in ionic liquids, Prog. Nucl. Magn. Reson. Spectrosc. 51 (2007) S. Pandey, Analytical applications of room-temperature ionic liquids: A review of recent efforts, Anal. Chim. Acta 556 (2006) M. Koel, Ionic liquids in chemical analysis, Crit. Rev. Anal. Chem. 35 (2005) T.D. Ho, A.J. Canestraro, J.L. Anderson, Ionic liquids in solid-phase microextraction: A review, Anal. Chim. Acta 695 (2011) F. van Rantwijk, R.A. Sheldon, Biocatalysis in ionic liquids, Chem. Rev. 107 (2007) R. Hagiwara, J.S. Lee, Ionic liquids for electrochemical devices, Electrochemistry 75 (2007) D.S. Silvester, Recent advances in the use of ionic liquids for electrochemical sensing, Analyst 136 (2011) M.-. Bermúdez, A.-. Jiménez, J. Sanes, F.J. Carrión, Ionic liquids as advanced lubricant fluids, Molecules 14 (2009) H. Zhao, Innovative applications of ionic liquids as "green" engineering liquids, Chem. Eng. Commun. 193 (2006) F. Zhou, Y. Liang, W. Liu, Ionic liquid lubricants: Designed chemistry for engineering applications, Chem. Soc. Rev. 38 (2009)
56 40 Chapter I 112. L.J. Lozano, C. Godínez, A.P. de los Ríos, F.J. Hernández-Fernández, S. Sánchez- Segado, F.J. Alguacil, Recent advances in supported ionic liquid membrane technology, J. Membr. Sci. 376 (2011) A.B. Pereiro, J.M.M. Araújo, J.M.S.S. Esperana, I.M. Marrucho, L.P.N. Rebelo, Ionic liquids in separations of azeotropic systems - A review, J. Chem. Thermodyn. 46 (2012) H. Tadesse, R. Luque, Advances on biomass pretreatment using ionic liquids: An overview, Energy Environ. Sci. 4 (2011) A. Berthod, M.J. Ruiz-Ángel, S. Carda-Broch, Ionic liquids in separation techniques, J. Chromatogr. A 1184 (2008) L. Vidal, M.-. Riekkola, A. Canals, Ionic liquid-modified materials for solid-phase extraction and separation: A review, Anal. Chim. Acta 715 (2012) M. Kumar, N. Trivedi, C.R.K. Reddy, B. Jha, Toxic effects of imidazolium ionic liquids on the green seaweed Ulva lactuca: Oxidative stress and DNA damage, Chem. Res. Toxicol. 24 (2011) M. Alvarez-Guerra, A. Irabien, Design of ionic liquids: An ecotoxicity (Vibrio fischeri) discrimination approach, Green Chem. 13 (2011) J. Arning, M. Matzke, Toxicity of ionic liquids towards mammalian cell lines, Curr. Org. Chem. 15 (2011) BASF, BASIL processes, (2012).
57 Chapter II MIXED GAS SEPARATION STUDY FOR THE HYDROGEN RECOVERY FROM H 2 /CO/N 2 /CO 2 POST COMBUSTION MIXTURES USING A MATRIMID MEMBRANE
58 42 Chapter II
59 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid membrane 43 ABSTRACT In this chapter, the membrane based separation of hydrogen from binary, ternary and quaternary mixtures of H2, N2, CO and CO2 is presented. Gas permeability values through a polyimide Matrimid 5218 membrane were experimentally obtained using a permeation technique at a constant pressure. Dense films were fabricated by solution casting of polymer solutions in dichloromethane using two methods: casting knife and Petri dishes. The influence of the feed gas composition, temperature ( o C), pressure (2-6 bar), and sweep gas flow rates on the permeation of gases through the prepared membranes was experimentally analyzed. As expected, the pure gas permeability of H2 was only slightly dependant on pressure and had an average value of 24 Barrer at 30 o C. Hydrogen permeability was not affected by the presence of nitrogen and carbon monoxide, and as a result the mixed gas selectivities for the H2/N2/CO mixtures are very close to the ideal selectivities calculated from pure gas permeation data. On the contrary, a strong dependency of the hydrogen permeability on CO2 concentration was observed even at low concentrations of CO2. A reduction of 42 % of the hydrogen permeability coefficient was obtained when a mixture of 10/90 vol % H2/CO2 was used as feed gas. Accordingly H2/CO2 selectivity decayed from a value of 4.2 calculated from pure gas permeabilities to 2.7 when permeation data were obtained in mixed gas experiments. The preferential sorption of CO2 on the Langmuir sites of the excess free volume portion of the polymer allowed explaining and quantifying this phenomenon. The dual-mode sorption, partial immobilization model was used to describe H2 and CO2 permeation behavior of pure, binary, ternary and quaternary mixtures. The model sorption parameters for N2 and CO2 in the polymer Matrimid 5218 were obtained from the literature meanwhile those for H2 and for CO were unknown and resulted from the fitting of the experimental data to the proposed model. Satisfactory agreement between predicted permeability results and experimental data with a correlation coefficient (R) higher than 0.95 and mean squared relative error (MSRE) lower than 0.01 was attained. Thus, this chapter reports useful knowledge related to the intrinsic material properties, considering gas mixtures of industrial interest and essential when other membrane configurations like hollow fibers, mixed matrix membranes or polymer blends are proposed.
60 44 Chapter II 2.1 THE DUAL-MODE SORPTION, PARTIAL IMMOBILIZATION THEORY Gas sorption and diffusion in glassy polymeric membranes has been described by several established models but the use of the dual-mode sorption, partial immobilization theory has been more prevalent . This model originally proposed by Barrer et al.  has been extended by Michaels el al. , Paul et al. , Koros et al.  and many others. According to the dual-mode sorption model, gas sorption (Cm) in a polymer occurs in two types of sites, Henry and Langmuir sites respectively. The first type is filled by gas molecules dissolved in the equilibrium free volume portion of the material (concentration CD) and the second one corresponds to the population dissolved in the excess free volume of the glassy polymer (CH) . 1 II 1 1 II 2 here, p (bar) is the pressure and kd (cm 3 (STP)/cm 3 /bar) represents the Henry law constant. c H (cm 3 (STP)/cm 3 /bar) is the Langmuir capacity constant and characterizes the total sorption capacity of the lower density regions (unrelaxed gaps) in a glassy polymer for a particular penetrant. The parameter b (1/bar) is the Langmuir affinity constant which characterizes the tendency of a given penetrant to sorb in the Langmuir mode. The affinity constants for non-condensable penetrants such as helium and hydrogen are small, while more easily condensable polar and polarizable penetrants such as carbon dioxide tend to have significantly larger affinity constants . The dual-mode theory has been extended to multicomponent gas mixtures and is presented in Equation II 3 : 1 II 3 The primary effect for a mixture is the simple competition by the various penetrants for the excess free volume fraction of the polymer which causes a significant depression in the sorption of all components of the mixture .
61 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid membrane 45 All the parameters in Equation II - 3 are for pure components. They are obtained from sorption isotherms of pure gases in glassy polymers. Their use for predicting mixture sorption assumes to be negligible the plasticizing effects over kd, penetrant - penetrant interactions influences on both bi and c H, and bulk flow phenomena. As a consequence of the existence of two types of adsorption sites in glassy polymeric membranes two diffusion coefficients can be defined. DD is used for the mobility of the gas population dissolved in the equilibrium free volume of the polymer and DH for the mobility of the gas population contained in the excess free volume. Then, the Fick s law expression for flux (J) through the membrane has the form: II 4 rearranged to 1 II 5 The ratio DH/DD can be grouped as follows: II 6 were F can be viewed as the moving fraction of the Langmuir s population. Then, 1 II 7 The substitution of Equation II - 1, the ratio dch/dcd gives:
62 46 Chapter II II 8 CH, b and kd can be grouped as follows: II 9 where K is a concentration sorption parameter. The substitution of Equation II 8 and II 9 into Equation II 7 gives: 1 1 II 10 the integration from the high pressure side to the low pressure side across the membrane, leads to the expression of permeability expressed by Equation II - 11, which is valid when DD and DH are constant and the downstream pressure is negligible . 1 II 11 1 For mixed gas permeation expressions analogous to Equation II - 11 can be obtained for any number of additional components in the feed : 1 1 II 12 Alternatively, Equation II - 12 can be expressed in terms of component fugacity rather than partial pressures. The use of penetrant fugacity is clearly preferred as non-ideal gas phase mixture effects can be easily accounted for .
63 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid membrane II 13 In Equation II - 13 the solubility parameters c H, b, k D, are those of pure gases and are based on pressure not on pure gas fugacity because the differences are rather small . By fitting Equation II - 13 with mixed gas experimental data of permeability versus fugacity of the gaseous phase, one can obtain diffusivities for the Henry s law and Langmuir mode. The final expression of the dual-mode sorption, partial immobilization model (Equation II 13) shows this empirical model as an easy to use tool for the estimation of pure and mixed gas permeability data variation with pressure. Other semiempirical approaches have been proposed, using group contribution methods , a modified activity coefficient approach , or suggestions derived from molecular thermodynamic considerations . Unfortunately, all of them do not allow any reliable predictive evaluation  THE NON-EQUILIBRIUM LATTICE FLUID NELF MODEL A reliable tool to estimate the mixed gas solubility in glassy polymers, in the common case in which such data are not experimentally available for the system of interest, has proven to be the NELF model developed by Sarti et al. [13-15]. The NELF model enables to calculate the solubility isotherms in glassy polymers, on the basis of the results on non equilibrium thermodynamics of glassy polymers. It offers an explicit relationship between penetrant fugacity on one hand, and penetrant solubility in the polymer and the glassy polymer density on the other hand. Thus it accounts for the strong and important relationship existing between the solubility and fractional free volume in the glassy phase. The NELF model adopts the Lattice Fluid representation of pure substances and their mixtures [16-19]. A two dimensional representation of the Lattice Fluid model description of a hexamer is given in Figure II - 1. There are multiple configurations available to a system of N molecules each of which occupies r sites (an r mer) and N0 vacant sites (holes). A random mixing of the r mers which each other and with the vacant sites is assumed.
64 48 Chapter II Figure II 1. A two-dimensional example of a pure lattice fluid. Hexamers are distributed over the lattice, but not all sites are occupied . The NELF model extend the Sanchez Lacombe equation of state for amorphous phases to the non equilibrium domain typical of glassy polymers, using the same parameters to represent the pure components properties and the same mixing rules to calculate the mixture behavior. For all the penetrants, these parameters can be determined using either PVT (pressure- volume temperature) data or vapor liquid equilibrium data, while for the polymers they are usually calculated by fitting the PVT data above TG with the Sanchez Lacombe equation of state EXPERIMENTHAL METHODOLOGY Materials The commercial polymer Matrimid 5218 (polyimide of 3,3, 4,4 benzophenone tetracarboxylic dianhydride and diamino-phenylidane) was kindly provided by Huntsman Advanced Polymers in powder form. Dichloromethane (CH2Cl2) (Panreac) solvent was used as received for the preparation of the polymer solutions. Gases were purchased from Air Liquide (Spain) with a purity of at least %.
65 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post 49 combustion mixtures using a Matrimid membrane Preparation of dense planar Matrimid polymeric membranes Dense planar polymeric membranes (Figure II 2) with thickness ranging from 30 to 50 μm were prepared by solution casting according to two procedures, described as follows: Figure II 2. Image of a typical Matrimid dense film prepared in this work (A) Using a casting knife (Elcometer see Figure II 3): 1. Polymer powder drying under complete vacuum at 120oC for at least 12 h (Selecta vacuum oven). 2. Preparation of polymeric solutions of 20 cm3 of 15 wt % under continuous stirring of the polymer powder with CH2Cl2 as solvent for at least 24 h. 3. Solution casting on a glass plate using a casting knife (Elcometer 3580) of thin wet films. The gap between the blade of the casting knife and the glass plate was from 0.2 to 0.5 mm. 4. Drying of the cast films at room temperature in a covered box for 24 h under a continuous flow of N2 in order to prevent phase inversion by water absorption from air. 5. Removing of the homogeneous dense films from the glass plate by rinsing with a small amount of water and further drying in a vacuum oven (Selecta Vacioterm-T) at 120 oc for 24 hours and 200 mbar in order to eliminate the remaining solvent. 6. Cutting off the membrane in circular shape with a diameter of 4.45 cm
66 50 Chapter II Figure II 3. The Elcometer casting knife used for the preparation of polymeric dense films (B) Using a Petri dish 1. Polymer powder drying under vacuum at 120 o C for at least 12 h (Selecta vacuum oven). 2. Preparation of polymeric solutions concentrations (Csol) of 3 5 wt % under continuous mixing of the polymer powder with CH2Cl2 as solvent for at least 24 h. The needed solution volume (Vsol) for one Petri dish with the diameter d, depends on the thickness desired for the dry film and is estimated according to the following formula: Vsol = (πd 2 /4) (δdry/csol) (II - 14) 3. Filtration with a syringe driven filter unit (Millipore hydrophobic PTFE 0.2 µm) and concomitant solution casting on a Petri dish (9.5 cm diameter) of thin wet films. 4. Drying of the cast films at room temperature in a covered box for 24 h under a continuous flow of N2 in order to prevent phase inversion by water absorption from air. The steps 5. and 6. similar to the previous procedure. The polymer solutions used for solution casting with a casting knife had 15 % wt polymer concentration because sufficiently viscous solution is needed in order to prevent it from running over the central part. Because of the extra filtration step the films prepared using Petri dishes had in general a better morphology. Polymeric solutions are not entirely homogeneous and even after large periods of mixing they still contain non-solved polymer particles, thus the importance of filtration before casting. The only drawback in using Petri dishes is that polymer solution can adhere to the walls determining a variation in the thickness of the circular shape film, i. e. thinner in the middle and thicker toward the
67 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid membrane 51 edge. Membranes with a constant thickness where obtained using large Petri dishes by cutting of the membrane from the middle of the film. In general the optimum membrane thickness was experienced to be around 30 µm and membrane thickness should not exceed 50 µm when Matrimid polyimide is used as membrane material. CH2Cl2 is a good, but highly volatile solvent with a normal boiling point of 40 o C. The rapid evaporation of the solvent makes the preparation of homogenous films difficult, i. e. it cools the casting solution, causing gelation of the polymer. The result is a film with a mottled, orange-peel-like surface . When membranes were prepared using the casting knife, smooth films were obtained by covering the cast films with a glass plate raised 1 cm above the film to slow down the evaporation of the solvent. When membranes where prepared using Petri dishes, those were closed with their own cover.a less volatile solvent can be used also. Table II 1 list the boiling points and hazard information for solvents in which Matrimid has a good solubility at 20 wt % as stated in the data sheet provided by the polymer producer (see Appendix I). Table II 1. Matrimid solvents boiling points and hazard information Solvent Boling Point ( o C) Hazards Dichloromethane 39.6 R40 Ethylene chloride R11, R45, R36/37/38, Chloroform 61.2 R22, R38, R40, R48/20/22 Tetrachloroethane possible human carcinogen  Tetrahydrofurane (THF) 66 R11, R19, R39/37 1, 4 Dioxane R11, R19, R36/37, R40, R66 Acetophenone 202 Harmful (Xn) Cyclohexanone R10, R20, m Cresol R20, R24, R25, R34, γ Butyrolactone 204 R22, R36, Dimethylformamide (DMF) 153 R61, R20/21, R36 Dimethylacetamide (DMAc) R61, R20/21 N methylpirolidone (NMP) R36/37/38, R61 R10: Flammable, R11: Highly flammable, R19: May form explosive peroxides, R20: Harmful by inhalation, R22: Harmful if swallowed, R24: Toxic in contact with skin, R25: Toxic if swallowed, R34: Causes burns, R36: Irritating to eyes, Irritating to skin, R40: Limited evidence of a carcinogenic effect, R61: May cause harm to the unborn child, R66: Repeated exposure may cause skin dryness or cracking, R20/21: Harmful by inhalation and in contact with skin, R36/37: Irritating to eyes and respiratory system, R36/37/38: Irritating to eyes, respiratory system and skin, R48/20/22: Harmful: danger of serious damage to health by prolonged exposure through inhalation and if swallowed.
68 52 Chapter II The Risk phrases listed in Table II 1 are defined in the Appendix III of European Union Directive 67/548/EEC. Taken into account hazard considerations, from all the possible solvents, the more appropriate and already used in literature for Matrimid membrane manufacture are underlined. When solvents with high boiling points are used, prolonged drying step is needed (up to 2 weeks in vacuum oven at 100 o C for NMP). Also, in order to obtain a defect free membrane, the mixture of two solvents with high and low boiling points can be done Membrane characterization The membrane thickness was measured using a digital micrometer Mitutoyo Digmatic Series 369 (accuracy ± mm) (see Figure II - 4). This micrometer is equipped with two plates of 2 mm diameter specially designed to measure thin films. The resulted values of thickness represent an average of five measurements, one in the center of the membrane and four in the borders. Thickness deviations from the average did not exceed 2 µm in any of the membranes used. Figure II 4. The digital micrometer used for the measurement of membranes thickness In order to check the complete evaporation of the solvent, thermogravimetric analysis ( o C, 10 o C/min) were performed to film samples before and after vacuum oven drying using a Shimatzu Scientific DTG 60H equipment. Figure II -5 shows that before vacuum drying the membranes contain some residual solvent having an 8.5 wt % loss at 350 o C. The vacuum oven treated sample (Figure II 6) had a 1 wt % mass loss at 350 o C and 68.4 wt % at 600 o C. Considering the Matrimid polymer Tg value of o C it can be concluded that no residual solvent was left in the polymer sample and that the membrane manufacturing procedure was correct.
69 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid membrane 53 Figure II 5. Thermal gravimetric analysis report for a Matrimid film sample before vacuum oven drying step Figure II 6. Thermal gravimetric analysis report for a Matrimid film sample after vacuum oven drying step
70 54 Chapter II Mixed gas separation set - up Figure II - 7 shows a schematic diagram of the experimental permeation set-up and Figure II 8 shows a photographic image taken from the experimental set - up. The design of the feed part of the set-up confers the possibility of performing pure and mixed (binary, tertiary and quaternary) gas permeation experiments, at predetermined gas concentrations and flow rate levels. The desired concentration of each component of the mixture is obtained by controlling its flow rate by means of mass flow controllers (Brooks 5850S), with a 100 cm 3 (STP) min -1 upper limit for the total flow rate. These mass flow controllers present a flow accuracy of 0.9 % at full scale. At 5 % of the full scale the error is 4.7 %. The gas mixture flows over the polymeric membrane film mounted in the membrane test cell and leaves the system via the backpressure regulator (Brooks 5866), which controls the total pressure in the feed side of the membrane. In the permeate side the total pressure is maintained at atmospheric level. The gas permeates through the membrane material and is removed by an argon sweep gas. The flow rate of the sweep gas was controlled with a mass flow controller (Brooks 5850S), with a 10 cm 3 (STP) min -1 full scale and the same characteristic accuracies as the previous ones. The concentration (vol %) of each component in the sweep gas stream leaving the permeate side of the cell is determined via gas chromatography (Agilent Micro GC 3000) equipped with a thermal conductivity detector. The GC is suited with two columns, 1) molecular sieve 5A for H2, CO and N2 separation, that employs Ar as carrier gas, and 2) PLOT U for CO2 separation, that employs He as carrier gas. Ar was used as carrier and sweep gas instead of the cheaper He because He has a similar thermal conductivity with H2 and therefore H2 cannot be measured by the chromatograph detector in the presence of He. Due to the differences in concentration at the permeate side of the membrane two chromatographic methods were developed: one for the fast permeating gases i.e. H2 and CO2 and the other for the slow permeating gases i.e. N2 and CO. The only difference between these two methods is the injection time which is 20 times higher in the method used for CO and N2 analysis; this allows a higher accuracy at low concentrations. Therefore, the error associated to the chromatographic analysis was minimized and the coefficient of variation calculated from peak area deviations of calibration samples was less than 0.4%. A detailed description of the chromatographic methods is found in Appendix II.
71 Figure II 7. The experimental permeation set up with a detailed view of the permeation cell, (A) Mass flow controller; (B) Control box; (C) Heating oven; (D) Membrane test cell; (E) backpressure regulator; (F) Mass flowmeter, (G) Gas chromatograph Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post 55 combustion mixtures using a Matrimid membrane
72 56 Chapter II Figure II 8. The photographic image of the experimental permeation set up with the heating oven open for a better viewing of the testing cell. The polymeric film to be characterized is inserted in the permeation test cell (see scale drawings in Appendix III) that includes a porous metallic plate (Mott Corp OD = 1.750, ID =0.125, media grade= 20, material 316LSS) as support and a filter paper that prevents scratching of the membrane by the metallic support. The membrane test-cell is thermostatized into a heating oven (Memmert Excel). The membrane is cut off from the dried polymeric film in circular shape and after the insertion in the membrane test cell it results an effective membrane area of cm 2. The two compartments of the permeation cell are sealed with O-rings (Viton). Before starting a series of experiments a vacuum pump was used to evacuate the whole test cell from undesired species for at least half an hour. Tests were conducted at specific conditions until constant steady-state values of permeate flux and composition were reached and the permeate, retentate and feed streams remained unchanged for at least 1 h. During this period the concentration of each component was analyzed at least five times. When a series of experiments were run several times the standard deviation is illustrated in the graphics as bars.
73 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid membrane 57 For pure and mixed gas experiments, permeabilities were calculated using Equation II - 15, A Δ II 15 where Qi is the permeate flow rate for the component i, δ is the membrane thickness, A is the membrane area, Δpi is the component i partial pressure gradient through the membrane. Δpi is equal to the partial pressure in the feed side considering a null value of the partial pressure in the permeate side. The permeate flow rate value was determined by multiplying the experimental concentration of component i (vol %) in the permeate times the Ar sweep gas flow rate. Data were fitted to the model by using fugacities instead of partial pressures (Equation II 13). Fugacities of the components were calculated using the Peng-Robinson equation  for each experimental point at the particular experimental conditions of temperature and total pressure Experimental procedure and operation conditions Pure gas permeation experiments were performed in order to obtain and compare the permeation results with literature data and in this way to assure the reliability of the testing system, and also to have a benchmark for the mixed gas results at 30 o C and three operational pressures, 2, 4 and 6 bar. The sweep gas flow rate was varied in order to determine the occurrence of concentration polarization phenomena in the permeate side of the membrane and in this way to select the minimum value of this variable that permits to avoid secondary effects when analyzing permeance data. For these experiments, a membrane of 47.8±2 µm thickness was used. Then, the temperature dependency of the permeability coefficients for H2, CO2, CO and N2 was determined experimentally. Measurements were made for each gas at five or six different temperatures in the range o C, and a feed pressure of 4 bar using the membrane of 47.8±2 µm thickness for H2 and CO2 and of 28.9±2 µm thickness for CO and N2. Steady-state values of permeate flux were obtained overnight and the permeability of gases at the specific temperatures was determined in consecutive days.
74 58 Chapter II Finally, experiments with binary, ternary and quaternary gas mixtures of H2, N2, CO and CO2 were performed at composition and operation experimental conditions listed in Table II 2 at feed flow rates of 100 cm 3 (STP) min -1 and sweep gas flow rates of 6 cm 3 (STP) min -1. Table II 2. Gas composition and operation experimental conditions for mixed gas experiments. Mixture ID Composition (vol %) Pressure (bar) Temperature ( o C) H 2/N 2 2, 3, 4, 5, 10, 30, 50, ±2 of H 2 in N 2 H 2/CO 2 10, 30, 50, 70, 90 4, ±2 of H 2 in CO 2 H 2/CO 10, 30, 50, 70, ±2 of H 2 in CO H 2/CO 2/N 2 20/60/20, 20/40/40, ±2 20/20/60, 40/40/20, 40/20/40, 60/20/20 H 2/CO 2/N 2/CO 16.3/5.3/60.7/17.8 (M1) ±2 20/20/30/30 (M2) 40/20/20/20 (M3) 60/20/10/10 (M4) 20/30/30/20 (M5) Membrane thickness (µm) 2.4. RESULTS AND DISCUSSION H2, N2, CO2 and CO pure gas permeation experiments Table II - 3 lists the average permeability of pure gases as an average of several runs. The permeability coefficients decrease in the following order of average values (Barrer): P H2 = 23.6 > P CO2 = 5.7 > P CO = 0.43 > P N2 = 0.17, which is also the order of increasing kinetic diameters of the gas molecules. These results are in agreement with literature data collected in Table II - 3, that present an average H2 permeability of 23.0 ± 5.1 Barrer, an average CO2 permeability of 7.9 ± 2.0 Barrer and an average N2 permeability of 0.26 ± 0.05 Barrer, values obtained in a narrow range of temperatures (30-35 o C) and pressures (2-4 bar). With regard to CO no previous data of its permeability in Matrimid 5218 membranes have been reported, thus the obtained value in this work PCO = 0.43 Barrer, constitutes original data for this material.
75 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid membrane 59 Table II 3. Pure gas permeabilities and ideal selectivities values for planar dense Matrimid 5218 membrane Permeability (Barrer) Ideal Selectivity Exp. Conditions Ref. H2 CO2 N2 CO H2/N2 H2/CO2 H2/CO T ( o C) P (bar) this work      1 Barrer = 1 x cm 3 (STP) cm cm -2 s -1 cmhg -1 Sweep gas flow rate effect Figure II - 9 shows that for the highly permeable H2 the permeability reaches a asymptotic value of 24.1 Barrer when using sweep gas flow rates 6 cm 3 (STP) min -1. At lower Argon flow rates, hydrogen accumulates at the permeate side resulting in a decrease of the effective concentration driving force through the membrane. Figure II 9. Effect of sweep gas flow rate on H2 permeability, at 30 o C and 4 bar feed pressure.
76 60 Chapter II Temperature effect The temperature dependency of the permeability coefficients for H2, CO2, CO and N2 was determined experimentally and is plotted in Figure II Figure II- 10. The permeability of pure H2, CO2, CO and N2 as a function of temperature at 4 bar feed pressure. As temperature increased all four gas permeabilities increased. Arrhenius plots are represented in Figure II - 10 showing straight lines with high correlation coefficients (R 2 > 0.99) in all cases. Having established the validity of the Arrheniustype dependence with temperature expressed by Equation II 16 where R = 8.31 J mol -1 K -1 is the general gas constant and T is the temperature (K), the specific parameters for permeation of H2, CO2, N2 and CO were calculated (Table II - 4). II 16 The permeation activation energy Eap increased in the order CO2 < H2 < CO < N2, the same as reported in other glassy polymeric membranes [27, 28] for the case of CO2, H2 and N2. The very low EaP value of CO2 compared with those of H2, CO and N2, could be attributed primarily to the lower heat consumption for CO2 diffusion, lowering the amount of energy associated to the permeation phenomenon, as reported for ABS copolymer membranes .
77 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid membrane 61 Table II 4. Arrhenius parameters for CO2, N2, H2 and CO permeation through a Matrimid 5218 dense film Arrhenius parameters Gas N2 H2 CO2 CO Ref. P0 (Barrer) this work (pure gas) this work (quaternary gas mixture) EaP (kj mol -1 ) this work (pure gas) this work (quaternary gas mixture)   Using the Equation I - 8 (from Chapter I) to calculate ideal gas selectivity values at different temperatures, the relative effects of temperature on the ideal selectivity for H2/CO2, H2/N2, H2/CO and CO/N2 separations through the Matrimid membrane α can be determined. Thus, the ideal selectivity H2/CO2 increases with temperature from a value of 4.0 at 30 o C to 5.3 at 100 o α C, while the selectivity H2/N2 decreases with temperature from at 30 o C to 81.8 at 100 o C, as shown in Figure II Figure II 11. Ideal selectivity variation with the temperature for (a) H2/CO2, CO/N2 and (b) H2/N2, H2/CO gas pairs at 4 bar feed pressure
78 62 Chapter II The pairs H2/CO and CO/N2 present the same trend of decreasing selectivity with temperature from a value of 55.1 to 40.5 and of 2.5 to 2.0 respectively. In glassy polymers the two parameters determining the permeability, i.e., the diffusion and solubility (Equation I - 7) exhibit also an Arrhenius type dependence with temperature as the permeability parameter. The associated activation energy of diffusion (ED) is positive meanwhile the enthalpy of sorption ( Hs) is negative . Therefore increasing temperature has an opposite effect: the diffusion coefficient increases meanwhile the solubility coefficient decreases. Prior work  on the permeability dependence with temperature of dense Matrimid membrane showed that ED increased in the order H2 < CO2 < N2 meanwhile the absolute value of Hs increased in the order H2 < N2 < CO2. In all cases ED is higher than Hs and their sum gives the energy of permeation (EaP) which is always positive and thus their relative contribution determines the increasing rate of permeability with temperature for gases. In the case of CO2 at low temperatures, the CO2 solubility was the major contributing factor to the permeability because of the low diffusivity but as the temperature increased the regime was shifted from diffusion - limited to sorption - limited because of the higher dependence of diffusivity on temperature. Thus, the increasing rate of CO2 permeability with temperature was lower than the increasing rate of H2 and therefore the H2/CO2 selectivity increased. Feed pressure effect Pure gas permeability values obtained at different feed pressures are presented in Table II - 3. For H2, N2 and CO there is a slight decrease in permeability with pressure but it does not exceed pure gases deviations of 5% encountered in literature and therefore this variation cannot be attributed to an influence of pressure over permeability in the pressure range under study. In the case of CO2 the permeability observed a 19 % decrease in the pressure range under study. The behavior of H2, CO and N2 is typical for low-sorbing penetrants in glassy polymeric membranes , their transport being more diffusion dependent meanwhile the behavior of CO2 shows higher solubility dependence. When the pressure increases, the solubility coefficient of CO2 decreases determining a higher decrease in the permeability coefficient for CO2 than for the more inert H2, N2 and CO. Similar influence of pressure on CO2 permeability has been previously reported by several studies with other glassy polymers [1, 30]. As shown in Figure II 12, in glassy polymers CO2 permeability can decrease with pressure until it reaches a minimum value from which it began to increase again.
79 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid membrane 63 The pressure at which permeability presents a minimum is named the plasticization pressure. The decrease in gas permeability is related to competitive solubility effects between the gas and the polymer matrix, the polymer sorption sites becoming saturated with gas molecules and is predicted by the dual mode sorption model. From the plasticization pressure onwards, the polymeric chain packing is disrupted by the penetrant molecules due to the increase in the segmental mobility that expands both the frequency and the average size of transient gaps that enable diffusion, thereby increasing the permeability. Figure II Literature results for CO2 permeability as function of CO2 pressure for a 30 µm thickness Matrimid dense film at 22 o C . It has been demonstrated that the plasticization pressure depends on the solvent from where the polymeric films were cast from, on the final membrane thickness and on the experimental temperature, but it corresponds to a constant concentration of CO2 (cm 3 (STP)/cm 3 ) into the polymer matrix. Table II 5 list the variation in the CO2 plasticization pressure. In the present work the maximum pressure studied was of 6 bar so the plasticization pressure of Matrimid by CO2 was not reached for the 30 µm film under study. Therefore the experimental results of permeability for CO2 can be adjusted by the dual sorption partial immobilization model in the entire range of pressure studied.
80 64 Chapter II Table II 5. Plasticization pressure of Matrimid films cast from different solvents at different temperatures . Solvent Film thickness Temperature Plasticization (µm) ( o C) pressure (bar) CHCl DMAc NMP H2/N2/CO/CO binary, ternary and quaternary mixed gas permeation experiments Analysis of H2 permeation H2 / N2 mixtures H2 /N2 mixture is formed by a fast permeating gas, i.e. H2, and a slow permeating gas, i.e. N2. This type of mixtures might present concentration polarization phenomena at the feed side of the membrane at low concentrations of the fast permeating gas. Figure II - 13 shows that concentration polarization occurs at hydrogen concentrations below 10 vol %. Then, at concentrations higher than 10%, hydrogen permeability leveled off to a constant value, equal to the pure hydrogen permeability, as it is shown in Figure II This indicates that from this level, H2 transport is not affected by the presence of N2 as co-partner in the overall gas transport through the polymer matrix, demonstrating that there is no coupling or competitive sorption between the two species. N2 permeability presented no variation with its concentration, i.e., its partial pressure.
81 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid membrane 65 Figure II 13. H2 permeability variation with its feed concentration in mixtures with N2, at 30 o C and 4 bar feed pressure. Figure II 14. H2 Permeation variation with its fugacity for mixtures: H2/CO2 at 4 and 6 bar, H2/N2 and H2/CO at 4 bar total pressure and 30 o C. Data points represent experimental values and lines are model results.
82 66 Chapter II H2 / CO2 mixtures As it can be seen in Figure II - 14, H2 permeability was strongly affected by the PH presence of CO2. For a total pressure of 6 bar, the value of 2 with a mixture 10/90 (vol%) H2/CO2 became 42% lower than the permeability obtained working with pure gas. Furthermore, hydrogen permeability is influenced by the total pressure of the feed gas, that is, at a given hydrogen partial pressure, hydrogen permeability increases at lower CO2 partial pressure. Then, hydrogen permeability is better plotted as a function of CO2 fugacity (Figure II - 15) that shows similar H2 permeabilities at equal CO2 fugacities, but independent of the presence of other components. Figure II H2 permeability variation with CO2 fugacity for mixtures: H2/CO2 at 4 and 6 bar, H2/N2/CO2 and H2/N2/CO2/CO at 4 bar total feed pressure and 30 o C. Data points represent experimental values and lines are modeling results. These results indicate competitive sorption between H2 and CO2 for the sorption sites present in the matrix, which get saturated at a certain pressure, thereby leading to a decrease in solubility at higher penetrant pressures. At a given concentration (vol %) of the feed mixture, as the feed pressure is increased, more sorption of carbon dioxide in the Langmuir sites occurs because of carbon dioxide s larger affinity constant and solubility in polyimide Matrimid membrane. As a consequence
83 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid membrane 67 hydrogen molecules are prevented to diffuse and therefore the effect of competitive sorption between carbon dioxide and hydrogen is increased. It can also be mentioned that when a pure H2 permeation experiment was performed after an experiment with CO2, the time needed to reach a steady state H2 permeability value was much larger than the usual 30 min established in the procedure. It can be assumed that H2 permeability was affected even by trace levels of the CO2 present in the installation tubes or even in the membrane as sorbed specie. H2 / CO mixtures Figure II - 14 shows that H2 permeability is not influenced by the presence of CO in the feed gas mixture, and therefore there is no evidence of competitive transport phenomena between these two species. Also, the permeability of CO is equal to the pure gas permeability reported in Table II - 3. Ternary and quaternary mixtures Hydrogen permeation data for H2/CO2/N2 ternary mixtures is shown in Figure II The arrows indicate the concentration of each component in the mixture. Figure II 16. H2 permeability variation in H2, N2 and CO2 ternary mixtures, at 30 o C and 4 bar At a constant concentration of CO2 the H2 permeability coefficient is constant even if the concentration of N2 changes substantially; therefore it is clear that hydrogen transport is affected only by the amount of CO2. The supplementary presence of N2 does not affect the transport of H2.
84 68 Chapter II In the case of the quaternary gas mixtures, the mixture labeled M1 in Table II 2, represents a synthetic mixture similar to the dry post-combustion gas stream obtained in the production of carbon black. The next three mixtures (M2, M3 and M4) had a constant concentration of CO2, an increasing concentration of H2 and a constant and equal to unity ratio N2/CO. The last quaternary mixture studied (M5) had a slightly higher partial pressure of CO2. The results in terms of H2 permeability are plotted all together in Figure II 15 where three points differentiate. The upper left pint is the value of the H2 permeability coefficient of the mixture M1. The next one in decreasing order is actually a cumulus of three points corresponding to the H2 permeability coefficient of the mixtures M2, M2 and M3 were the constant concentration of CO2 determined a lower but constant permeability value for H2 regardless the concentrations of N2 and CO. This makes clear once more that hydrogen transport is affected only by the amount of CO2. The supplementary presence of either N2 or CO does not affect the transport of H2. The lowest H2 permeability value belongs to mixture M5 with a higher concentration of CO2. The Arrhenius specific parameters for permeation with the quaternary mixture M1 were calculated, obtaining slightly different values to those obtained with pure gases. These values are summarized in Table II - 4. Analysis of CO2 permeation In all mixtures (binary H2/CO2 at 4 and 6 bar total pressure, CO2/N2, ternary H2/CO2/N2 and quaternary H2/N2/CO2/CO mixtures) the transport rate of CO2 is slightly lower than for the pure gas but it presents a similar behavior of decreasing permeability with increasing CO2 fugacity (Figure II - 17). Also, CO2 permeability data are equal for all mixtures at the same values of CO2 partial pressure, indicating that the CO2 transport rate is almost unaffected by the nature of the other components. Therefore, the competitive sorption between H2 and CO2 influences considerably more the transport rate of H2 than the transport rate of CO2.
85 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid membrane 69 Figure II 17. CO2 Permeation variation with CO2 fugacity for mixtures: H2/CO2 at 4 and 6 bar, CO2/N2 and H2/CO2/N2 at 4 bar total feed pressure and 30 o C. Data points represent experimental values and lines are modeling results Mixed gas selectivity As a result of the lower H2 permeability in mixtures with CO2, the real selectivity for the H2/CO2 gas pair, calculated from the permeability data obtained in mixed gas experiments, results in an average value of 2.93 (Figure II - 18). The latter value is significantly lower than the selectivity calculated from pure gas permeability data, which resulted in an average value of 4.2. In Figure II 18 the ideal selectivity is calculated from gas permeability values obtained with pure H2 and respectively CO2 at 2, 4 and 6 bar total feed pressure; meanwhile the mixed gas selectivity is calculated from feed and permeate gas concentration values according to Equation I 9 (Chapter I).
86 70 Chapter II Figure II 18. H 2 /CO 2 selectivity variation with H 2 fugacity in the feed for pure and mixed (H 2 /CO 2 ) feed gas Similarly depression in H2 permeability in mixtures with CO2 was reported in surface modified 6FDA-durene polyimide membranes where the H2/CO2 selectivity decreased from an ideal value of 101 to a value of 42 . The same phenomenon occurs in the reverse selective membranes that exhibit favorable interactions with CO2 and permeate preferentially CO2 to H2. These membranes exhibit a CO2/H2 selectivity higher than 1. One example is the work of Chen et al.  that reveals a drastic increase in CO2/H2 selectivity in mixed gas test compared to the selectivity obtained from pure gas permeability coefficients for membranes made of copolymers between poly(ethylene oxide) and a polyimide Mathematical modelling The adequacy of the dual sorption-partial immobilization model for the prediction of H2 and CO2 permeation through Matrimid 5218 membrane was tested. Experimental permeability data, corresponding to pure, binary, ternary and quaternary mixtures, were fitted to Equation II - 13 by a non-linear multiparametric regression procedure using the Aspen Custom Modeler (AspenTech) software tool. Pure gas dual-mode solubility parameters were taken from the literature [34, 35], for CO2 and N2 and are listed in Table II 6. Up to our knowledge there are no published data of dual-sorption model parameters for H2 and CO in Matrimid polymer, although some authors have studied the sorption of H2 in other glassy polymers [27, 36].
87 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid membrane 71 Table II 6. Available literature data for the dual sorption model parameters for N2 and CO2 in Matrimid dense films  Model parameter Gas N2 CO2 b (1/bar) kd (cm 3 (STP) cm -3 bar -1 ) (cm 3 (STP) cm -3 ) K= / To facilitate calculation, a new set of parameters was defined as follows, A = k D 1 D D (II- 17) A2 = k FKD = D c b (II- 18) D D H H By substitution of Equations (II - 17) and (II - 18) into Equation (II - 13), two new equations are obtained as follows: P H 2 = A 1H b H 2 f H 2 + b N 2 f A2 H 2 + b CO 2 CO 2 f CO 2 + b CO f CO (II - 19) P CO2 = A 1CO b H 2 f H 2 + b N 2 A f CO2 2CO2 + b CO2 f CO2 + b CO f CO (II - 20) The resulting model is composed of two equations with six independent parameters: A1H2, A1CO2, A2H2, A2CO2, bh2, bco. The regression solution was unique due to the vast domain of experimental data used. The estimated values of the parameters are given in Table II - 7. As expected, the CO2 Langmuir s population moving fraction F = 0.07 was lower than 1 . In the case of H2 permeation, due to the lack of sorption parameters in Matrimid polymer, the results obtained are expressed as a function of the grouped parameters A1 and A2 and the affinity parameter b. The estimated value of the latter, bh2 = 0.05 bar -1, is close to the one reported by El-Azzami and Grulke  of 0.09 bar -1 in a natural glassy polymer, Chitosan, at 20 o C. On the other hand, the value of the Langmuir solubility parameter for carbon monoxide obtained by fitting the experimental results is bco = 0.05 bar -1.
88 72 Chapter II Table II 7. Dual-mode sorption, partial immobilization model estimated parameters for H2 and CO2 permeation in Matrimid 5218 membrane Model parameter A = k D 1 D D (Barrer) A k FKD D c 2 = D D = H Hb (Barrer) b (1/bar) Gas H2 CO known value DD (cm 2 /s) DH (cm 2 /s) K F Figure II - 19 shows the parity graph of the experimental and simulated permeability coefficients of H2 and CO2. There is a satisfactory agreement between predicted results and experimental data with correlation coefficient (R) higher than 0.95 and mean squared relative error (MSRE) lower than Figure II 19. Parity graphs of the predicted H2 (a) and CO2 (b) gas permeability data by the dual sorption-partial immobilization model with the experimental results
89 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid membrane CONCLUSIONS The mixed gas permeation through a Matrimid homogeneous thick film has been investigated over the full range of concentrations for the separation of H2 from N2, CO and CO2. Also, the influence of temperature and pressure on gas permeation was examined. For pure gases, the permeability coefficients decreased in the following order of average values (Barrer): PH2 = 23.6 > PCO2 = 5.7 > PCO = 0.43 > PN2 = 0.17, which is also the order of increasing kinetic diameters of the gas molecules. As temperature increased all four gas permeabilities increased. The ideal α selectivity H 2 / CO 2 α α increases with temperature, while the selectivity H 2 / N 2 H 2 / COdecreases with temperature. The same behavior with temperature was observed for a quaternary gas mixture. For the highly permeable H2 gas the concentration polarization phenomenon was put in evidence for H2/N2 mixtures at feed concentrations lower than 10 vol % H2. In pure gas, at a feed pressure of 6 bar and a temperature of 30 o C, the hydrogen permeability was 23.1 Barrer, and the ideal H2/CO2 selectivity was 4.4. In mixed gas experiments, for binary 10/90 (vol %) H2/CO2 mixtures, competitive sorption between H2 and CO2 led to significant decays both in H2 α permeability, which was reduced to 13.8 Barrer and in the selectivity H 2 / CO 2that decreased to 2.7. For CO2, transport rate was unaffected by the presence of hydrogen, nitrogen and carbon monoxide. H2 and CO2 permeation behavior from pure, binary, ternary and quaternary mixtures (H2/N2/CO/CO2) through planar Matrimid membrane was satisfactorily described by the dual-mode sorption, partial immobilization model. The model sorption parameters for H2 and for CO were unknown and obtained from the fitting of the experimental data to the proposed model. These results provide useful knowledge related to the intrinsic material properties, considering gas mixtures of industrial interest and essential when other membrane configurations like hollow fibers, mixed matrix membranes or polymer blends are proposed. and
90 74 Chapter II References 1. S. Matteucci, Y. Yampolskii, B.D. Freeman, I. Pinnau, Transport of Gases and Vapors in Glassy and Rubbery Polymers, in: Materials Science of Membranes for Gas and Vapor Separation, John Wiley & Sons, Ltd, New York, 2006, pp R.M. Barrer, J.A. Barrie, J. Slater, Sorption and diffusion in ethyl cellulose. Part III. Comparison between ethyl cellulose and rubber, J. Polym. Sci. 27 (1958) A.S. Michaels, W.R. Vieth, J.A. Barrie, Solution of gases in polyethylene terephthalate, J. Appl. Phys. 34 (1963) K. Toi, G. Morel, D.R. Paul, Gas sorption and transport in poly(phenylene oxide) and comparisions with other glassy polymers., J. Appl. Polym. Sci. 27 (1982) W.J. Koros, A.H. Chan, D.R. Paul, Sorption and transport of various gases in polycarbonate, J. Membr. Sci. 2 (1977) R.W. Baker, Membrane Technology and Applications, 2nd edition ed., John Wiley and Sons, New York, J.D. Wind, Improving polyimide membrane resistance to carbon dioxide plasticization in natural gas separations, Ph.D. dissertation, The University of Texas at Austin (2002). 8. W.J. Koros, D.R. Paul, A.A. Rocha, Carbon dioxide sorption and transport in polycarbonate, J. Polym. Sci., Polym. Phys. 14 (1976) E.S. Sanders, W.J. Koros, H.B. Hopfenberg, V.T. Stannett, Pure and mixed gas sorption of carbon dioxide and ethylene in poly(methyl methacrylate), J. Membr. Sci. 18 (1984) T. Oishi, J.M. Prausnitz, Estimation of solvent activities in polymer solutions using a group-contribution method, Ind. Eng. Chem., Process Des. Dev. 17 (1978) R.M. Conforti, T.A. Barbari, P. Vimalchand, M.D. Donohue, A lattice-based activity coefficient model for gas sorption in glassy polymers, Macromolecules 24 (1991) R.G. Wissinger, M.E. Paulaitis, Molecular thermodynamic model for sorption and swelling in glassy polymer-co2 systems at elevated pressures, Ind. Eng. Chem. Res. 30 (1991) M. Minelli, S. Campagnoli, M.G. De Angelis, F. Doghieri, G.C. Sarti, Predictive model for the solubility of fluid mixtures in glassy polymers, Macromolecules 44 (2011)
91 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid membrane M.C. Ferrari, M. Galizia, M.G. De Angelis, G.S. Sarti, Vapor Sorption and Diffusion in Mixed Matrices Based on Teflon AF 2400, in: Y. Yampolskii, B. Freeman (Eds.), Membrane Gas Separation, Wiley, Chichester, 2010, pp F. Doghieri, G.C. Sarti, Predicting the low pressure solubility of gases and vapors in glassy polymers by the NELF model, J. Membr. Sci. 147 (1998) R.H. Lacombe, I.C. Sanchez, Statistical thermodynamics of fluid mixtures, J. Phys. Chem. 80 (1976) I.C. Sanchez, R.H. Lacombe, Statistical thermodynamics of polymer solutions, Macromolecules 11 (1978) I.C. Sanchez, R.H. Lacombe, An elementary molecular theory of classical fluids. Pure fluids, J. Phys. Chem. 80 (1976) I.C. Sanchez, R.H. Lacombe, Elementary equation of state for polymer liquids., J. Polym. Sci. Part B Polym. Lett. 15 (1977) U. S. Enviromental protection agency, Hazard Summary -1,1,2,2-Tetrachloroetane, (2007). 21. M. Koretsky, Engineering and Chemical Thermodynamics, John Wiley & Sons, New Jersey, Y. Zhang, I.H. Musselman, J.P. Ferraris, K.J. Balkus Jr., Gas permeability properties of Matrimid membranes containing the metal-organic framework Cu-BPY-HFS, J. Membr. Sci. 313 (2008) S.S. Hosseini, M.M. Teoh, T.-S. Chung, Hydrogen separation and purification in membranes of miscible polymer blends with interpenetration networks, Polymer 49 (2008) H.-W. Rösler, Membrantechnolgie in der Prozessindustrie - Polymere Membranwerkstoffe, Chem. Ing. Tech. 77 (2005) H.-Y. Zhao, Y.-M. Cao, X.-L. Ding, M.-Q. Zhou, Q. Yuan, Effects of cross-linkers with different molecular weights in cross-linked Matrimid 5218 and test temperature on gas transport properties, J. Membr. Sci. 323 (2008) S. Shishatskiy, C. Nistor, M. Popa, S.P. Nunes, K.V. Peinemann, Polyimide asymmetric membranes for hydrogen separation: Influence of formation conditions on gas transport properties, Adv. Eng. Mater. 8 (2006) L.A. El-Azzami, E.A. Grulke, Dual mode model for mixed gas permeation of CO2, H2, and N2 through a dry chitosan membrane, J. Polym. Sci. Part B 45 (2007)
92 76 Chapter II 28. K. Tanaka, H. Kita, K. Okamoto, A. Nakamura, Y. Kusuki, Gas permeability and permselectivity in polyimides based on 3,3',4,4'-biphenyltetracarboxylic dianhydride, J. Membr. Sci. 47 (1989) J. Marchese, E. Garis, M. Anson, N.A. Ochoa, C. Pagliero, Gas sorption, permeation and separation of ABS copolymer membrane, J. Membr. Sci. 221 (2003) K. Simons, K. Nijmeijer, J.G. Sala, H. van der Werf, N.E. Benes, T.J. Dingemans, M. Wessling, CO2 sorption and transport behavior of ODPA-based polyetherimide polymer films, Polymer 51 (2010) A. Bos, I.G.M. Pünt, M. Wessling, H. Strathmann, CO2-induced plasticization phenomena in glassy polymers, J. Membr. Sci. 155 (1999) T.-S. Chung, L. Shao, P.S. Tin, Surface modification of polyimide membranes by diamines for H2 and CO2 separation, Macromol. Rapid Comm. 27 (2006) H. Chen, Y. Xiao, T.-S. Chung, Synthesis and characterization of poly (ethylene oxide) containing copolyimides for hydrogen purification, Polymer 51 (2010) T.T. Moore, W.J. Koros, Gas sorption in polymers, molecular sieves, and mixed matrix membranes, J. Appl. Polym. Sci. 104 (2007) C.A. Scholes, W.X. Tao, G.W. Stevens, S.E. Kentish, Sorption of methane, nitrogen, carbon dioxide, and water in matrimid 5218, J. Appl. Polym. Sci. 117 (2010) S. Zhou, S.A. Stern, The solubility of hydrogen in glassy poly(vinyl acetate) at elevated pressures, J. Membr. Sci. 50 (1990) C.L. Aitken, W.J. Koros, D.R. Paul, Gas transport properties of biphenol polysulfones, Macromolecules 25 (1992)
93 Chapter III HYDROGEN MIXED GAS SEPARATION STUDY USING ASYMETRIC HOLLOW FIBER MEMBRANES
94 78 Chapter III
95 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane 79 ABSTRACT The characterization of mixed gas permeation through hollow fiber membranes is essential for the industrial application of gas separation technology. In chapter II specific phenomena that occur in the permeation of H2-containing gas mixtures through planar dense Matrimid membranes and determine a different transport behavior with respect to pure gas were reported. Phenomena like concentration polarization and competitive transport were thoroughly studied and modeled. In this chapter the same application is assessed using asymmetric hollow fibers membranes because large-scale gas separation applications demand highly productive membranes with high membrane surface/volume ratios and membranes with hollow fiber geometry have a distinct advantage over flat sheet membranes as they possess a much thinner dense skin layer and thus they are much more productive. This chapter is focused on the characterization of H2-containing gas mixtures permeation through asymmetric hollow fiber membranes using binary (H2/N2, H2/CO, H2/CO2) and quaternary (H2/N2/CO/CO2) gas mixtures at a constant temperature of 30 o C and pressures up to 10 bar. Also, the effect of temperature over mixed gas permeation was studied using a H2/N2/CO/CO2 quaternary mixture similar to the flue gases obtained in carbon black manufacturing. First, in order to compare gas separation behavior of hollow fiber with dense films, asymmetric hollow fibers fabricated from the same polymeric material as the dense films (Matrimid), were used. Then, as means of further increasing gas selectivity towards H2 and suppressing CO2 plasticization new asymmetric hollow fiber membranes were fabricated from polymer blends of Matrimid and polybenzimidazole (PBI). Fibers with good morphology and without defects were obtained only from the pure Matrimid. Regrettably, polymer blending lead to fibers with poor mechanical properties. Also, the comparative permeation performance between Matrimid and a much more permeable material PPO was done using commercial PPO asymmetric hollow fibers modules obtained from Parker Filtration and Separation B.V. Using a Matrimid based hollow fiber membrane, the ideal selectivity values obtained for H2/N2, H2/CO and H2/CO2 gas pairs were of 74.4, 42.6 and 5 respectively with a H2 permeance of 67 GPU at 2.3 bar feed pressure. For mixtures that contain H2 and CO2 the performance was better than that of dense films since a lower depression in the permeability of H2 was observed. Phenomena related to the complex morphology of the asymmetric hollow fibers like substructure resistance, induced accelerated plasticization with CO2 and competitive sorption effects between H2/CO2 are presented. Therefore, it is clear that use of thick film data to design or select
96 80 Chapter III membrane materials only gives a rough approximation of the performance that might be realized in practice. In contrast with Matrimid hollow fiber membranes the use PPO hollow fiber membranes gives considerably higher gas permeability with a value of 2152 GPU for pure H2 at the expense of lower gas selectivities with values for H2/N2, H2/CO and H2/CO2 gas pairs of 30, 22 and 3 respectively. Thus the H2 concentration in the permeate of a PPO hollow fiber module was of only 40 vol % meanwhile in the Matrimid hollow fiber module was more than double (87-89 vol %) PREPARATION OF ASYMMERTIC HOLLOW FIBER MEMBRANES - BACKGROUND The fabrication of hollow fibers membranes is based on a dry/wet spinning method when a phase inversion process takes place. The concept of phase inversion covers a range of different techniques such as solvent evaporation, precipitation by controlled evaporation, thermal precipitation, precipitation from the vapor phase and immersion precipitation . In all cases the starting point is a thermodynamically stable solution which is subject to demixing (phase separation). A membrane is made by casting a polymer solution on a support and then bringing the solution to phase separation by means of solvent outflow and/or nonsolvent inflow [2, 3]. This can be done by temperature changes or changes in composition. The phase separation process by immersion precipitation allows the formation of defect-free, high-flux membranes [1, 4] that have an asymmetric structure with a thin, selective skin on a much thicker but highly porous supporting layer. The thin selective layer is formed during the short healing period or dry step (i.e., free standing evaporation) prior to the immersion in the non-solvent bath where phase separation occurs to the rest of the membrane. These membranes developed within the Loeb-Sourirajan process allowed the industrial breakthrough in 1960 s of synthetic membrane processes such as reverse osmosis and ultrafiltration and in 1979 the breakthrough of gas separation process for hydrogen recovery. The phase diagram of a typical membrane forming system by the dry/wet phase inversion technique is schematically shown in Figure III 1 . The system has three components: a polymer, a solvent and a nonsolvent, which is miscible with the solvent but not with the polymer. The corners of the triangle represent pure components, the sides represent binary mixtures of the two components connected and the interior of the triangle represents a ternary mixture of the three components. The binodal boundary divides the phase diagram into a single-phase region, where the three components are miscible in all compositions, and a two-phase region, where
97 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane 81 the system separates into two phases. The tie lines connect points on the binodal that are in equilibrium. A composition within this two-phase region always lies on a tie line and it splits into two phases represented by the two intersections between the tie lines and the binodal. Thus one end point of the tie line is rich in polymer and the other end point is poor in polymer. At the end of phase separation, the polymer-rich phase forms the membrane matrix, whereas the polymer-lean phase forms the membrane pores. The spinodal boundary further divides the two-phase region into a metastable region and an unstable region. Within the metastable region the phase separation proceeds via a nucleation and growth of one of the phases and results in cellular structures. Within the unstable region the phase transition is characterized by a fast and uniform separation of the two phases that leads to interconnected, bicontinuous structures. Figure III 1. Scheme of the three component phase diagram indicating a starting solution formed of three components: polymer, solvent and nonsolvent . Application of such a dry/wet process in hollow fiber geometry is more complicated than with simple flat sheets. All mass transfer associated with the dry step in fiber spinning must occur during the nascent fiber s residence time in the air gap (see Experimental methodology section), which is extremely shorter than with flat sheets. Therefore the formation conditions must be set to values that allow a rapid formation of a defect free outer skin layer during the nascent fiber s residence time in the air gap:
98 82 Chapter III (I) First it must be decided if a non solvent will be used within the dope solution. The use of a non-solvent approaches the dope solution composition closer to the binodal boundary allowing a rapid phase separation (see Figure III 1). EtOH is usually chosen as non-solvent instead of water because water is such a strong non-solvent that practical titration of the spin dope close to the binodal becomes difficult. (II) Then, the dope formulation is based on experimentally estimations of the binodals for the multi-component (solvent, non-solvent, and polymer) system on the basis of cloud point measurements. Figure III 2 shows literature binodal results for the ternary NMP, EtOH, Matrimid system. Figure III 2. Binodals for the ternary NMP, EtOH and Matrimid system at 23 o C  (III) In order to obtain a good morphology of the functional layer, from the various possible formulations found close to the binodal line, the optimum corresponds to polymer concentrations a few lower than the critical polymer concentration (c. p. c.). C. p. c. is defined as the polymer concentration point from where the dope solution viscosity increases exponentially with the polymer concentration and it is calculated from the intersection of the tangent lines to the two domains of the viscosity trend curve as shown in Figure III 3 where real literature data for various polymer/solvent systems of interest in this work are reported.
99 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane 83 Figure III 3. The trend of changes in dope viscosity as a function of polymer concentration in the solvent . (IV) A higher temperature of the dope than the air gap temperature allows a rapid evaporation of the solvent when the dope solution enters the air gap. As the nascent fiber cools down the viscosity increases giving a mechanically stable nascent fiber. The viscosity variation with temperature of all dope solutions used in this work (see Experimental and methodology section) is shown in Figure III 4. (V) In order to obtain a defect-free top layer, a volatile solvent can be added in small concentration to the dope solution. Figure III 4. Dope solution viscosity variation with temperature
100 84 Chapter III 3.2. EXPERIMENTAL METHODODOLOGY Materials The commercial polymer Matrimid 9725 (polyimide of 3,3, 4,4 -benzophenone tetracarboxylic dianhydride and diamino-phenylidane) was kindly provided by Huntsman Advanced Polymers. Matrimid 9725 is a micropulverized version of Matrimid Polybenzimidazole (PBI) polymer was obtained from PBI Performance Products, Inc. The 1-methyl-2-pirrolidone (NMP) solvent and ethanol (EtOH) as non-solvent (absolute grade, 99.9% purity) were used as received for the preparation of the polymer solutions. Solvent exchange fluids included EtOH (technical grade, 96-98% purity), hexane and tap water. LiCl salt was used for the stability (in order to avoid gelation) of the dope formed by polymer blending of Matrimid with PBI. Gases were purchased from Air Liquide (Spain) with a purity of at least %. PPO hollow fibers modules were provided by Parker Filtration and Separation B. V Fabrication of asymmetric hollow fiber membranes by the dry/wet spinning process The operation conditions applied for the fabrication of the asymmetric hollow fiber membranes are listed in Table III 1. The pure Matrimid based hollow fibers were labeled D1 and three different fibers were obtained (D1-M1, D1-M2, D1-M3) by varying the gap height. The two Matrimid - PBI polymer blend based fibers were labeled D2 and D3. For the pure Matrimid hollow fibers the operation conditions are based on optimized procedures reported in the literature [6, 8-10]. In the case of the formulation of Matrimid/PBI dopes (D2 and D3), NMP was preferred as solvent instead DMAc that was used in literature  because is a less hazardous solvent. Therefore, the critical polymer concentration had to be determined for the dope D2 that is based on two components: polymer blend and solvent. The viscosity of polymer solution samples of increasing concentration was measured with a Haake Viscotester 550 (see Figure III - 4). The resulting c. p. c. value of 26.4 wt% is somewhat higher than the reported value of 22% in DMAc (see Figure III - 3). Also, a new and optimized formulation for the Matrimid PBI dope - D3 was proposed by using a non solvent (EtOH) as additional component. In order to determine the formulation of the dope - D3, EtOH was added in 3 cm 3 quantities to a
101 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane wt % binary mixture (polymer blend and NMP) until demixing occurred at 23.5 wt % polymer and 21.7 wt % EtOH. The optimum formulation of the dope D3 is close to the demixing concentration but a much higher polymer concentration was preferred due to a higher necessary viscosity for spinning. As shown in Figure III 5 at 50 o C the viscosity if the dope D3 is still much lower than the viscosities of the dopes D1 and D2 and therefore a lower temperature of 25 o C were preferred for spinning. Regrettably, the experimentally determination of the binodal for the multi-component system (polymer blend, NMP, EtOH) was not carried out. Table III 1. Formation Conditions for the asymmetric hollow fiber membranes Dope composition (wt%) D1 D2 D3 Matrimid:PBI (1:0) 26.2 (1:1) 26.4 (1:1) 27.6 NMP EtOH Additives (LiCl) Bore composition (wt%) NMP H2O Spinning conditions Tube in orifice OD spinneret (mm) ID Dope temperature ( o C) Dope flow rate (cm 3 h -1 ) Bore flow rate (cm 3 h -1 ) Air gap height (cm) D1 - M D1 - M2 6 D1 - M3 3 Room temperature ( o C) Room humidity % Quench Temperature water ( o C) Take-up rate (m min -1 ) Sequential dehydration procedure (1) Water baths continuous flow 24 h (2) MeOH baths 3 (20 min each) (3) Hexane baths 3 (20 min each) (4) Ambient dry
102 86 Chapter III Figure III 5. The trend of changes in solution viscosity as a function of polymer concentration in the solvent. For the fabrication of all fibers a similar procedure was applied using a spinning equipment located at the Membrane Technology Group, University of Twente (see Figure III 6 and Figure III - 7). The polymer powder was dried in a vacuum oven at 100 o C for at least 12 h prior to use. The dope solution was prepared at 50 o C in a Pyrex vessel with mechanical stirring (Heidolph RZR 2041) and a coiled condenser to prevent ethanol loss. After mixing for at least 8 hours the dope solution was filtered with a 15 µm sintered metallic filter (Bekipor STAL3 Bekaert) and poured in a sealed spinning dope tank where it was left to degas at the specified dope temperature for 24 h before spinning. The bore solution and the water quench bath were also left to degas 24 h before spinning. Polymer solution and bore fluid were simultaneously pumped through a tube-in-orifice spinneret using gear pumps. Figure III 8 shows the spinneret assembly with several detailed views from the upper and lower part and a vertical cross section with dimensions. A triple - orifice spinneret was used as a dual spinneret by closing the external channel. The extruded fibers passed first through an air gap before entering in the coagulation bath filled with tap water at room temperature. The nascent fiber was oriented by a guiding wheel and pulled by a third and forth wheel, that had the same pulling speed, into a collecting wheel with the perimeter of 1 m from where they were cut and rinsed for 24 h in a water bath with continuous renewal of tap water. Next, the solvent exchange procedure using methanol and hexane listed in Table III 1 and III - 2 was applied. The solvent exchange process was found to play a critical role in the resulting membrane morphology and permeation performance . After spinning, the porous
103 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane 87 substructures of the hollow fiber membranes are filled with water. Drying such water wet membranes can cause significant changes in porous structure due to the enormous capillary forces that are present during water removing. The solvent exchange procedure used in this work replaces water with more volatile fluids of lower surface tension before drying. Figure III 6. Hollow fiber spinning set up: (1) spinning dope tank; (2) bore liquid vessel; (3) spinneret; (4) coagulation bath; (5) fiber guiding wheel; (6, 6 ) pulling wheels; (7) spinning line; (8) water spray; (9) fiber collecting wheel.
104 88 Chapter III Figure III 7. Image of the spinning line used for the fabrication of the asymmetric hollow fiber membranes (University of Twente). Figure III 8. The triple - orifice spinneret used for the fabrication of the asymmetric hollow fiber membranes (A: outer channel closed, B: dope channel, C: bore channel).
105 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane Permeation set-up Membrane permeation properties were determined using an experimental setof this thesis. The planar membrane module was replaced with a hollow fiber membrane module.. The Matrimid hollow up and procedure described in the Chapter II fiber module was built by insertion of 1 fiber of ~10 cm length within a tubular stainless steel container in a counter-flow configuration as shown in Figure III 9 and Figure III An epoxidic resin was used for sealing. The resulting membrane area was of 1.3 cm 2. The PPO hollow fiber module was used as received and was composed of 5 fibers 15 cm length with an outer fiber diameter of 0.53 µm. The resulting membrane area was of 12.5 cm 2 Figure III - 9. Hollow fiber module configuration Figure III 10. Hollow fiber module image
106 90 Chapter III The Matrimid hollow fiber module was pressurized with the feed gas mixture at the bore side and an argon sweep gas was passed through the fiber shell to remove and transport the permeate to a gas chromatograph (Agilent Micro GC 3000). Details on the analytical method are given in the Appendix II of this thesis. The feed flow was in counter-current with the argon sweep gas flow. A sweep gas was used due to the very low permeate flow rate that is obtained when a hollow fiber module is built from only one fiber with low permeability. This configuration allowed the removal of side effects like concentration polarization and thus ideal hydrodynamic conditions were achieved. In the case of the PPO hollow fiber module, because of the high gas permeability and a much higher membrane area, there was no need for the use of a sweep gas in the permate. Therefore, when we worked with pure gases the permeate and retentate gas streams were composed of pure gases and thus the gas chromatograph was not used. The permeance coefficient was calculated from known values of pressure and flow rate. When working with gas mixtures, the permate and retentate were analyzed with the recalibrated gas chromatograph with multiple gas mixtures of increasing gas concentration up to values of 90 vol %. The same analytical method was used. The feed gas pressure was measured at both the inlet and outlet ports of the membrane module. At the inlet port of the membrane module a pressure gauge (Swagelok PGI-40M-BC9-LANX) was inserted and at the outlet port, the pressure was indicated by a back pressure regulator (Brooks 5866), which controls the pressure in the feed side of the membrane. For the calculation of the gas permeability through the membrane the logarithmical mean between the pressures at the entrance and exit of the module (feed and retentate stream pressures) was used as total feed pressure at each phase Experimental procedure and operation conditions Matrimid hollow fiber In the gas separation experiments well aged fibers were used since the impact of physical aging over the permeation properties of Matrimid hollow fiber asymmetric membranes has been revealed to determine a decrease in the permeation of N2 in time even after 250 days of storage prior to permeation experiments . Before studying pure and mixed gas permeation, the occurrence of the concentration polarization phenomenon was studied in order to be avoided. This phenomenon was studied using the fibers labeled D1 - M3 by varying the feed flow
107 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane 91 rate for pure H2 and for binary mixtures H2/N2 = 50/50 (vol ratio) from 10 to 200 cm 3 (STP) min -1 at total pressures of 2, 4 and 6 bar and at a constant temperature of 30 o C. Then, pure and mixed gas permeation studies were carried-out at feed pressures ranging from 2 to 10 bar with H2, CO2, CO and N2 using the Matrimid hollow fibers membranes D1 M1, at a constant temperature of 30 o C. Permeation experiments with mixed gases were performed with binary mixtures (H2/CO2, H2/N2 and H2/CO) and with a quaternary mixture (H2/CO2/N2/CO) at compositions listed in Table III - 2 using the Matrimid hollow fiber membrane M1 and M3 developed as described in section Also, the influence of temperature over the permeance of mixed gases was analyzed for the quaternary H2/CO2/ N2/CO mixture of 16.3/5.3/60.7/17.8 (vol %), temperatures ranging from 30 to 130 o C at a pressure of 4 bar using the hollow fiber D1 M1. Table III - 2. Mixed gas compositions used for gas permeation experiments Gas mixture Compositions (vol %) H2/CO2 20/80, 40/60, 60/40, 80/20 H2/N2 20/80, 50/50, 80/20 H2/CO 20/80, 50/50, 80/20 H2/CO2/N2/CO /5.3/60.7/17.8 PPO hollow fiber Permeation experiments using PPO hollow fibers with pure gases were performed at pressure gradients within the range from 0.4 to 0.8 bar for H2, 0.4 to 1.2 bar for CO2 and 1 to 5 bar for CO and N2 at a constant temperature of 30 o C. When working at feed pressures higher than 1.8 bar for H2 and 2.2 bar for CO2, due to the high gas permeation flow of the 5 fiber module, the permeate flow rate was higher than the maximum capacity of the mass flow meter installed at the permeate side (10 cm 3 (STP) min -1 ) and therefore we could not further measure the gas permeance. Permeation experiments with mixed gases were performed with a quaternary mixture H2/CO2/N2/CO = 16.3/5.3/60.7/17.8 vol % in the pressure gradient range from 1 to 4.9 bar at a constant temperature of 30 o C.
108 92 Chapter III 3.3. RESULTS AND DISCUSSION Morphological and structural characterization Pure Matrimid hollow fibers The morphological and structural characteristics of the asymmetric hollow fibers were investigated using SEM analysis. Figure III 11 shows SEM images of the three pure Matrimid hollow fibers fabricated in this work. The Matrimid hollow fiber membranes displayed satisfactory cross-sectional circularity and concentricity with constant wall thickness. The values of the outer and inner diameters of the fibers were evaluated from an average of at least 4 cross-sectional SEM images taken from samples cuts at different length of the same fiber (Table III - 3). Table III - 3. Structural dimensions of Matrimid asymmetric hollow fiber membranes Membrane OD (µm) ID (µm) Skin layer thickness, δ (nm) H2 CO2 N2 CO D1 - M1 500±10 291± D1 - M2 427± ±1 not measured D1 - M3 381±13 143± The outer diameter of the fibers seems to increase as the air gap height decreases. The dimensions of the fiber D1 - M1 are practically equal to the dimensions of the spinneret. The effect of air gap height on the macroscopic dimensions of a hollow fiber is complex, the outer diameter can increase or decrease as the air gap height increases . All hollow fiber have a typical asymmetric structure; a dense thin top layer at the outside supported by a spongy porous substructure with isolated finger like macrovoids found at the internal wall. The macrovoids are more predominant for fiber D1 - M1, less for fiber D1 - M2 and inexistent for fiber D1 - M3. The presence of macrovoids is not detrimental as it does not influence the separation performance but only decrease the mechanical resistance of the membrane. For industrial high-pressure gas separation processes however, macrovoids should not be present in support structure.
109 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 93 post combustion mixtures using a Matrimid hollow fiber membrane Figure III SEM images of Matrimid hollow fibers, left - cross section; right detail of the dense skin layer: (A) fiber D1 - M1; (B) fiber D1 M2 and (C) fiber D1 M3.
110 94 Chapter III As shown in Table III 3, the thickness of the external dense skin layer (l) decreases when the air gap height decreases with values calculated from pure gas permeation data obtained at a feed pressure of 2 bar using Eq. (III - 1) for each gas: 10 III 1 where the permeability (Barrer) represents the intrinsic permeation property of the polymeric material that is obtained from pure gas permeation experiments with a dense Matrimid film of known thickness, and the permeance (GPU) is the transport flux per unit transmembrane driving force through a hollow fiber. The pure gas permeability of the Matrimid dense film and the hollow fiber permeance used for the calculation of the dense layer thickness in the asymmetric hollow fibers developed in this study are listed in Table III -4. The fiber dimensions and pure gas permeability results obtained in this work are comparable with published literature data (Table III 4). Table III - 4. Pure gas permeation data for Matrimid asymmetric hollow fibers at 30 o C. Mem. type P (bar) Permeance (GPU) Ideal selectivity H 2 CO 2 N 2 CO H 2/N 2 H 2/CO 2 H 2/CO CO 2/N 2 Hollow fiber D1 - M ± ± ± ± ± ± ± ± ± ± Hollow fiber D1 - M ±5.7 40± ± ±9.2 41± ± ±6.9 43± ± Matrimid dense (Barrer) (Barrer) (Barrer) (Barrer) film a Knudsen selectivity a : average values from the literature [12-17], 1 GPU = 1 x 10 6 cm 3 (STP) cm -2 s -1 cmhg -1
111 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane 95 According to Koros and co-workers , the thickness of the dense polymer layer in an asymmetric hollow fiber structure used for gas separation should have around 100 nm. However, as shown in Table III- 5 in general, the majority of studies achieved higher thickness values, showing the difficulty in obtaining such a thin layer thickness without surface defects. Among the published results, the hollow fiber fabricated by Favvas et al.  with an asymmetric layer thickness of 72.8 nm had low gas selectivity and were considered defective. Table III 5. Literature data for gas permeance and fiber dimensions of Matrimid based asymmetric hollow fiber membranes. Fiber dimensions Gas permeability (GPU) P OD (µm) Wall (µm) l (nm) He H 2 CO CO 2 CH 4 O 2 N 2 (bar) T ( o C) Ref   [9, 18]  a 0.2 a  a 0.2 a   b  a binary mixtures CO 2/CH 4 = 20/80 (vol%), b dual layer asymmetric hollow fiber (Polysulphone- inner layer, Matrimid/PBI=1/1 wt% blend outer layer) The results (Table III 3) from the calculation of the asymmetric layer thickness are quite different depending on the tested gas. In the literature [6, 23] the thickness of the dense layer is usually calculated with one gas, usually O2. The effect of film thickness on the gas permeation characteristics of glassy polymer membranes was thoroughly studied in literature and it was demonstrated that the use of the intrinsic dense film permeability data to estimate skin thickness from flux observations on asymmetric or composite membrane structures is a very approximate method . Another method consists of fitting permeability versus permeance data for a number of different pure gases in the same plot and to obtain the thickness from the
112 96 Chapter III slope  (see Figure III - 12). In our case the latter procedure gives an average value of 354 nm for fiber D1 - M1 when pure gas (H2, CO2, CO and N2) permeability versus permeance data obtained in the feed pressure range between 2 to 10 bar are plotted together (Figure III 12). This result is close to the thickness calculated from permeability/permeance data using pure H2, since the slope value is actually determined by the gas with the highest permeance. The dependence in the value of the dense layer thickness on the tested gas indicates a complex morphology of the external asymmetric skin that is discussed later in section Figure III 12. Permeability versus permeance plot for the determination of the Matrimid hollow fiber asymmetric layer thickness
113 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane 97 Matrimid PBI blend hollow fibers Figure III 13 shows SEM images of the two hollow fibers obtained from the Matrimid PBI polymer blend. The fiber D2 is hollow with satisfactory crosssectional circularity and concentricity and with constant wall thickness, but does not have a porous structure, it seems that it has a dense morphology over the entire wall. For the formulation of the fiber D3 dope, EtOH non solvent was added as means of approaching decomposition and thus achieving a porous morphology. As shown in Figure III 13 (B) this procedure was somewhat successful, a spongy like structure morphology was obtained with a low pore size, but the inner diameter of the fiber D2 is too small. Also, a lack of mechanical stability was observed for both fibers. Dense films from Matrimid/PBI=1/1 (wt%) polymer blend were also prepared following strictly the same recipe developed in literature . The resulted dense films presented a good morphology but they also had a lack of mechanical stability. The films were so brittle that it broke when transmembrane pressure of 2 bar was applied. The recipe needs further improvement and the use of a dual layer hollow fiber spinning process must be contemplated . Figure III SEM images of Matrimid:PBI=1:1 hollow fibers, left - cross section; right - detail of the shell: (A) fiber D2 cm; (B) fiber D3.
114 98 Chapter III Gas permeation through asymmetric Matrimid hollow fibers Concentration polarization phenomena The occurrence of concentration polarization phenomena was not found at the feed side of the membrane in the case of the permeation of pure H2 whose permeance values remained constant with the feed flow rate. In contrast the concentration polarization phenomenon was found for H2/N2 mixtures at feed flow rates lower than 50 cm 3 min -1 as depicted by Figure III 14. Therefore, for further gas permeation experiments the feed flow rate and the sweep gas flow rate were kept constant at 100 cm 3 (STP) min -1 and at 10 cm 3 (STP) min -1 respectively. Figure III 14. The effect of feed gas flow rate on H2 permeance at 30 o C and feed pressures of 2, 4 and 6 bar for mixtures H2/N2 = 50/5 (vol ratio), using membrane D1 - M3. Pure gas permeation Pure gas permeance and ideal selectivity data are listed in Table III - 4. All data represent an average from several runs. The permeance of all gases is higher for membrane D1 - M3 than for membrane D1 - M1. In the case of membrane D1 - M3, the different gas pair values of ideal selectivity are low (15.7% of the intrinsic selectivity of a dense film for H2/N2 gas pair) and approaching the Knudsen selectivity showing that this hollow fiber possesses important surface defects. In literature, asymmetric hollow fiber membranes with a gas selectivity of only 55% of a dense film values where considered to be moderately defective membranes meanwhile those with a gas selectivity equal with the Knudsen selectivity where considered to be severely
115 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane 99 defective membranes . To recover the intrinsic selectivity of the material, usually a post-treatment by applying a PDMS coating is applied. This method is not attractive at commercial scale and therefore we preferred to further use in our study the defect free fiber D1 M1. It can be observed that the developed Matrimid hollow fiber D1 - M1 possesses gas permeance and ideal selectivity values similar to published data for commercial hollow fiber membrane used for H2 separation and recovery, with selectivity values of 80 and 50 for H2/N2 and H2/CO respectively [4, 27]. As it can be calculated from the values reported in Table III 4, the ideal selectivity values of the hollow fiber membrane D1 - M1 for the gas pairs H2/N2 and H2/CO are of 67 % and 78 % of a dense Matrimid film. In contrast, at 2 bar the selectivity of H2/CO2 gas pair is of 150 % of dense film. These contrary results show again the complexity of the asymmetric layer morphology. Between the skin layer and the porous substrate a transition layer (substructure) can exist. This transition layer might have small enough pores to determine gases to flow in a Knudsen regime and to contribute substantially to the overall membrane resistance, as previously has been reported by Koros et al. [28, 29]. The gas transport through porous membranes in the Knudsen regime is slow and comparable to the one governed by solution-diffusion mechanism in dense membranes and it takes place when the pore radius is lower than 0.05 times the mean free path (λ) of the gas molecules . λ increases in the following order: CO2 < N2 < CO < H2 with noticeable higher values for H2. At 1 bar and K the λ values for CO2, N2, CO and H2 are listed in Table III 6 and are calculated using Equation III - 2  2. III 2 where R is the general constant of gases (8.31 J mol -1 K -1 ), T is the temperature (K), NA is the Avogadro s number (6.023 x ), d (m) is the molar average collision diameter with values taken from Hirschfelder  and p (Pa) is the pressure. The resulting λ values have the unit in meter. Table III 6 also, lists the d values of the gases of interest in our work. The much higher λ value for H2 than for the N2, CO and CO2 determines a pore radius range in which the transport of H2 is in Knudsen regime meanwhile the transport of CO, N2 and CO2 is faster (slip flow for pore radius between 0.05 λ and 50 λ or viscous flow for pore radius higher than 50 λ). At 1 bar this range is between 3.43 nm (= 0.05λ CO) and 5.55 nm (= 0.05 λ H2). A higher contribution of Knudsen flow to the transport of H2 than to the transport of CO and N2 could determine a higher
116 100 Chapter III overall resistance to the transport of H2 and therefore the lower H2/CO and H2/N2 selectivity values experienced for hollow fibers than those obtained for dense films. Table III 6. The values of the molar average collision diameter, d, and gas mean free path, λ. Gas d (nm) λ (nm)* H CO N CO *λ values were calculated at 1 bar and K If only Knudsen transport resistance is assumed for the substructure then also the H2/CO2 selectivity should be lower for hollow fibers than for dense membranes, but quite on the contrary this value is higher and therefore the overall membrane resistance is higher for CO2 than for H2. For the transport of the more condensable CO2, a contribution of surface flow through porous media could be assumed . In surface flow mechanism a film of densely packed condensed molecules is formed at the pore wall interface and moves at a steady state velocity along the surface. Surface diffusion is a process that influences and occurs in parallel with Knudsen diffusion. The liquid film formed on the pore wall gas interface decreases the effective pore diameter and thus the contribution to the overall transport of Knudsen regime is increased. In order to evaluate the contribution of the substructure to the overall resistance a simple resistance model where skin and substructure resistance are considered to be connected in series can be considered as depicted by Figure III 15 [29, 30, 32]. Figure III 15. Resistances connected in series in composite membranes.
117 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane 101 In this case the following equations apply [29, 30, 32]. III 3 III 4 where Rtot is the total resistance to gas transport (reciprocal of the permeance), Rskin and Rsub refer to the skin layer and the substructure and subscripts a and b refer to two different gases. The skin layer resistance is given by the intrinsic value of the resistance of a dense film. Therefore, the ratio of the resistances for permeants a and b, that is the asymmetric layer selectivity, (αskin)a/b, is equal to the ratio of permeability of a to b of a dense film, that is the dense film selectivity, (αdense film)a/b: / / III 5 The ratio of the overall resistance for permeants a and b, of the hollow fibers is: / III 6 Substituting Eq. III 4 and III 5 into Eq. III 6, gives: / / / III 7 The rearrangement of Eq III 7 gives: / / / / 1 / III 8 If Knudsen selectivity is assumed for the microporous substructure selectivity, then using the intrinsic dense Matrimid selectivity values for H2/N2 and CO2/N2 gas pairs ( / and / ) the ratio of substructure resistance to skin layer resistance can be calculated at different transmembrane pressures. The results in terms of relative contribution of substrate resistance to the overall membrane resistance for the hollow fiber membrane D1 - M1 are listed in Table III 7 and are calculated from the values reported in Table III - 4.
118 102 Chapter III Table III 7. The relative contribution of substrate resistance to the overall membrane resistance for the hollow fiber membranes D1 - M1 towards the permeation of pure H2 and CO2 Pressure (bar) Rsub/Rtot (%) H2 CO From the values reported in Table III 7 it can be noticed that an important contribution to the overall transport resistance through the hollow fiber membrane is given by the substructure, with values as high as 61 % for CO2 at 2.3 bar and K. In the case of H2, the pressure does not have a significant effect over the substructure resistance. This indicates that the transport of H2 through the porous substructure is driven only by a Knudsen mechanism since the Knudsen coefficient is constant with pressure. Although for the calculation of the Rsub/Rtot (%) values for CO2 only Knudsen flow was assumed, the variation with pressure of this fraction indicates a contribution of the surface flow to the transport of CO2. Assuming a Henry s law for the gas adsoption on the pore wall, the amount of gas adsorbed in the polymer material increases with pressure and therefore the contribution of the substructure resistance to the total resistance increases. In the case of fiber D1 - M1, another remarkable aspect is that, in the pressure range studied, from 2 to 10 bar, H2, CO and N2 pure gas permeance data (see Table III - 4) remained almost constant with pressure. In contrast, the permeance of CO2 strongly rose, reaching an increase of 42% from 2 to 10 bar. This tendency in the permeation of condensable gases like CO2 is already very well documented in the literature for asymmetric hollow fibers, thin and thick planar membranes and it is attributed to plasticization phenomena [33, 34]. In the literature it has been reported that in dense Matrimid thick films (thickness around 30 µm) the permeability of CO2 first decreases with pressure until it reaches a minimum at 15 bar at 35 o C  and at 12 bar at 22 o C  from which it begins to increase. The decrease in gas permeability is related to the decrease in gas solubility coefficient with pressure since the polymer sorption sites found in the polymer matrix become saturated with gas molecules at increasing values of pressure. At the
119 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane 103 plasticization pressure, the polymeric chain packing is disrupted by the penetrant molecules due to the increase in the segmental mobility that expands both the frequency and the average size of transient gaps that enable diffusion, thereby increasing the permeability. It was reported in literature that in Matrimid thin films (thickness below 5.2 µm)  or for even thinner films as those obtained in asymmetric hollow fibers, the minimum may even disappear and the permeability increases immediately from low feed pressures. The accelerated plasticization is assumed to occur because of the steep swelling induces stress gradients related to the thinner membrane / film thickness . Comparative results for the variation with pressure of CO2 permeance in Matrimid hollow fibers were previously reported in other studies . In our work, the different trend in the transport rate of H2 and CO2 determines a decrease in the H2/CO2 ideal selectivity with pressure from a value of 5.0 at 2 bar to 3.4 at 10 bar as shown in Table III - 4. Mixed gas permeation Figure III - 16 shows the permeation results for H2 transport from binary H2/CO2 feed mixtures plotted against the fugacity of H2 (Fig. III - 16.a) and plotted against the fugacity of CO2 (Fig III- 16.b) at different total feed pressures for the hollow fiber D1 M1. In comparison with pure gas permeation results, the permeance of H2 in mixtures is lower and, for a constant gas composition, it decreases at increasing total feed pressure, i.e., when the fugacity of both H2 and CO2 increases. This phenomenon is related to the competitive sorption between H2 and CO2 for the sorption sites which are associated to the excess (non-equilibrium) free volume fraction of the polymer . Working with a gas mixture the availability of the sorption sites for one component is lowered due to the presence of the other component and thus its transport rate is also lowered when it is compared with pure gas transport rate. While H2 is a relatively inert and fast permeating gas whose transport rate is diffusion based, CO2 is a more condensable gas and possesses higher solubility in membranes. Therefore the polymer sorption sites are preferentially occupied with CO2 than with H2 leading in both hollow fiber and flat membranes to a higher decay in the permeability of H2 than in the permeability of CO2, for H2/CO2 gas mixtures with respect to pure gases.
120 104 Chapter III Figure III H2 permeance variation as function of the fugacity of H2 (a) and of CO2 (b) for H2/CO2 mixtures and pure H2 in asymmetric Matrimid hollow fiber membranes D1 M1. The lines are drawn to guide the eye.
121 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane 105 In flat membranes (see Chapter II 2.4.2, Figure II - 15) the mixed gas permeation of H2 was dependant of only the fugacity of CO2; i.e., equal values for the H2 mixed gas permeability data were obtained for H2/CO2 mixtures when the fugacity of CO2 was kept constant and the fugacity of H2 was increased. In contrast in hollow fiber membranes this behavior is not repeatable and lower H2 permeance values were obtained at higher fugacity of H2 for the same fugacity of CO2 (see Fig. III - 16.b.). The explanation of such behavior will be discussed later on after analyzing the CO2 permeation data. Figure III - 17 shows the permeation results for CO2 transport in binary H2/CO2 mixtures plotted against the fugacity of CO2 for different feed composition in the range H2/CO2 = 20/80 to H2/CO2 = 80/20. The maximum operating pressure was 10 bar and therefore the maximum attainable fugacity of CO2 in the mixture H2/CO2 = 80/20 was of 2 bar. The permeance of CO2 decreased with its fugacity for the H2/CO2 mixture of 80/20 (vol %), remained practically constant for the mixture H2/CO2 = 60/40 (vol %) and for the rest of the mixtures (with CO2 concentration > 40%) the CO2 permeance increases as the concentration of CO2 in the mixtures increased, reaching values close to pure CO2 permeance data. This tendency corresponds to a balance between two contrary effects that affect CO2 transport through a thin Matrimid layer: competitive sorption and plasticization phenomenon for H2/CO2 mixtures in hollow fibers. While plasticization increases the permeation of CO2 with pressure, competitive sorption between H2 and CO2 determine a decrease in the permeation of CO2. As shown in the Chapter II, section 2.4.2, using thick planar Matrimid films plasticization was not found and the permeability of CO2 obtained with H2/CO2 mixtures was slightly lower than pure gas permeability and presented a similar behavior of decreasing permeability with increasing CO2 fugacity  (also, see Figure II 17 from Chapter II). In Matrimid hollow fibers, at high concentration of H2 in the H2/CO2 mixture, competitive sorption prevails and the permeance of CO2 decreases with its fugacity. As the concentration of CO2 increases, plasticization counteracts competitive sorption and equality between the two phenomena is reached when the permeance of CO2 remains constant with its fugacity. At high concentration of CO2 in the H2/CO2 mixture plasticization dominates the transport rate of CO2 and the permeance of CO2 increases with its fugacity. Similar results were reported in literature for CO2/CH4 mixtures in Matrimid asymmetric hollow fiber membranes. In some studies [10, 37, 38] plasticization was dominant at high CO2 feed gas concentrations (80 vol % CO2) while competitive sorption effects were dominant at low CO2 feed gas concentrations (20 vol %). In another study  working with a 10/90 (vol %) CO2/CH4 feed mixture competitive sorption was also dominant and the permeance of CO2 decreased with CO2 partial pressure.
122 106 Chapter III Figure III CO2 permeance variation with its fugacity for H2/CO2 mixtures and pure CO2 in asymmetric Matrimid hollow fiber membrane D1 - M1. The lines are drawn to guide the eye. Plasticization of the membrane by CO2 can also affect the transport rate of H2. Figure III - 18 shows the ratio between H2 permeance and respectively permeability values obtained working with pure gas and binary H2/CO2 feed mixtures for asymmetric hollow fibers and dense films. The effect of using thin asymmetric layers in hollow fiber (fiber D1 - M1) structure versus planar thick Matrimid films is also resembled.
123 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane 107 Figure III Hollow fiber M1 vs. planar dense membrane comparative study for the depression in the permeation of H2 for H2/CO2 mixtures in respect to pure gas, at total feed pressure of 4 bar (a) and 6 bar (b). The pure and mixed gas H2 permeability values for planar films were reported in Chapter II, section of this thesis. At a total feed pressure of 6 bar the decay in the permeation values of H2 in respect to pure gas values is higher for Matrimid films than for hollow fibers: in Matrimid planar films the decay was of 45% meanwhile the decay in the hollow fibers the decay was of only 21%. Under the used operating conditions, in dense Matrimid films the CO2 plasticization phenomena was not found, and only the competitive sorption phenomena was present, thus we can conclude that the CO2 plasticization phenomena found in the permeation of H2/CO2 mixtures trough Matrimid hollow fibers determines higher permeation values for H2. This is better explained in terms of so called transport plasticization that can occurs in the presence of highly sorbing penetrants, which are capable of swelling the polymer matrix to introduce additional free volume that enable higher values for penetrant diffusion . As shown in Figure III - 16, for mixtures with a higher concentration in H2 and the same concentration in CO2 the plasticization with CO2 is lower, competitive sorption phenomenon dominates and thus the decay in the permeation of H2 with respect to pure gas is higher. Hollow fiber mixed gas selectivity values, calculated as described in Chapter I, section Eq. I 9, have been plotted in Figure III - 19 for H2/CO2 mixtures.
124 108 Chapter III Figure III H2/CO2 selectivity variation with the fugacity of H2 for binary H2/CO2 mixtures in asymmetric Matrimid hollow fiber membranes. The lower permeation of H2 in binary H2/CO2 mixtures determines a considerably lower selectivity for the H2/CO2 gas pair than the ideal selectivity. The mixed gas selectivity strongly varies with gas composition and pressure with values of α = 3.1 for the 20/80 H2/CO2 mixture at a total pressure of 10 bar and H2 fugacity of 2 bar compared to 4.6 for the 80/20 H2/CO2 mixture at total pressure of 2 bar. The selectivity values are lower for mixtures than for pure gases but are higher than the average mixed gas selectivity obtained with planar membranes with a value of 2.7. Two factors might contribute to determine this difference: a lower depression in the transport rate of H2 in H2/CO2 mixtures for hollow fiber than for dense films and a higher substructure resistance towards the transport of CO2. In the case of the mixtures of H2 with relatively more inert gases: N2 and CO the permeance values for H2 are close to pure gas values and are slightly lower when the copartner for H2 was CO (Figure III - 20). This demonstrates that between H2 and N2 or CO only slight competitive sorption effects are found, which are relatively stronger for H2/CO mixtures than for H2/N2 mixtures. Contrary to other report , there is no plasticization phenomena present in H2/CO mixtures or for pure CO whose permeance is constant within the pressure range 1-10 bar (see Table III - 4). These results are consistent with published literature data for pure H2 and CO and for H2/CO mixtures in another polyimide membrane .
125 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane 109 Figure III H2 permeance variation with its fugacity for pure H2, binary H2/N2, H2/CO and quaternary H2/CO2/N2/CO gas mixtures and in asymmetric Matrimid hollow fiber membrane D1 - M1. Figure III - 20 also shows H2 permeance values for the quaternary H2/CO2/N2/CO mixture. With respect to pure gas permeability a small percentage of CO2 (5.36 vol %) as it is found in the tail gas from carbon black manufacturing determines a 12 % decrease in the permeance values for H2 working at a total feed pressure of 8 bar. The concentration of H2 in the permeate stream leaving the hollow fiber membrane module was between 87 and 89 vol % calculated if Ar sweep gas is not taken into account. We assume that under industrial operating conditions the concentration of H2 in the permeate stream is expected to be somehow lower, since our experimental values were obtained close to ideal operation conditions: counter currently plug flow and very low stage cut.
126 110 Chapter III Temperature effect over mixed gas experiments The influence of temperature over the permeance of mixed gases was analyzed for the quaternary H2/CO2/N2/CO mixture of 16.3/5.3/60.7/17.8 (vol %) at temperatures ranging from 30 to 130 o C and a pressure of 4 bar and a constant feed and sweep gas flow rate of 100 cm 3 (STP) min -1 and of 10 cm 3 (STP) min -1 respectively. This mixture represents a synthetic mixture similar to the dry post combustion gas stream obtained in the production of carbon black. As temperature increased all four gas permeabilities increased. Arrhenius plots are represented in Figure III - 21 showing an Arrhenius - type dependence with temperature for temperatures up to 110 o C. At temperatures higher than 110 o C the permeance of all gases had lower values than the corresponding to the Arrhenius type dependence. Matrimid hollow fiber membranes were reported to maintain stable permeation properties at temperatures up to 150 o C . In the case of the hollow fibers obtained in this work, at T > 110 o C, we assume that the decay in permeance can be attributed to structural modifications in the morphology of the membrane. The reorientation of the polymeric chains in order to attain equilibrium is faster and a possible densification can occur under the pressure working conditions. The specific Arrhenius parameters (the permeation activation energy, Eap and P0) for permeance of H2, CO2, N2 and CO in the synthetic mixture were calculated (Table III - 8). The Eap values for H2 and CO2 are similar to those obtained in planar dense membranes (see Table II - 4). On the other hand the Eap values obtained for N2 and CO are lower than in planar dense membranes, giving the following order in the increase of the Eap: CO2 < N2 < CO < H2. Figure III- 21. The permeance of mixed H2/CO2/CO/N2 = 16.3/5.3/60.7/17.8 (vol %) as a function of temperature at 4 bar feed pressure.
127 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane 111 Table III 8. Arrhenius parameters for CO2, N2, H2 and CO permeation through a Matrimid hollow fiber membrane for quaternary H2/CO2/N2/CO mixture of 16.3/5.3/60.7/17.8 (vol %) Arrhenius parameters Gas N2 H2 CO2 CO P0 (GPU) EaP (kj mol -1 ) Figure III 22 shows the effects of temperature on the mixed gas selectivity for H2/CO2, H2/N2, H2/CO and CO/N2 separations through the Matrimid hollow fiber membrane. The mixed gas selectivity / increases with temperature from a value of 5.33 at 30 o C to 7.0 at 110 o C. The selectivity of the other gas pairs is almost constant with temperature with an average value of 109 for /, 40 for / and with a slight increase from a value of 1.8 at 30 o C to 2.8 at 30 o C for / Figure III 22. Mixed gas selectivity variation with the temperature for (a) H2/CO2, N2/CO and (b) H2/N2, H2/CO gas pairs at 4 bar feed pressure for a quaternary H2/CO2/N2/CO mixture of 16.3/5.3/60.7/17.8 (vol %), through Matrimid hollow fiber membranes.
128 112 Chapter III Gas permeation through asymmetric PPO hollow fibers The use of asymmetric hollow fibers based on PPO material is generally for the easy task separation of O2 from N2. Therefore the use of the highly permeable PPO is advantageous for achieving high gas productivity. In this work it was decided to perform a comparative study between hollow fiber membranes made of materials with contrasting gas permeation properties (Matrimid and PPO). However we found experimental difficulties related with the analysis of PPO hollow fibers. A more thoughtful research is needed and the few results obtained are herein given. Table III 9 lists the permeance and ideal selectivity values for the pure gas permeation through the PPO asymmetric hollow fiber module obtained at a pressure gradient of 1 bar and 30 o C. All data represent an average from several duplicates. The different gas pair values of ideal selectivity are similar to published data for PPO dense films. Literature published data for the gas permeability coefficient through PPO membranes is found in a wide range of values. It was shown that the casting solvent has an important influence over the gas permeability through PPO planar films . However, the fabrications conditions of the commercial PPO asymmetric hollow fibers used in this work are proprietary and not known. The thickness of the external dense skin (δ) was calculated fitting permeability versus permeance data for H2, CO2, CO and N2 pure gases (see Figure III - 23) and an average value of 39.5 nm was obtained in the feed pressure range between 2 to 10 bar. This result is similar to the asymmetric layer thickness of approximately nm as referenced by the provider (Parker Filtration). Table III - 9. Pure gas permeation data for PPO asymmetric hollow fibers and dense films. Mem. type Permeance (GPU) or Permeability (Barrer) Hollow fiber PPO dense film a Ideal selectivity H2 CO2 N2 CO H2/N2 H2/CO2 H2/CO CO2/N2 2152± ± ± a : values from literature [25, 45, 46]
129 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane 113 Figure III 23. Permeability versus permeance plot for the determination of the PPO hollow fiber asymmetric layer thickness Figure III 24. Pure and mixed gas permeance variation with the pressure gradient for the asymmetric PPO hollow fiber membranes.
130 114 Chapter III Figure III 24 shows that in the narrow pressure range studied pure gas permeance data remained constant with pressure for all components. In contrast to Matrimid asymmetric hollow fiber membranes, CO2 plasticization phenomenon was not found in the PPO membranes. In literature, when mixed gas permeation (CO2/CH4) was analyzed for asymmetric hollow fiber membranes based on several polymers (cellulose acetate, Matrimid, PPO) and polymer blends (polyethersulfone/matrimid, polyimide P84/Matrimid, Matrimid), PPO membranes appeared to be less susceptible to plasticization, but gave low mixed gas CO2/CH4 selectivities . When analyzing the mixed gas permeation data, it is noticed that the mixed gas permeance of H2 and CO2 is considerably lower than for pure gases and it has decreasing values as the total pressure gradient increases. On the other hand, the mixed gas permeance of CO and of N2 is similar to pure gas permeance. We assume that the pure gas permeance data for H2 and CO2 has significant experimental error due to the experimental difficulties encountered in the measurement of the transmembrane pressure. On the other hand, when we worked with the quaternary gas mixture that has a high concentration of low permeating N2 we were able to increase the feed gas pressure to considerably higher values and thus we could precisely know and control the operation conditions. Considering also that the mixed and pure gas permeance coefficients for N2 and CO are similar, we assume that the mixed gas permeation data has a low experimental error. Therefore it can be concluded that the decrease in the permeance coefficient for H2 and CO2 for the quaternary gas mixture is again determined by competitive sorption effects. The concentration of H2 in the permeate stream leaving the hollow fiber membrane module was of only 40 vol % meanwhile for the Matrimid hollow fiber module was of 89 vol%. At the same time, the mixed gas solubility coefficient for the various gas pairs of interest are significant lower in the PPO membranes than in the Matrimid membranes. The H2/N2 and H2/CO mixed gas selectivity varied from 20 to 5 and 15 to 5 respectively in the pressure range studied for the quaternary gas mixture H2/CO2/N2/CO = /5.3/60.7/17.8. The H2/CO2 mixed gas selectivity was constant with a value of 2.
131 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane CONCLUSIONS Distinct gas separation performance was found for Matrimid asymmetric hollow fibers with respect to planar membranes fabricated from the same polyimide. First, in the case of pure gas permeation, a higher membrane substructure resistance for CO2 than for H2 followed by N2 and CO determines a higher H2/CO2 and lower H2/N2 and H2/CO ideal separation factors with respect to planar membranes. As in planar dense membrane, the permeance of H2, N2 and CO remained almost constant with pressure (up to 10 bar) with average values of 65.8 GPU for H2, 0.93 GPU for N2 and 1.63 GPU for CO. In contrast, the permeance of CO2 strongly increased with pressure, with values of 13.4 GPU at 2 bar and 19.1 GPU at 10 bar, showing a contrary behavior to planar membranes. This is related to an CO2 induced accelerated plasticization in the asymmetric hollow fiber membrane due to a much thinner dense skin layer compared to the usual thickness of an planar dense membrane (0.1 ~ 0.5 µm compared to 30 µm). In the case of the permeation of gas mixtures, as in planar membranes, competitive sorption effects determine a decrease in the permeation of H2 with respect to pure gas. For H2/CO2 binary mixtures this depression is higher than for H2/N2 or H2/CO mixtures for which is almost null. Due to plasticization induced higher transport rate of H2, in H2/CO2 mixtures, the decay in the permeation of H2 is not as high as in planar membranes. A maximum decay in the permeation of H2 of 21 % was reached at H2 fugacity below 1 bar at 6 bar total feed pressure, meanwhile in the planar membrane the decay was of 46 % in the same conditions. These results determine a strong variation of the mixed gas H2/CO2 selectivity with the composition and pressure with values ranging from 4.6 to 3.1. These values are higher than in planar membranes, the minimum of 3 reached for the composition H2/CO2 = 20/80 at 10 bar total pressure of 3.1 approaches the average value of 2.9 obtained in planar membrane. In contrast with Matrimid hollow fiber membranes the use PPO hollow fiber membranes gives considerably higher gas permeability at the expense of lower gas selectivities. Thus, when a feed gas mixture with a similar composition to the post combustion dry flue gas coming from carbon black manufacturing was used (H2/CO2/N2/CO = 16.3/5.3/60.7/17.8 vol %), the H2 concentration in the permeate of a PPO hollow fiber module was of only 40 vol % meanwhile the Matrimid hollow fiber module was more than double (87-89 vol %). It makes clear that use of thick film data to design or select membrane materials only gives a rough approximation of the performance that might be realized in practice. Our results suggest that for H2 mixtures that contain CO2 the hollow fiber membrane performance is better than of planar membranes.
132 116 Chapter III References 1. M. Mulder, Basic Principles of Membrane Technology, Kluwer Academic Publishers, Dordrecht, D.M. Koenhen, M.H.V. Mulder, C.A. Smolders, Phase separation phenomena during the formation of asymmetric membranes., J. Appl. Polym. Sci. 21 (1977) J.G. Wijmans, J. Kant, M.H.V. Mulder, C.A. Smolders, Phase separation phenomena in solutions of polysulfone in mixtures of a solvent and a nonsolvent: relationship with membrane formation, Polymer 26 (1985) R.W. Baker, Membrane Technology and Applications, 2nd edition ed., John Wiley and Sons, New York, P.Z. Çulfaz, Microstructured hollow fibers and microsieves: Fabrication, characterisation and filtration applications, PhD dissertation, University of Twente (2010). 6. D.T. Clausi, W.J. Koros, Formation of defect-free polyimide hollow fiber membranes for gas separations, J. Membr. Sci. 167 (2000) S.S. Hosseini, N. Peng, T.S. Chung, Gas separation membranes developed through integration of polymer blending and dual-layer hollow fiber spinning process for hydrogen and natural gas enrichments, J. Membr. Sci. 349 (2010) G. Dong, H. Li, V. Chen, Factors affect defect-free Matrimid hollow fiber gas separation performance in natural gas purification, J. Membr. Sci. 353 (2010) J.S. Lee, W. Madden, W.J. Koros, Antiplasticization and plasticization of Matrimid asymmetric hollow fiber membranes-part A. Experimental, J. Membr. Sci. 350 (2010) T. Visser, N. Masetto, M. Wessling, Materials dependence of mixed gas plasticization behavior in asymmetric membranes, J. Membr. Sci. 306 (2007) S.A. McKelvey, D.T. Clausi, W.J. Koros, A guide to establishing hollow fiber macroscopic properties for membrane applications, J. Membr. Sci. 124 (1997) H.-Y. Zhao, Y.-M. Cao, X.-L. Ding, M.-Q. Zhou, Q. Yuan, Effects of cross-linkers with different molecular weights in cross-linked Matrimid 5218 and test temperature on gas transport properties, J. Membr. Sci. 323 (2008) S. Shishatskiy, C. Nistor, M. Popa, S.P. Nunes, K.V. Peinemann, Polyimide asymmetric membranes for hydrogen separation: Influence of formation conditions on gas transport properties, Adv. Eng. Mat. 8 (2006)
133 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane H.-W. Rösler, Membrantechnolgie in der Prozessindustrie - Polymere Membranwerkstoffe, Chem. Ing. Tech. 77 (2005) S.S. Hosseini, M.M. Teoh, T.S. Chung, Hydrogen separation and purification in membranes of miscible polymer blends with interpenetration networks, Polymer 49 (2008) Y. Zhang, I.H. Musselman, J.P. Ferraris, K.J. Balkus Jr., Gas permeability properties of Matrimid membranes containing the metal-organic framework Cu-BPY-HFS, J. Membr. Sci. 313 (2008) O.C. David, D. Gorri, A. Urtiaga, I. Ortiz, Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid membrane, J. Membr. Sci. 378 (2011) S.B. Carruthers, G.L. Ramos, W.J. Koros, Morphology of integral-skin layers in hollow-fiber gas-separation membranes, J. Appl. Polym. Sci. 90 (2003) E.P. Favvas, G.C. Kapantaidakis, J.W. Nolan, A.C. Mitropoulos, N.K. Kanellopoulos, Preparation, characterization and gas permeation properties of carbon hollow fiber membranes based on Matrimid 5218 precursor, J. Mater. Process. Technol. 186 (2007) L. Jiang, T.-S. Chung, D.F. Li, C. Cao, S. Kulprathipanja, Fabrication of Matrimid/polyethersulfone dual-layer hollow fiber membranes for gas separation, J. Membr. Sci. 240 (2004) X. Ding, Y. Cao, H. Zhao, L. Wang, Q. Yuan, Fabrication of high performance Matrimid/polysulfone dual-layer hollow fiber membranes for O2/N2 separation, J. Membr. Sci. 323 (2008) S. Sridhar, R.S. Veerapur, M.B. Patil, K.B. Gudasi, T.M. Aminabhavi, Matrimid polyimide membranes for the separation of carbon dioxide from methane, J. Appl. Polym. Sci. 106 (2007) S.B. Carruthers, G.L. Ramos, W.J. Koros, Morphology of integral-skin layers in hollow-fiber gas-separation membranes, J. Appl. Polym. Sci. 90 (2003) Y. Huang, D.R. Paul, Effect of film thickness on the gas-permeation characteristics of glassy polymer membranes, Ind. Eng. Chem. Res. 46 (2007) V. Abetz, T. Brinkmann, M. Dijkstra, K. Ebert, D. Fritsch, K. Ohlrogge, D. Paul, K.-. Peinemann, S.P. Nunes, N. Scharnagl, M. Schossig, Developments in membrane research: From material via process design to industrial application, Adv. Eng. Mat. 8 (2006)
134 118 Chapter III 26. J.C. Jansen, M. Macchione, E. Drioli, On the unusual solvent retention and the effect on the gas transport in perfluorinated Hyflon AD membranes, J. Membr. Sci. 287 (2007) M. Peer, S.M. Kamali, M. Mahdeyarfar, T. Mohammadi, Separation of hydrogen from carbon monoxide using a hollow fiber polyimide membrane: Experimental and simulation, Chem. Eng. Technol. 30 (2007) D.T. Clausi, S.A. McKelvey, W.J. Koros, Characterization of substructure resistance in asymmetric gas separation membranes, J. Membr. Sci. 160 (1999) I. Pinnau, W.J. Koros, Relationship between substructure resistance and gas separation properties of defect-free integrally skinned asymmetric membranes, Ind. Eng. Chem. Res. 30 (1991) T. Matsuura, Synthetic Membranes and Membrane Separation Processes, 1st ed., CRC Press, Inc., Florida, J.O. Hirschfelder, C.F. Curtiss, R.B. Bird, The Molecular Theory of Gases and Liquids, John Wiley & Sons, Inc., New York, J.M.S. Henis, M.K. Tripodi, Composite hollow fiber membranes for gas separation: The resistance model approach, J. Membr. Sci. 8 (1981) S. Matteucci, Y. Yampolskii, B.D. Freeman, I. Pinnau, Transport of Gases and Vapors in Glassy and Rubbery Polymers, in: Materials Science of Membranes for Gas and Vapor Separation, John Wiley & Sons, Ltd, 2006, pp K. Simons, K. Nijmeijer, J.G. Sala, H. van der Werf, N.E. Benes, T.J. Dingemans, M. Wessling, CO2 sorption and transport behavior of ODPA-based polyetherimide polymer films, Polymer 51 (2010) A. Bos, I.G.M. Pünt, M. Wessling, H. Strathmann, Plasticization-resistant glassy polyimide membranes for CO2/CO4 separations, Sep. Purific. Technol. 14 (1998) A. Bos, I.G.M. Pünt, M. Wessling, H. Strathmann, CO2-induced plasticization phenomena in glassy polymers, J. Membr. Sci. 155 (1999) M. Wessling, M. Lidon Lopez, H. Strathmann, Accelerated plasticization of thin-film composite membranes used in gas separation, Sep. Purific. Technol. 24 (2001) T. Visser, M. Wessling, Auto and mutual plasticization in single and mixed gas C3 transport through Matrimid-based hollow fiber membranes, J. Membr. Sci. 312 (2008)
135 Mixed gas separation study for the hydrogen recovery from H2/CO/N2/CO2 post combustion mixtures using a Matrimid hollow fiber membrane T. Visser, G.H. Koops, M. Wessling, On the subtle balance between competitive sorption and plasticization effects in asymmetric hollow fiber gas separation membranes, J. Membr. Sci. 252 (2005) W.J. Koros, R.T. Chern, V. Stannett, H.B. Hopfenberg, Model for permeation of mixed gases and vapors in glassy polymers., J. Polymer Sci. Part A-2, Polymer physics 19 (1981) J.S. Lee, W. Madden, W.J. Koros, Antiplasticization and plasticization of Matrimid asymmetric hollow fiber membranes. Part B. Modeling, J. Membr. Sci. 350 (2010) K. Haraya, K. Obata, N. Itoh, Y. Shndo, T. Hakuta, H. Yoshitome, Gas permeation and separation by an asymmetric polyimide hollow fiber membrane, J. Membr. Sci. 41 (1989) W.J. Koros, D.G. Woods, Elevated temperature application of polymer hollow-fiber membranes, J. Membr. Sci. 181 (2001) D.M. Sterescu, D.F. Stamatialis, E. Mendes, J. Kruse, K. Rätzke, F. Faupel, M. Wessling, Boltom-modified poly(2,6-dimethyl-1,4-phenylene oxide) gas separation membranes, Macromolecules 40 (2007) D.M. Sterescu, D.F. Stamatialis, E. Mendes, M. Wübbenhorst, M. Wessling, Fullerene-modified poly(2,6-dimethyl-1,4-phenylene oxide) gas separation membranes: Why binding is better than dispersing, Macromolecules 39 (2006) A. Alentiev, E. Drioli, M. Gokzhaev, G. Golemme, O. Ilinich, A. Lapkin, V. Volkov, Y. Yampolskii, Gas permeation properties of phenylene oxide polymers, J. Membr. Sci. 138 (1998)
136 120 Chapter III
137 Chapter IV ON THE IMPROVED ABSORPTION OF CARBON MONOXIDE IN THE IONIC LIQUID 1-HEXYL-3- METHYLIMIDAZOLIUM CHLOROCUPRATE
138 122 Chapter IV
139 On the improved absorption of carbon monoxide in 1-hexyl-3-methylimidazolium chlorocuprate 123 ABSTRACT This chapter is focused on the design of a liquid phase system to be used in facilitated transport-supported ionic liquid membranes (SILMs) for the recovery of carbon monoxide from gaseous streams based on the ability of CO molecules to form π complexation bonds with Cu + ion. As liquid phase we propose the use of the ionic liquid 1-hexyl-3-methyl-imidazolium chlorocuprate prepared by the direct mixture of copper(i) chloride (CuCl) with 1-hexyl-3-methylimidazolium chloride ([hmim][cl]). A comprehensive look at the reaction mechanism and the equilibrium parameters obtained from the experimental characterization of the physical and chemical solubility of carbon monoxide in pure [hmim][cl], and in mixtures CuCl/[hmim][Cl] is presented. The gas equilibrium solubility experimental work was carried out in the CuCl/[hmim][Cl] molar ratio range from 0 to 0.75, temperature from K to K and pressures up to 20 bar. The values of the Henry s law constant for the physical solubility of CO in [hmim][cl] changed from 15.3 x 10-3 mol kg -1 bar -1 to 2.7 x 10-3 mol kg -1 bar -1 as the temperature increased from to K. The chemical solubility of CO in the reactive ionic liquid media increased with the increase of the concentration of CuCl, with the increase of pressure and with temperature decreasing. In the operation range of variables the maximum absorption of CO was of 2.26 mol kg -1 that was reached working at 20 bar, at CuCl/[hmim][Cl] molar ratio of 0.75 and K. These results are higher than reported values obtained using the COSORB solution (a CuAlCl4tol2 complex in toluene) that is industrially used , although the operation conditions are not equal. In the latter case, 1.3 mol l -1 CO was absorbed at CO pressures of 1 bar and a of 1.7 mol l -1 initial complex concentration. An equilibrium model that quantitatively describes the occurring reactions and phenomena was proposed and the equilibrium reaction parameters where determined. The calculated enthalpy of complexation presents a negative value of kj mol -1 and a reaction equilibrium constant, Keq with values between 8.5 and 16 Kg mol -1 in the temperature range from 30 o C to 0 o C was found.
140 124 Chapter IV 4.1. THE SELECTION OF CARRIER/SOLVENT SYSTEM The facilitated transport of carbon monoxide by a metallic salt was already studied in literature with water-based systems [2-4] and organic-based systems [5-8]. In Chapter I, Table I 7 of this thesis, a brief overview was made and the following extra remarks can be added. Water based systems: The solubility of CuCl in water is of only 1.1 x 10-3 M . It can be increased by forming cationic complexes with ammonia, amines and other basic ligands (alkanol amines or pyridine). This basic ligands also acts as stabilizing agents for Cu(I) against disproportion (Eq. IV 1) since in aqueous systems, the cupric state of copper is more stable than the cuprous state . The competitive equilibrium in such systems may be described by the following reactions: IV 1 IV 2 IV 3 IV 4 where L can be any type of ligand (a solvent, an anion, or a stabilizing agent) Copper(II) effectively coordinates ligands classified as hard bases, such as water, in reaction (IV - 2). This consumes cupric ions and drives reaction (IV - 1) to further disproportionation of cuprous ions. To prevent depletion of Cu(I) by this mechanism, reaction (IV - 3) must compete with reaction (IV - 2). This can be accomplished via introduction of a stabilizing ligand to retain Cu(I) in the monovalent state. For example, at 25 C the ratio between the equilibrium constant of the forward and backward reaction, K1 = 10 6 in pure water; in aqueous ammonia solution, K1 = 10-2 . On the other hand, adding a complexing stabilizing ligand decreases cuprous ion activity. A lower activity indicates decreased interactions with carbon monoxide. Another disadvantage of water based systems is that
141 On the improved absorption of carbon monoxide in 1-hexyl-3-methylimidazolium chlorocuprate 125 cuprous solutions are oxidized to the inactive cupric state when exposed to air (Eq. IV 4) Cuprous salts also dissolve readily in acidified solutions of various electrolytes with the formation of anionic complexes in the form, where x is determined by the ratio of the salt concentrations. The solubility of CuCl in aqueous solutions of KCl and HCl is in the range of M at 1.0 M KCl and 0.1 M HCl . The use of chloride ions as stabilizing ligands for the cuprous ion has several advantages. The chloride electrolytes have a negligible vapor pressure, minimizing the loss of solution components, they are less readily oxidized by oxygen and the disproportionation reaction is retarded. Noble et al. reported that facilitation factors as high as 20 were obtained in the transport of carbon monoxide when acidified solutions of CuCl were used as liquid media for supported liquid membranes . The facilitation factor increased with an increase of total carrier concentration and a decrease in feed gas concentration. A parasitic binding mechanism was proposed: IV 5 IV 6 Organic based systems: Nonaqueous copper solutions exhibit minimal disproportionation of cuprous ions and do not require addition of a stabilizing ligand . This is because the solvent often acts as a weakly complexing stabilizer. However, an inert (oxidizerfree) atmosphere must be maintained and moisture must be excluded to prevent disproportionation. Nearly all cuprous salts are quite soluble in coordinating solvents such as alkyl thiocyanates, alkyl sulfides, amines, and nitriles. Solubility in aromatics is generally low. However, cuprous aluminum tetrachloride (CuAlCl4) and cuprous tetrafluoroborate (CuBF4) form stable complexes with aromatics, leading to high solubility. Cuprous trifluoroacetate (CuCF3COO) dissolves in aromatics due to its low crystal energy . The facilitated transport of carbon monoxide with Cu(I) dissolved in DMSO using N-methylimidazole as ligand gave ideal separation factors CO/N2 of 36.9 .
142 126 Chapter IV Ligand-Cu(I) complexes based on various pyridylalkylamine compounds in THF as solvent have been proposed  with a structure example shown in the Figure IV - 1. High equilibrium constant with values ranging from M were found. Figure IV 1. The reaction scheme pyridylalkylamine Cu(I) based complexes with carbon monoxide. On the principle of improving the utility of metal ions as carriers via the formation of complex ions, other metal ions have also been used. Complex ions derived from macrocycles or other polydentate are attractive for studying the facilitated transport since they are relatively stable . The reversible binding of CO with several Fe(II) tetraimine complexes in benzonitrile was studied by Sharma et al. and Koval et al. [5, 6], and it was shown that the nitrile solvent ligands could be replaced by other ligands such as CO as illustrated in Figure IV 1. The stability of this complex towards oxidation in benzonitrile suggested the possibility of constructing of a membrane system for the separation of CO from O2. Low facilitation factors of maximum 2.8 were found for the Fe(Me2Ph2TIM) complex carrier and it was determined that the limiting factor is the solubility of the carrier.
143 On the improved absorption of carbon monoxide in 1-hexyl-3-methylimidazolium chlorocuprate 127 Figure IV 2. Structural drawing depicting the reversible 1:1 complexation reaction of Fe(II) macrocyclic complex ions with carbon monoxide, R1=R2=CH3, R3=H for Fe(TIM), R1=R2=R3=CH3 for Fe(Me4TIM) and R1=CH3, R2=C6H5, R3=H for Fe (Me2Ph2TIM) and R1=R2=R3=C6H5 for Fe(Ph4TIM). The separation of carbon monoxide from gas mixtures using palladium based complexes with 1,1,2- trichloroethane (TCE) as solvent has also been proposed in a continuous bench-scale apparatus consisting of absorber and stripper columns  (see Figure IV - 3). The binding of CO become stronger in turn as I is replaced by Br, Cl, or NCO. Only the Pd based complexes with Cl and Br had a satisfactory solubility of 0.15 and M respectively. Figure IV 3. Structural drawing depicting the reversible 1:1 complexation reaction of Pd(0) macrocyclic complex with carbon monoxide
144 128 Chapter IV Mass transfer, rather than reaction, was indicated as the controlling rate process. The kinetics were fast and high reaction equilibrium constant were obtained (35000 M -1 ) for Br based complex. As described in Chapter I, section of this thesis, the key issue in developing a supported liquid membrane separation process based on reversible complexation is the ability of a carrier to bind selectively to the permeant with appropriate equilibrium (Keq) and rate constants. The complexation reaction should be strong enough in order be selective, but should also be reversible in order for the permeating species to be released at the permeate side of the membrane. From the values reported in table I 7 it can be concluded that the magnitude of Keq for copper (I) based systems is within the recommended range by Noble et al  (2 x 10 2 M -1 and 2 x 10 4 M -1 ) and therefore copper (I) can be considered as the optimum carrier in membrane facilitated transport. Once the optimum metal carrier was identified, a solvent must be chosen also. We decided to use an ionic liquid as solvent as means to obtain stable SILMs due to their negligible vapor pressure and their high viscosity which could avoid solvent loss due to evaporation and also, slow down the displacement of the liquids from the micropores under pressure. Possible ionic liquids/carrier agent systems are summarized in Table IV 1. These systems are based on the supposition that the use as solvent of an imidazolium - based ionic liquid with the identical anion as the anion of the copper based salt will provide a successful solubilization for the copper (I) salt. For instance it is known that the mixture of CuCl with [Rmim][Cl] leads to a so called Lewis acid-based ionic liquid  where the metal halide CuCl acts as Lewis acid. Depending on the relative proportions of CuCl and [Rmim][Cl] several anionic species are present at equilibrium [15-18] as reported in Table IV - 2. Consequently [Rmim][Cl] based ionic liquids are able to solubilize high amounts of CuCl. Therefore, at this early research stage of the chemical absorption of carbon monoxide in ionic liquid media we decided to start with CuCl/[Hmim][Cl] based systems. The drawback of these types of ionic liquids is their water sensitivity; they absorb water from the atmosphere leading to their decomposition by hydrolysis . Also HCl can be formed, giving them a highly corrosive character. Furthermore, Cu (I) can disproportionate to Cu(II) and Cu 0. To avoid these phenomena, the samples should be stored in vacuum sealed vials or be quickly used after preparation. However these absorption media are by far more stable than aqueous medium.
145 On the improved absorption of carbon monoxide in 1-hexyl-3-methylimidazolium chlorocuprate 129 Table IV 1. Possible ionic liquids/carrier agent systems to be used as liquid phase in SILMs Ionic liquid 1-hexyl-3-methylimidazolium chloride, [Hmim][Cl] 1-octyl-3-methylimidazolium chloride, [Omim][Cl] 1-decyl-3-methylimidazolium chloride, [Dmim][Cl] 1-hexyl-3-methylimidazolium bromide, [Hmim][Br] 1-octyl-3-methylimidazolium bromide, [Omim][Br] 1-decyl-3-methylimidazolium bromide, [Dmim][Br] 1-hexyl-3-methylimidazolium iodide, [Hmim][I] 1-octyl-3-methylimidazolium trifluoromethanesulfonate, [Omim][OTf] 1-hexyl-3-methylimidazolium trifluoromethanesulfonate, [Hmim][OTf] 1-decyl-3-methylimidazolium trifluoromethanesulfonate, [Dmim][OTf] 1-hexyl-3-methylimidazolium acetate, [Hmim][Ac] 1-butyl-3-methylimidazolium trifluoroacetate, [Bmim][TfAc] Carrier agent Copper (I) chloride Copper (I) bromide Copper (I) iodide Copper(I) trifluoromethanesulfonate toluene or benzene complex: [CuOTf]2 C6H6 or [CuOTf]2 C7H9 Copper (I) acetate Copper (I) trifluoroacetate Table IV - 2. Anionic species presented in equilibrium at various molar ratios of CuCl and [Rmim][Cl] [15-18] Molar ratio CuCl/[Rmim][Cl] [0/1 1/1] Environment Reactions Basic (chlorine rich ) CuCl + 2 Cl CuCl + ncl CuCl 2 CuCl (n = 1, 2) (1+ n ) 2+ n Predominant anionic specie 2 CuCl 3 1/1 Neutral CuCl + Cl 2CuCl 2 CuCl 2 Cu 2Cl 3 + Cl CuCl 2 [1/1 2/1] Acidic (chlorine poor) CuCl + ycucl 2 (y = 1, etc.) Cu ycl y Cu 2Cl 3 Cu 3Cl 4
146 130 Chapter IV To conclude, this chapter studies the reactive absorption of CO in a copper (I) based ionic liquid formed by the mixture of [hmim][cl] and CuCl salt. The equilibrium parameters, namely the equilibrium constant, Keq, and the enthalpy of reaction, Hr, were evaluated. In addition new data for the physical solubility of CO in [hmim][cl] are also reported EQUILIBRIUM MODELING In order to describe the absorption process, an equilibrium model able to explain quantitatively the occurring reactions and phenomena is required. First we considered that all the copper (I) introduced in the reaction medium was active for the π-complexation reaction and that the strength of the π-bound formed between CO and the different copper based anionic species present at equilibrium (see Table IV - 2) was equal. Additionally, CuCl 2 is the most abundant copper chloride species 3 in the molar ratio of CuCl/[hmim][Cl] lower than 1 used in this work, according to [15-18] (see Table IV 2). Figure IV 4 shows a schematic depiction of the physical followed by the chemical solubility of CO in the ionic liquid media considered as absorption mechanism as previously found for propylene reactive absorption in Ag + /BmimBF4 based systems . The equilibrium reaction is shown in Equation IV - 7 for the case of a 1:1 copper (I):carbon monoxide complex. CO + 2 CuCl 3 Cu ( CO) Cl (IV 7) 2 3 The equilibrium constant is defined as follows, 2 [ Cu( COCl ) 3 ] K eq = (IV 8) 2 [ CO] [ CuCl ] 3 2 where [ Cu ( CO ) Cl ] is the equilibrium concentration of the complex, [CO] is 3 the equilibrium concentration of physically absorbed carbon monoxide into the 2 ionic liquid and [ CuCl ] is the equilibrium concentration of copper (I) chloride anionic specie. 3
147 On the improved absorption of carbon monoxide in 1-hexyl-3-methylimidazolium chlorocuprate 131 Figure IV 4. Schematic depiction of physical followed by chemical solubility of CO in ionic liquid media The concentration of physically dissolved carbon monoxide is given by the Henry s law, [ CO ] =k p (IV 9) H CO where kh is the Henry s constant (mol kg -1 bar -1 ) and pco is the partial pressure of carbon monoxide that is equal to the total pressure in the system when working with pure gases. The following mass balance equations can be applied, where the equilibrium concentration of the total absorbed CO, [CO]T, is obtained from the sum between the physically and chemically absorbed gas, Equation (IV- 10), and the concentration of copper (I) chloride anionic specie at equilibrium is given by the difference between 2 the initial concentration, [ CuCl 3 ] 0, and the equilibrium concentration of the complex specie, Equation (IV 11).
PHYSICAL SOLVENTS FOR ACID GAS REMOVAL Marek Ściążko, Prof. Schematic of a CCS system Technical options for CO2 capture Schematic of a coal-fired power plant with post-combustion CO2 capture Amine-based
CHAPTER 7 THE DEHYDRATION AND SWEETENING OF NATURAL GAS Natural gases either from natural production or storage reservoirs contain water, which condense and form solid gas hydrates to block pipeline flow
Production of Hydrogen RJ Allam Air Products Why Hydrogen? H 2 + ½ O 2 H 2 O H -57.8 kcal/mole H 2 is an energy vector, is converted to water which has minimal environmental impact. H 2 is a non-polluting
TECHNICAL INFORMATION ABOUT NATURAL GAS CLEANING AND TREATMENT I / 13 1 Natural Gas Cleaning and Treatment EDL and DBI are able to offer the basic and detail engineering including selection of technology
UOP Selexol TM Technology for Acid Gas Removal 2009 UOP LLC. All rights reserved. UOP 5241F-01 Main Points of Presentation Overview of the Selexol process Natural gas applications Syngas applications Selexol
Biogas upgrading technologies Swedish Gas Centre IEA Bioenergy Task 37 Energy from biogas and landfill gas Anaerobic digestion 1000 800 kg 600 400 H2O CH4 CO2 VS Ash 200 0 Before AD After AD Biogas cleaning
PRISM Membrane Systems For Oil Refinery Applications Air Products PRISM Membrane Systems are found in many steps of the oil refining process. From refinery off-gas streams to the purge-gas recycle, PRISM
PETROCHEMICALS C. R. Deddis BP Exploration Operating Company Ltd., UK Keywords: Petrochemicals, hydrocarbons, natural gas, cracking, olefins, aromatics, polymers, fibers. Contents 1. Introduction 2. Petrochemicals
Syngas Purification Units From Gasification to Chemicals www.airliquide.com Global experience Since the integration of Lurgi, a pioneer in gasification technologies, Air Liquide has widely expanded its
12.1 How do sub-atomic particles help us to understand the structure of substances? Simple particle theory is developed in this unit to include atomic structure and bonding. The arrangement of electrons
LNG Dehydration(Drying of Natural Gas) Absorption and refrigeration with hydrate inhibition is the most common dehydration process used to meet pipeline sales specifications. TEG is most common in absorption
Organic Chemistry Questions 1 Molecules of 1-propanol and 2-propanol have different (1) percentage compositions (2) molecular masses (3) molecular formulas (4) structural formulas 2 Which compound is an
Balancing chemical reaction equations (stoichiometry) This worksheet and all related files are licensed under the Creative Commons Attribution License, version 1.0. To view a copy of this license, visit
Crude Oil & Natural Gas Properties Crude Oil Refinement General appearance of crude oil Chemical Composition of crude oil Origin of Oil -Physical Properties of Crude Oil - Relations between physical properties
CATALYTIC SCIENCE SERIES VOL. 10 Series Editor: Graham J. Hutchings Concepts in Syngas Manufacture Jens Rostrup-Nielsen Lars J. Christiansen Haldor Topsoe A/S, Denmark Imperial College Press Contents Preface
CHAPTER 10: INTERMOLECULAR FORCES: THE UNIQUENESS OF WATER Problems: 10.2, 10.6,10.15-10.33, 10.35-10.40, 10.56-10.60, 10.101-10.102 10.1 INTERACTIONS BETWEEN IONS Ion-ion Interactions and Lattice Energy
CHAPTER 10 REVIEW States of Matter SECTION 1 SHORT ANSWER Answer the following questions in the space provided. 1. Identify whether the descriptions below describe an ideal gas or a real gas. ideal gas
The Next Generation of Activated Carbon Adsorbents for the Pre- Combustion Capture of Carbon Dioxide. Power Plant Modelling Workshop at University of Warwick Dr. Joe Wood,Prof. Jihong Wang, Simon Caldwell,
1 Refining 101 Dennis Sutton March 2012 The Petroleum Industry Exploration The Petroleum Industry Exploration Production & Supply The Petroleum Industry Exploration Production & Supply REFINING The Petroleum
Ammonia: The Key to a Hydrogen Economy Ammonia Fuel Cell Systems Jason C. Ganley Howard University Department of Chemical Engineering Washington, DC 1 Presentation Outline Introduction to Fuel Cells Characteristics
Physical & Chemical Properties Properties Carbon black can be broadly defined as very fine particulate aggregates of carbon possessing an amorphous quasi-graphitic molecular structure. The most significant
CHAPTER 3 PROPERTIES OF NATURAL GASES The behavior of natural gas, whether pure methane or a mixture of volatile hydrocarbons and the nonhydrocarbons nitrogen, carbon dioxide, and hydrogen sulfide, must
Process Technology Advanced bioethanol production and renewable energy generation from ligno-cellulosic materials, biomass waste and residues The INEOS Bio process technology produces carbon-neutral bioethanol
1. A gas absorbs 0.0 J of heat and then performs 15.2 J of work. The change in internal energy of the gas is a) 24.8 J b) 14.8 J c) 55.2 J d) 15.2 J ANS: d) 15.2 J PAGE: 6.1 2. Calculate the work for the
Chapter 2 Chemical and Physical Properties of Sulphur Dioxide and Sulphur Trioxide 2.1 Introduction In order to appreciate the impact of the properties of liquid sulphur dioxide and liquid sulphur trioxide
IBP 2778_10 HIGH EFFICIENCY ON CO2 REMOVAL IN NATURAL GAS WITH UCARSOL SOLVENTS Thiago V. Alonso 1 Copyright 2010, Brazilian Petroleum, Gas and Biofuels Institute - IBP This Technical Paper was prepared
C1 Crude Oil Quiz 1. What is combustion? A reaction between oxygen and a fuel that releases energy. 2. Which pollutant gases are produced during the combustion of fossil fuels? Particulates, carbon dioxide,
1. The average kinetic energy of water molecules increases when 1) H 2 O(s) changes to H 2 O( ) at 0ºC 3) H 2 O( ) at 10ºC changes to H 2 O( ) at 20ºC 2) H 2 O( ) changes to H 2 O(s) at 0ºC 4) H 2 O( )
INTRODUCTORY CHEMISTRY Concepts and Critical Thinking Sixth Edition by Charles H. Corwin Chapter 13 Liquids and Solids by Christopher Hamaker 1 Chapter 13 Properties of Liquids Unlike gases, liquids do
AALTO UNIVERSITY SCHOOL OF CHEMICAL TECHNOLOGY KE-40.4120 Introduction to biorefineries and biofuels Assignment 8: Comparison of gasification, pyrolysis and combustion Aino Siirala 309141 Assignment submitted
Carbon Black Industry Technology Properties Applications Carbon Black The first commercial nano-material An allotrope of carbon, mainly differing from graphite and so-called amorphous carbon by its physical
Lecture 7 Gaseous emission control by adsorption GASEOUS EMISSION CONTROL BY ABSORPTION AND ADSORPTION INTRODUCTION Combustion processes generate various primary and secondary air pollutants such as carbon
Wet Scrubbers for Gasifier Gas Cleaning Paper # 49 Andrew C. Bartocci Envitech, Inc. 2924 Emerson Street- Suite 320 San Diego, CA 92106 Ph: 619-223-9925, ext. 203 ABSTRACT Concern for global climate change
THE WAY TO SOMEWHERE Sub-topics 1 Diffusion Diffusion processes in industry RATE PROCESSES IN SOLIDS At any temperature different from absolute zero all atoms, irrespective of their state of aggregation
Coal Gasification: The Technology and Its Viability as a Future Energy Source Edward S. Rubin Department of Engineering and Public Policy Carnegie Mellon University Pittsburgh, Pennsylvania Presentation
Properties and uses of substances Periodic table and properties and uses of elements relative to their positions. SCN 3-15a Explore groups 1, 7 and 0 and their organisation in the periodic table. Atomic
Automotive Base Oil Presentation What is a Base Oil? The refined petroleum mineral or synthetic material that is produced by a refinery to a required set of specifications. A lubricant s quality can depend
May 1997 REFERENCE DATA SHEET ON AIR POLLUTION CONTROL DEVICES By: Gary M. Hutter, Ph.D With the passage of the 1971 Clean Air Act, American industry experienced a significantly increased need to reduce
Located in the Energy Center at Discovery Park, Purdue University Coal-To-Gas & Coal-To-Liquids CCTR Basic Facts File #3 Brian H. Bowen, Marty W. Irwin The Energy Center at Discovery Park Purdue University
Assessment Chapter Test A Chapter: States of Matter In the space provided, write the letter of the term or phrase that best completes each statement or best answers each question. 1. The kinetic-molecular
Centre No. Candidate No. Surname Signature Initial(s) Paper Reference(s) 4335/2H London Examinations IGCSE Chemistry Paper 2H Higher Tier Monday 9 May 2005 Morning Time: 2 hours Examiner s use only Team
EXAMPLE EXERCISE 4.1 Change of Physical State State the term that applies to each of the following changes of physical state: (a) Snow changes from a solid to a liquid. (b) Gasoline changes from a liquid
Stoichiometric Analysis of Gasification Lecture-G-L6-2x Marek Ściążko, Prof. Copyright-MS-2013 1 Introduction Gasification is a process in which a carbon containing feedstock is thermochemically converted
SEPURAN Green Membrane technology for upgrading biogas efficiently Gas separation with SEPURAN Evonik, the creative industrial group from Germany, is one of the world leaders in specialty chemicals. As
MERCURY REMOVAL FROM NATURAL GAS AND LIQUID STREAMS Giacomo Corvini, Julie Stiltner and Keith Clark UOP LLC Houston, Texas, USA n ABSTRACT Mercury is often present in natural gas, petrochemical and some
Andreas Thon (Autor) Operation of a System of Interconnected Fluidized Bed Reactors in the Chemical Looping Combustion Process https://cuvillier.de/de/shop/publications/6652 Copyright: Cuvillier Verlag,
Chemistry Entrance Examination Topics 1. General characteristics of the group 6 elements of the main subgroups on the basis of the position in the Periodic table and of atomic structure. Sulfuric acid,
Product Information DOWEX Resins as Organic Solvent Desiccants DOWEX* ion exchange resins can be used as desiccants for organic solvents, after having been dried to a low moisture level, in a manner similar
DP Chemistry Review Topic 1: Quantitative chemistry 1.1 The mole concept and Avogadro s constant Assessment statement Apply the mole concept to substances. Determine the number of particles and the amount
Exam 2 CHEM 1100 Version #1 Student: 1. The heat energy released or absorbed by a chemical reaction is generally determined by the difference between the energy that A. must be put in to break the bonds
1. Which is the structural formula of methane? 6. Which hydrocarbon is a member of the alkane series? 7. How many carbon atoms are contained in an ethyl group? 1 3 2 4 2. In the alkane series, each molecule
Lecture 8 Biomass gasification methods Thermochemical conversion method Principle Gasifiers Operationtypes-Applications The thermo-chemical decomposition of hydrocarbons from biomass in a reducing (oxygen
Coal Gasification Development for IGFC (EAGLE Project) Sadao Wasaka Energy and Environment Technology Development Department New Energy And Industrial Technology Development Organization Tokyo, Japan Masao
1. What Is Gasification Gasification is a reactive process, which use the organic matter (biomass) energy or fossil energy (coal, peat) and convert them into hydrogen, carbon monoxide, methane, other hydrocarbons
Gasifier Feedstock Hydrokinetics A SUNY Cobleskill Initiative Douglas Goodale, Ph.D., SUNY Cobleskill, Cobleskill, NY David Waage P.E., SUNY Cobleskill, Cobleskill, NY Contract funded through: - US Department
Chapter 13 - LIQUIDS AND SOLIDS Problems to try at end of chapter: Answers in Appendix I: 1,3,5,7b,9b,15,17,23,25,29,31,33,45,49,51,53,61 13.1 Properties of Liquids 1. Liquids take the shape of their container,
Click here to return to Contents page Integration of biomass gasification in a gas-engine cogeneration system F Pratola, M L Pellizza, F Repetto, E Maggio, C Amorino INTEGRATION OF BIOMASS GASIFICATION
COKE PRODUCTION FOR BLAST FURNACE IRONMAKING By Hardarshan S. Valia, Scientist, Ispat Inland Inc INTRODUCTION A world class blast furnace operation demands the highest quality of raw materials, operation,
Abstract Ecological Aspects of Oil Shale Processing Y. Zhirjakov, Institute of Oil Shale Research Tallinn Technical University Tallinn, Estonia 26 th Oil Shale Symposium Oil shale belongs to lean and environmentally
Experiment 1: Thin Layer Part A: understanding R f Part B: R f & solvent polarity Part C: R f & compound functionality Part D: identification of commercial food dye components Reading: MHS Ch. 17 pgs 219-235
NATURAL GAS PROCESSING H. K. Abdel-Aal National Research Center (NRC), Cairo, Egypt Keywords: sour natural gas, gas sweetening, gas dehydration, amines, glycols, hydrates, hydrogen sulfide, NGL, cryogenic
ECONOMICAL OPTION FOR CO 2 / METHANE SEPARATION IN PRODUCED GAS CONTAINING A HIGH CO 2 FRACTION F. Patrick Ross, P.E. TPR Consulting 9907 Sagecourt Drive Houston, Texas 77089 (713) 870-9208 firstname.lastname@example.org
Overview The standards for chemistry establish scientific inquiry skills and core content for all chemistry courses in DoDEA schools. In chemistry, students acquire a fundamental knowledge of the substances
Coal Gasification Based DRI Solution for Indian Ironmaking By: Rob Cheeley, Sales Manager Markus Leu, Plant Sales Manager Midrex Technologies, Inc. Introduction As one of the world s most vibrant and growing
Intermolecular forces are electromagnetic forces that hold like molecules together. Strong intermolecular forces result in a high melting point and a solid state at room temperature. Molecules that are
5s Solubility & Conductivity OBJECTIVES To explore the relationship between the structures of common household substances and the kinds of solvents in which they dissolve. To demonstrate the ionic nature
Adsorption Technologies: our work our life our passion. Molecular Sieve Adsorbents Zeochem Molecular Sieve Adsorbents Zeochem, a manufacturer of high quality molecular sieves and chromatography gels, was
10.3155/2008CP175.91 Testing of Ammonia Based CO 2 Capture with Multi- Pollutant Control Technology Paper # 91 Christopher R. McLarnon, Ph.D. Powerspan Corp., 100 International Drive, Suite 200, Portsmouth,
UNFCCC Technical workshop on modalities and procedures for carbon dioxide capture and storage in geological formations as clean development mechanism project activity CO2 Capture Technologies 7 8 September,
Experiment 3 Separation by Solvent Extraction Objectives To separate a mixture consisting of a carboxylic acid and a neutral compound by using solvent extraction techniques. Introduction Frequently, organic
Biomass Gasification Biomass gasification, or producing gas from biomass, involves burning biomass under restricted air supply for the generation of producer gas. Producer gas is a mixture of gases: 18%
Simulation of a base case for future IGCC concepts with CO 2 capture Christian Kunze, Hartmut Spliethoff Institute for Energy Systems TU München for 4 th Clean Coal Technology Conference 2009 18 20 May,
Lecture 1: Kinetics vs. Thermodynamics: different but related Today s topics The basic concepts of Kinetics and Thermodynamics, and how to understand the difference and inter-relationship between the two
Chapter 2 The Chemical Context of Life Multiple-Choice Questions 1) About 25 of the 92 natural elements are known to be essential to life. Which four of these 25 elements make up approximately 96% of living
For Industrial Heating Equipment and Boilers Prepared for California Energy Commission (CEC) Prepared By: Southern California Gas Company (A Sempra Energy Utility) E3M Inc. May 2012 i Disclaimer The CEC
ASimple Guide to Oil Refining We all know that motor oil and gasoline come from crude oil. What many people do not realize is that crude oil is also the starting point for many diverse products such as
Synthesis Gas Purification in Gasification to Ammonia/Urea Plants GASIFICATION TECHNOLOGIES CONFERENCE October 4-6, 2004 Washington D.C Dave Heaven, John Mak Fluor Enterprises, Inc., Aliso Viejo, California,
8.10 Standard Heats of Formation We cannot have a table for the H values for every reaction there is, because there are too many of them. However, as we saw with Hess s Law, we can express any reaction
Name: Sunday, October 14, 2007 Test 1: Introduction to Chemistry 1. Two substances, A and Z, are to be identified. Substance A can not be broken down by a chemical change. Substance Z can be broken down
CHAPTER 4: MATTER & ENERGY Problems: 1,3,5,7,13,17,19,21,23,25,27,29,31,33,37,41,43,45,47,49,51,53,55,57,59,63,65,67,69,77,79,81,83 4.1 Physical States of Matter Matter: Anything that has mass and occupies
tec Energy Technology Projects Subject: Bergius 1: 1924 1945 Rev: April 2006 Fact Sheet Technology The information included in this document is property of. Use and reproduction of this document, without
Executive Summary This project was divided into two parts. One part evaluated possible catalysts for producing higher-alcohols (C 2 to C 5+ ) as fuel additives. The other part provided guidance by looking